#------------------------------------------------------------------------------
#$Date: 2017-03-02 19:20:33 +0200 (Thu, 02 Mar 2017) $
#$Revision: 192782 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/31/09/4310949.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4310949
loop_
_publ_author_name
'Jens Niermann'
'Wolfgang Jeitschko'
_publ_contact_author
;
         Jeitschko, Wolfgang
         Institut füer Anorganische und Analytische Chemie
         Universität Münster
         Wilhelm-Klemm-Strasse 8
         48149 Münster
         Bundesrepublik Deutschland
;
_publ_contact_author_email       jeitsch@uni-muenster.de
_publ_contact_author_fax         '049 251 833-3136'
_publ_contact_author_phone       '049 251 833-3120'
_publ_section_title
;
 Ternary Rare Earth Osmium Aluminides R7+xOs12Al61+y Belonging to a
 Structural Family with Layered Topology
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3264
_journal_page_last               3270
_journal_paper_doi               10.1021/ic0303035
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'Al61.51 Os12 Y7.86'
_chemical_formula_weight         4640.77
_chemical_name_systematic        Y7+xOs12Al61+y
_space_group_IT_number           193
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   13.015(2)
_cell_length_b                   13.015(2)
_cell_length_c                   9.030(2)
_cell_measurement_temperature    293(2)
_cell_volume                     1324.7(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.837
_diffrn_measured_fraction_theta_max 0.837
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2188
_diffrn_reflns_av_sigmaI/netI    0.0915
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            11538
_diffrn_reflns_theta_full        34.96
_diffrn_reflns_theta_max         34.96
_diffrn_reflns_theta_min         3.13
_exptl_absorpt_coefficient_mu    38.174
_exptl_crystal_density_diffrn    5.817
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2018
_refine_diff_density_max         12.004
_refine_diff_density_min         -8.516
_refine_diff_density_rms         1.036
_refine_ls_extinction_coef       0.000062(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.103
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     46
_refine_ls_number_reflns         914
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.103
_refine_ls_R_factor_all          0.1166
_refine_ls_R_factor_gt           0.0354
_refine_ls_shift/su_max          0.247
_refine_ls_shift/su_mean         0.058
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0547P)²+340.6468P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1268
_refine_ls_wR_factor_ref         0.1460
_reflns_number_gt                410
_reflns_number_total             914
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0303035_1.cif
_cod_data_source_block           193
_cod_depositor_comments
;
The following automatic conversions were performed:
data name '_publ_contact_autor' replaced with '_publ_contact_author'
as specified in the replacement file
'/home/antanas/src/cod-tools/trunk/data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 4998 2017-03-02 13:24:31Z antanas 
;
_cod_database_code               4310949
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Y1 Y 0.39189(4) 0.0000 0.2500 0.00840(9) Uani 1 4 d S . .
Y2 Y 0.0000 0.0000 0.2159(5) 0.008 Uiso 0.0988(16) 6 d SP . .
Y3 Y 0.0000 0.0000 0.2500 0.008 Uiso 0.738(2) 12 d SP . .
Os1 Os 0.202777(5) 0.405554(10) 0.0000 0.00579(2) Uani 1 2 d S . .
Al1 Al 0.20038(9) 0.0000 0.02840(13) 0.0131(3) Uani 1 2 d S . .
Al2 Al 0.61569(8) 0.0000 0.10392(12) 0.0102(2) Uani 1 2 d S . .
Al3 Al 0.16502(8) 0.28447(8) 0.2500 0.0074(3) Uani 1 2 d S . .
Al4 Al 0.27049(12) 0.52485(8) 0.2500 0.0124(3) Uani 1 2 d S . .
Al5 Al 0.59036(4) 0.18072(8) 0.0000 0.00358(15) Uani 1 2 d S . .
Al6 Al 0.0000 0.0000 0.0910(16) 0.009 Uiso 0.118(5) 6 d SP . .
Al7 Al 0.0000 0.0000 0.0000 0.009 Uiso 0.611(8) 12 d SP . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Os Os -1.2165 7.6030 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Al4 Y1 Al4 178.88(5) 7 3 ?
Al4 Y1 Al3 126.40(3) 7 3 ?
Al4 Y1 Al3 52.48(3) 3 3 ?
Al4 Y1 Al3 52.48(3) 7 7 ?
Al4 Y1 Al3 126.40(3) 3 7 ?
Al3 Y1 Al3 73.92(3) 3 7 ?
Al4 Y1 Al1 89.56(2) 7 16_556 ?
Al4 Y1 Al1 89.56(2) 3 16_556 ?
Al3 Y1 Al1 51.459(18) 3 16_556 ?
Al3 Y1 Al1 51.459(18) 7 16_556 ?
Al4 Y1 Al1 89.56(2) 7 . ?
Al4 Y1 Al1 89.56(2) 3 . ?
Al3 Y1 Al1 51.459(18) 3 . ?
Al3 Y1 Al1 51.458(18) 7 . ?
Al1 Y1 Al1 77.52(5) 16_556 . ?
Al4 Y1 Al2 89.983(1) 7 13_655 ?
Al4 Y1 Al2 89.983(1) 3 13_655 ?
Al3 Y1 Al2 88.589(17) 3 13_655 ?
Al3 Y1 Al2 88.589(17) 7 13_655 ?
Al1 Y1 Al2 126.99(3) 16_556 13_655 ?
Al1 Y1 Al2 49.47(3) . 13_655 ?
Al4 Y1 Al2 89.983(1) 7 4_655 ?
Al4 Y1 Al2 89.983(1) 3 4_655 ?
Al3 Y1 Al2 88.589(17) 3 4_655 ?
Al3 Y1 Al2 88.589(17) 7 4_655 ?
Al1 Y1 Al2 49.47(3) 16_556 4_655 ?
Al1 Y1 Al2 126.99(3) . 4_655 ?
Al2 Y1 Al2 176.47(4) 13_655 4_655 ?
Al4 Y1 Al2 90.51(2) 7 16_556 ?
Al4 Y1 Al2 90.51(2) 3 16_556 ?
Al3 Y1 Al2 136.708(15) 3 16_556 ?
Al3 Y1 Al2 136.709(15) 7 16_556 ?
Al1 Y1 Al2 116.88(3) 16_556 16_556 ?
Al1 Y1 Al2 165.60(3) . 16_556 ?
Al2 Y1 Al2 116.13(3) 13_655 16_556 ?
Al2 Y1 Al2 67.40(3) 4_655 16_556 ?
Al4 Y1 Al2 90.51(2) 7 . ?
Al4 Y1 Al2 90.51(2) 3 . ?
Al3 Y1 Al2 136.709(15) 3 . ?
Al3 Y1 Al2 136.710(15) 7 . ?
Al1 Y1 Al2 165.60(3) 16_556 . ?
Al1 Y1 Al2 116.88(3) . . ?
Al2 Y1 Al2 67.40(3) 13_655 . ?
Al2 Y1 Al2 116.13(3) 4_655 . ?
Al2 Y1 Al2 48.73(4) 16_556 . ?
Al4 Y1 Al5 52.857(19) 7 . ?
Al4 Y1 Al5 127.73(2) 3 . ?
Al3 Y1 Al5 134.519(12) 3 . ?
Al3 Y1 Al5 88.286(14) 7 . ?
Al1 Y1 Al5 138.535(16) 16_556 . ?
Al1 Y1 Al5 84.59(2) . . ?
Al2 Y1 Al5 48.659(16) 13_655 . ?
Al2 Y1 Al5 133.348(17) 4_655 . ?
Al2 Y1 Al5 83.99(2) 16_556 . ?
Al2 Y1 Al5 48.656(15) . . ?
Al4 Y1 Al5 52.857(19) 7 16_556 ?
Al4 Y1 Al5 127.73(2) 3 16_556 ?
Al3 Y1 Al5 134.519(12) 3 16_556 ?
Al3 Y1 Al5 88.285(14) 7 16_556 ?
Al1 Y1 Al5 84.59(2) 16_556 16_556 ?
Al1 Y1 Al5 138.534(16) . 16_556 ?
Al2 Y1 Al5 133.348(17) 13_655 16_556 ?
Al2 Y1 Al5 48.659(16) 4_655 16_556 ?
Al2 Y1 Al5 48.656(15) 16_556 16_556 ?
Al2 Y1 Al5 83.99(2) . 16_556 ?
Al5 Y1 Al5 84.72(2) . 16_556 ?
Al4 Y1 Al5 127.73(2) 7 13_655 ?
Al4 Y1 Al5 52.856(19) 3 13_655 ?
Al3 Y1 Al5 88.282(14) 3 13_655 ?
Al3 Y1 Al5 134.516(12) 7 13_655 ?
Al1 Y1 Al5 138.532(17) 16_556 13_655 ?
Al1 Y1 Al5 84.59(2) . 13_655 ?
Al2 Y1 Al5 48.658(16) 13_655 13_655 ?
Al2 Y1 Al5 133.349(17) 4_655 13_655 ?
Al2 Y1 Al5 84.00(2) 16_556 13_655 ?
Al2 Y1 Al5 48.659(15) . 13_655 ?
Al5 Y1 Al5 74.88(3) . 13_655 ?
Al5 Y1 Al5 130.332(18) 16_556 13_655 ?
Al4 Y1 Al5 127.73(2) 7 4_655 ?
Al4 Y1 Al5 52.856(19) 3 4_655 ?
Al3 Y1 Al5 88.282(14) 3 4_655 ?
Al3 Y1 Al5 134.516(12) 7 4_655 ?
Al1 Y1 Al5 84.59(2) 16_556 4_655 ?
Al1 Y1 Al5 138.532(16) . 4_655 ?
Al2 Y1 Al5 133.349(17) 13_655 4_655 ?
Al2 Y1 Al5 48.658(16) 4_655 4_655 ?
Al2 Y1 Al5 48.659(15) 16_556 4_655 ?
Al2 Y1 Al5 84.00(2) . 4_655 ?
Al5 Y1 Al5 130.332(18) . 4_655 ?
Al5 Y1 Al5 74.88(3) 16_556 4_655 ?
Al5 Y1 Al5 84.72(2) 13_655 4_655 ?
Al4 Y1 Os1 47.653(13) 7 5 ?
Al4 Y1 Os1 131.843(15) 3 5 ?
Al3 Y1 Os1 97.789(15) 3 5 ?
Al3 Y1 Os1 47.883(10) 7 5 ?
Al1 Y1 Os1 47.495(11) 16_556 5 ?
Al1 Y1 Os1 98.83(2) . 5 ?
Al2 Y1 Os1 130.656(14) 13_655 5 ?
Al2 Y1 Os1 47.766(11) 4_655 5 ?
Al2 Y1 Os1 91.826(18) 16_556 5 ?
Al2 Y1 Os1 125.324(15) . 5 ?
Al5 Y1 Os1 100.327(17) . 5 ?
Al5 Y1 Os1 44.514(8) 16_556 5 ?
Al5 Y1 Os1 173.912(16) 13_655 5 ?
Al5 Y1 Os1 95.855(18) 4_655 5 ?
Al4 Y1 Os1 47.653(13) 7 14 ?
Al4 Y1 Os1 131.843(15) 3 14 ?
Al3 Y1 Os1 97.789(15) 3 14 ?
Al3 Y1 Os1 47.883(10) 7 14 ?
Al1 Y1 Os1 98.83(2) 16_556 14 ?
Al1 Y1 Os1 47.495(11) . 14 ?
Al2 Y1 Os1 47.766(11) 13_655 14 ?
Al2 Y1 Os1 130.656(14) 4_655 14 ?
Al2 Y1 Os1 125.324(15) 16_556 14 ?
Al2 Y1 Os1 91.826(18) . 14 ?
Al5 Y1 Os1 44.515(8) . 14 ?
Al5 Y1 Os1 100.326(17) 16_556 14 ?
Al5 Y1 Os1 95.855(18) 13_655 14 ?
Al5 Y1 Os1 173.912(16) 4_655 14 ?
Os1 Y1 Os1 82.929(16) 5 14 ?
Al4 Y1 Os1 131.842(15) 7 3 ?
Al4 Y1 Os1 47.654(13) 3 3 ?
Al3 Y1 Os1 47.882(10) 3 3 ?
Al3 Y1 Os1 97.787(15) 7 3 ?
Al1 Y1 Os1 98.83(2) 16_556 3 ?
Al1 Y1 Os1 47.493(11) . 3 ?
Al2 Y1 Os1 47.766(11) 13_655 3 ?
Al2 Y1 Os1 130.656(14) 4_655 3 ?
Al2 Y1 Os1 125.325(15) 16_556 3 ?
Al2 Y1 Os1 91.828(17) . 3 ?
Al5 Y1 Os1 95.856(18) . 3 ?
Al5 Y1 Os1 173.911(16) 16_556 3 ?
Al5 Y1 Os1 44.513(8) 13_655 3 ?
Al5 Y1 Os1 100.326(17) 4_655 3 ?
Os1 Y1 Os1 140.871(16) 5 3 ?
Os1 Y1 Os1 84.193(13) 14 3 ?
Al4 Y1 Os1 131.842(15) 7 18_556 ?
Al4 Y1 Os1 47.654(13) 3 18_556 ?
Al3 Y1 Os1 47.882(10) 3 18_556 ?
Al3 Y1 Os1 97.787(15) 7 18_556 ?
Al1 Y1 Os1 47.493(11) 16_556 18_556 ?
Al1 Y1 Os1 98.82(2) . 18_556 ?
Al2 Y1 Os1 130.656(14) 13_655 18_556 ?
Al2 Y1 Os1 47.766(11) 4_655 18_556 ?
Al2 Y1 Os1 91.827(17) 16_556 18_556 ?
Al2 Y1 Os1 125.325(15) . 18_556 ?
Al5 Y1 Os1 173.911(16) . 18_556 ?
Al5 Y1 Os1 95.856(18) 16_556 18_556 ?
Al5 Y1 Os1 100.326(17) 13_655 18_556 ?
Al5 Y1 Os1 44.513(8) 4_655 18_556 ?
Os1 Y1 Os1 84.193(13) 5 18_556 ?
Os1 Y1 Os1 140.871(16) 14 18_556 ?
Os1 Y1 Os1 82.929(16) 3 18_556 ?
Al4 Y1 Al4 44.25(4) 7 9_655 ?
Al4 Y1 Al4 136.866(17) 3 9_655 ?
Al3 Y1 Al4 170.65(2) 3 9_655 ?
Al3 Y1 Al4 96.73(2) 7 9_655 ?
Al1 Y1 Al4 122.592(16) 16_556 9_655 ?
Al1 Y1 Al4 122.592(16) . 9_655 ?
Al2 Y1 Al4 91.220(14) 13_655 9_655 ?
Al2 Y1 Al4 91.220(14) 4_655 9_655 ?
Al2 Y1 Al4 51.005(17) 16_556 9_655 ?
Al2 Y1 Al4 51.004(16) . 9_655 ?
Al5 Y1 Al4 43.138(11) . 9_655 ?
Al5 Y1 Al4 43.138(11) 16_556 9_655 ?
Al5 Y1 Al4 98.597(18) 13_655 9_655 ?
Al5 Y1 Al4 98.597(18) 4_655 9_655 ?
Os1 Y1 Al4 75.320(12) 5 9_655 ?
Os1 Y1 Al4 75.320(12) 14 9_655 ?
Os1 Y1 Al4 135.730(11) 3 9_655 ?
Os1 Y1 Al4 135.730(11) 18_556 9_655 ?
Al4 Y1 Al4 136.866(17) 7 2_655 ?
Al4 Y1 Al4 44.25(4) 3 2_655 ?
Al3 Y1 Al4 96.73(2) 3 2_655 ?
Al3 Y1 Al4 170.65(2) 7 2_655 ?
Al1 Y1 Al4 122.592(16) 16_556 2_655 ?
Al1 Y1 Al4 122.592(16) . 2_655 ?
Al2 Y1 Al4 91.220(14) 13_655 2_655 ?
Al2 Y1 Al4 91.220(14) 4_655 2_655 ?
Al2 Y1 Al4 51.005(16) 16_556 2_655 ?
Al2 Y1 Al4 51.004(17) . 2_655 ?
Al5 Y1 Al4 98.594(18) . 2_655 ?
Al5 Y1 Al4 98.595(18) 16_556 2_655 ?
Al5 Y1 Al4 43.140(11) 13_655 2_655 ?
Al5 Y1 Al4 43.140(11) 4_655 2_655 ?
Os1 Y1 Al4 135.729(11) 5 2_655 ?
Os1 Y1 Al4 135.729(11) 14 2_655 ?
Os1 Y1 Al4 75.321(12) 3 2_655 ?
Os1 Y1 Al4 75.321(12) 18_556 2_655 ?
Al4 Y1 Al4 92.62(3) 9_655 2_655 ?
Al4 Y1 Al1 115.92(3) 7 14 ?
Al4 Y1 Al1 63.15(3) 3 14 ?
Al3 Y1 Al1 30.230(14) 3 14 ?
Al3 Y1 Al1 70.752(19) 7 14 ?
Al1 Y1 Al1 74.17(2) 16_556 14 ?
Al1 Y1 Al1 26.863(17) . 14 ?
Al2 Y1 Al1 58.84(2) 13_655 14 ?
Al2 Y1 Al1 118.12(2) 4_655 14 ?
Al2 Y1 Al1 152.184(15) 16_556 14 ?
Al2 Y1 Al1 118.45(2) . 14 ?
Al5 Y1 Al1 104.513(19) . 14 ?
Al5 Y1 Al1 156.510(17) 16_556 14 ?
Al5 Y1 Al1 73.158(15) 13_655 14 ?
Al5 Y1 Al1 112.136(19) 4_655 14 ?
Os1 Y1 Al1 112.042(18) 5 14 ?
Os1 Y1 Al1 73.756(16) 14 14 ?
Os1 Y1 Al1 28.892(13) 3 14 ?
Os1 Y1 Al1 77.261(19) 18_556 14 ?
Al4 Y1 Al1 146.853(15) 9_655 14 ?
Al4 Y1 Al1 101.225(19) 2_655 14 ?
Al4 Y1 Al1 63.15(3) 7 6 ?
Al4 Y1 Al1 115.92(3) 3 6 ?
Al3 Y1 Al1 70.753(19) 3 6 ?
Al3 Y1 Al1 30.229(14) 7 6 ?
Al1 Y1 Al1 26.863(17) 16_556 6 ?
Al1 Y1 Al1 74.17(2) . 6 ?
Al2 Y1 Al1 118.12(2) 13_655 6 ?
Al2 Y1 Al1 58.84(2) 4_655 6 ?
Al2 Y1 Al1 118.45(2) 16_556 6 ?
Al2 Y1 Al1 152.184(15) . 6 ?
Al5 Y1 Al1 112.138(19) . 6 ?
Al5 Y1 Al1 73.160(16) 16_556 6 ?
Al5 Y1 Al1 156.507(17) 13_655 6 ?
Al5 Y1 Al1 104.511(19) 4_655 6 ?
Os1 Y1 Al1 28.894(13) 5 6 ?
Os1 Y1 Al1 77.261(19) 14 6 ?
Os1 Y1 Al1 112.041(18) 3 6 ?
Os1 Y1 Al1 73.755(16) 18_556 6 ?
Al4 Y1 Al1 101.225(19) 9_655 6 ?
Al4 Y1 Al1 146.853(15) 2_655 6 ?
Al1 Y1 Al1 83.35(3) 14 6 ?
Al4 Y1 Al1 115.92(3) 7 5 ?
Al4 Y1 Al1 63.15(3) 3 5 ?
Al3 Y1 Al1 30.230(14) 3 5 ?
Al3 Y1 Al1 70.752(19) 7 5 ?
Al1 Y1 Al1 26.863(17) 16_556 5 ?
Al1 Y1 Al1 74.17(2) . 5 ?
Al2 Y1 Al1 118.12(2) 13_655 5 ?
Al2 Y1 Al1 58.84(2) 4_655 5 ?
Al2 Y1 Al1 118.45(2) 16_556 5 ?
Al2 Y1 Al1 152.184(15) . 5 ?
Al5 Y1 Al1 156.510(17) . 5 ?
Al5 Y1 Al1 104.513(19) 16_556 5 ?
Al5 Y1 Al1 112.136(19) 13_655 5 ?
Al5 Y1 Al1 73.158(16) 4_655 5 ?
Os1 Y1 Al1 73.756(16) 5 5 ?
Os1 Y1 Al1 112.042(18) 14 5 ?
Os1 Y1 Al1 77.261(19) 3 5 ?
Os1 Y1 Al1 28.892(13) 18_556 5 ?
Al4 Y1 Al1 146.853(15) 9_655 5 ?
Al4 Y1 Al1 101.225(19) 2_655 5 ?
Al1 Y1 Al1 59.29(3) 14 5 ?
Al1 Y1 Al1 52.77(3) 6 5 ?
Al4 Y1 Al1 63.15(3) 7 15 ?
Al4 Y1 Al1 115.92(3) 3 15 ?
Al3 Y1 Al1 70.753(19) 3 15 ?
Al3 Y1 Al1 30.229(14) 7 15 ?
Al1 Y1 Al1 74.17(2) 16_556 15 ?
Al1 Y1 Al1 26.863(16) . 15 ?
Al2 Y1 Al1 58.84(2) 13_655 15 ?
Al2 Y1 Al1 118.12(2) 4_655 15 ?
Al2 Y1 Al1 152.184(15) 16_556 15 ?
Al2 Y1 Al1 118.45(2) . 15 ?
Al5 Y1 Al1 73.161(16) . 15 ?
Al5 Y1 Al1 112.138(19) 16_556 15 ?
Al5 Y1 Al1 104.511(19) 13_655 15 ?
Al5 Y1 Al1 156.507(17) 4_655 15 ?
Os1 Y1 Al1 77.261(19) 5 15 ?
Os1 Y1 Al1 28.894(13) 14 15 ?
Os1 Y1 Al1 73.755(16) 3 15 ?
Os1 Y1 Al1 112.041(18) 18_556 15 ?
Al4 Y1 Al1 101.225(19) 9_655 15 ?
Al4 Y1 Al1 146.853(15) 2_655 15 ?
Al1 Y1 Al1 52.77(3) 14 15 ?
Al1 Y1 Al1 59.29(3) 6 15 ?
Al1 Y1 Al1 83.35(3) 5 15 ?
Al4 Y1 Os1 117.13(2) 7 17_656 ?
Al4 Y1 Os1 63.84(2) 3 17_656 ?
Al3 Y1 Os1 110.523(13) 3 17_656 ?
Al3 Y1 Os1 152.867(7) 7 17_656 ?
Al1 Y1 Os1 109.15(2) 16_556 17_656 ?
Al1 Y1 Os1 151.965(7) . 17_656 ?
Al2 Y1 Os1 117.82(2) 13_655 17_656 ?
Al2 Y1 Os1 65.237(19) 4_655 17_656 ?
Al2 Y1 Os1 27.141(4) 16_556 17_656 ?
Al2 Y1 Os1 58.37(2) . 17_656 ?
Al5 Y1 Os1 104.188(14) . 17_656 ?
Al5 Y1 Os1 69.398(14) 16_556 17_656 ?
Al5 Y1 Os1 72.532(15) 13_655 17_656 ?
Al5 Y1 Os1 26.211(5) 4_655 17_656 ?
Os1 Y1 Os1 105.502(13) 5 17_656 ?
Os1 Y1 Os1 148.643(11) 14 17_656 ?
Os1 Y1 Os1 104.633(9) 3 17_656 ?
Os1 Y1 Os1 70.485(8) 18_556 17_656 ?
Al4 Y1 Os1 77.764(16) 9_655 17_656 ?
Al4 Y1 Os1 30.624(10) 2_655 17_656 ?
Al1 Y1 Os1 126.843(13) 14 17_656 ?
Al1 Y1 Os1 124.057(17) 6 17_656 ?
Al1 Y1 Os1 99.289(15) 5 17_656 ?
Al1 Y1 Os1 176.590(13) 15 17_656 ?
Al4 Y1 Os1 117.13(2) 7 2_655 ?
Al4 Y1 Os1 63.84(2) 3 2_655 ?
Al3 Y1 Os1 110.523(13) 3 2_655 ?
Al3 Y1 Os1 152.867(7) 7 2_655 ?
Al1 Y1 Os1 151.965(7) 16_556 2_655 ?
Al1 Y1 Os1 109.15(2) . 2_655 ?
Al2 Y1 Os1 65.237(19) 13_655 2_655 ?
Al2 Y1 Os1 117.82(2) 4_655 2_655 ?
Al2 Y1 Os1 58.37(2) 16_556 2_655 ?
Al2 Y1 Os1 27.141(4) . 2_655 ?
Al5 Y1 Os1 69.398(14) . 2_655 ?
Al5 Y1 Os1 104.189(14) 16_556 2_655 ?
Al5 Y1 Os1 26.211(5) 13_655 2_655 ?
Al5 Y1 Os1 72.532(15) 4_655 2_655 ?
Os1 Y1 Os1 148.643(11) 5 2_655 ?
Os1 Y1 Os1 105.502(13) 14 2_655 ?
Os1 Y1 Os1 70.485(8) 3 2_655 ?
Os1 Y1 Os1 104.633(9) 18_556 2_655 ?
Al4 Y1 Os1 77.764(16) 9_655 2_655 ?
Al4 Y1 Os1 30.624(10) 2_655 2_655 ?
Al1 Y1 Os1 99.289(15) 14 2_655 ?
Al1 Y1 Os1 176.590(13) 6 2_655 ?
Al1 Y1 Os1 126.843(13) 5 2_655 ?
Al1 Y1 Os1 124.057(17) 15 2_655 ?
Os1 Y1 Os1 52.591(13) 17_656 2_655 ?
Al4 Y1 Os1 63.84(2) 7 6_655 ?
Al4 Y1 Os1 117.13(2) 3 6_655 ?
Al3 Y1 Os1 152.867(7) 3 6_655 ?
Al3 Y1 Os1 110.525(13) 7 6_655 ?
Al1 Y1 Os1 109.15(2) 16_556 6_655 ?
Al1 Y1 Os1 151.966(7) . 6_655 ?
Al2 Y1 Os1 117.82(2) 13_655 6_655 ?
Al2 Y1 Os1 65.238(19) 4_655 6_655 ?
Al2 Y1 Os1 27.140(4) 16_556 6_655 ?
Al2 Y1 Os1 58.37(2) . 6_655 ?
Al5 Y1 Os1 72.530(15) . 6_655 ?
Al5 Y1 Os1 26.209(5) 16_556 6_655 ?
Al5 Y1 Os1 104.190(14) 13_655 6_655 ?
Al5 Y1 Os1 69.400(14) 4_655 6_655 ?
Os1 Y1 Os1 70.485(8) 5 6_655 ?
Os1 Y1 Os1 104.632(8) 14 6_655 ?
Os1 Y1 Os1 148.644(11) 3 6_655 ?
Os1 Y1 Os1 105.503(13) 18_556 6_655 ?
Al4 Y1 Os1 30.624(10) 9_655 6_655 ?
Al4 Y1 Os1 77.764(16) 2_655 6_655 ?
Al1 Y1 Os1 176.590(13) 14 6_655 ?
Al1 Y1 Os1 99.290(15) 6 6_655 ?
Al1 Y1 Os1 124.057(17) 5 6_655 ?
Al1 Y1 Os1 126.844(13) 15 6_655 ?
Os1 Y1 Os1 53.295(5) 17_656 6_655 ?
Os1 Y1 Os1 78.159(11) 2_655 6_655 ?
Al4 Y1 Os1 63.84(2) 7 15_655 ?
Al4 Y1 Os1 117.13(2) 3 15_655 ?
Al3 Y1 Os1 152.867(7) 3 15_655 ?
Al3 Y1 Os1 110.525(13) 7 15_655 ?
Al1 Y1 Os1 151.965(7) 16_556 15_655 ?
Al1 Y1 Os1 109.15(2) . 15_655 ?
Al2 Y1 Os1 65.238(19) 13_655 15_655 ?
Al2 Y1 Os1 117.82(2) 4_655 15_655 ?
Al2 Y1 Os1 58.37(2) 16_556 15_655 ?
Al2 Y1 Os1 27.140(4) . 15_655 ?
Al5 Y1 Os1 26.209(5) . 15_655 ?
Al5 Y1 Os1 72.530(15) 16_556 15_655 ?
Al5 Y1 Os1 69.400(14) 13_655 15_655 ?
Al5 Y1 Os1 104.190(14) 4_655 15_655 ?
Os1 Y1 Os1 104.632(9) 5 15_655 ?
Os1 Y1 Os1 70.485(8) 14 15_655 ?
Os1 Y1 Os1 105.503(13) 3 15_655 ?
Os1 Y1 Os1 148.644(11) 18_556 15_655 ?
Al4 Y1 Os1 30.624(10) 9_655 15_655 ?
Al4 Y1 Os1 77.764(16) 2_655 15_655 ?
Al1 Y1 Os1 124.057(17) 14 15_655 ?
Al1 Y1 Os1 126.844(13) 6 15_655 ?
Al1 Y1 Os1 176.590(13) 5 15_655 ?
Al1 Y1 Os1 99.290(15) 15 15_655 ?
Os1 Y1 Os1 78.159(10) 17_656 15_655 ?
Os1 Y1 Os1 53.295(5) 2_655 15_655 ?
Os1 Y1 Os1 52.590(13) 6_655 15_655 ?
Al4 Y1 Y3 89.44(3) 7 . ?
Al4 Y1 Y3 89.44(3) 3 . ?
Al3 Y1 Y3 36.962(15) 3 . ?
Al3 Y1 Y3 36.961(15) 7 . ?
Al1 Y1 Y3 38.76(2) 16_556 . ?
Al1 Y1 Y3 38.76(2) . . ?
Al2 Y1 Y3 88.23(2) 13_655 . ?
Al2 Y1 Y3 88.23(2) 4_655 . ?
Al2 Y1 Y3 155.64(2) 16_556 . ?
Al2 Y1 Y3 155.64(2) . . ?
Al5 Y1 Y3 114.835(9) . . ?
Al5 Y1 Y3 114.835(9) 16_556 . ?
Al5 Y1 Y3 114.833(9) 13_655 . ?
Al5 Y1 Y3 114.833(9) 4_655 . ?
Os1 Y1 Y3 70.436(8) 5 . ?
Os1 Y1 Y3 70.436(8) 14 . ?
Os1 Y1 Y3 70.435(8) 3 . ?
Os1 Y1 Y3 70.435(8) 18_556 . ?
Al4 Y1 Y3 133.692(17) 9_655 . ?
Al4 Y1 Y3 133.692(17) 2_655 . ?
Al1 Y1 Y3 41.675(14) 14 . ?
Al1 Y1 Y3 41.675(14) 6 . ?
Al1 Y1 Y3 41.675(14) 5 . ?
Al1 Y1 Y3 41.675(14) 15 . ?
Os1 Y1 Y3 140.920(5) 17_656 . ?
Os1 Y1 Y3 140.920(5) 2_655 . ?
Os1 Y1 Y3 140.921(5) 6_655 . ?
Os1 Y1 Y3 140.921(5) 15_655 . ?
Al4 Y1 Y2 89.44(3) 7 . ?
Al4 Y1 Y2 89.44(3) 3 . ?
Al3 Y1 Y2 37.100(16) 3 . ?
Al3 Y1 Y2 37.099(16) 7 . ?
Al1 Y1 Y2 42.22(5) 16_556 . ?
Al1 Y1 Y2 35.30(5) . . ?
Al2 Y1 Y2 84.78(5) 13_655 . ?
Al2 Y1 Y2 91.69(5) 4_655 . ?
Al2 Y1 Y2 159.09(5) 16_556 . ?
Al2 Y1 Y2 152.18(5) . . ?
Al5 Y1 Y2 112.25(4) . . ?
Al5 Y1 Y2 117.38(4) 16_556 . ?
Al5 Y1 Y2 112.25(4) 13_655 . ?
Al5 Y1 Y2 117.38(4) 4_655 . ?
Os1 Y1 Y2 72.88(3) 5 . ?
Os1 Y1 Y2 68.03(3) 14 . ?
Os1 Y1 Y2 68.03(3) 3 . ?
Os1 Y1 Y2 72.88(3) 18_556 . ?
Al4 Y1 Y2 133.592(17) 9_655 . ?
Al4 Y1 Y2 133.592(17) 2_655 . ?
Al1 Y1 Y2 39.16(4) 14 . ?
Al1 Y1 Y2 44.29(4) 6 . ?
Al1 Y1 Y2 44.29(4) 5 . ?
Al1 Y1 Y2 39.16(4) 15 . ?
Os1 Y1 Y2 143.28(3) 17_656 . ?
Os1 Y1 Y2 138.43(4) 2_655 . ?
Os1 Y1 Y2 143.28(3) 6_655 . ?
Os1 Y1 Y2 138.43(4) 15_655 . ?
Y3 Y1 Y2 3.46(5) . . ?
Y2 Y2 Al6 180.000(3) 16_556 . ?
Y2 Y2 Al6 0.000(1) 16_556 16_556 ?
Al6 Y2 Al6 180.000(1) . 16_556 ?
Y2 Y2 Al7 180.000(1) 16_556 . ?
Al6 Y2 Al7 0.0 . . ?
Al6 Y2 Al7 180.000(1) 16_556 . ?
Y2 Y2 Al7 0.000(1) 16_556 4 ?
Al6 Y2 Al7 180.0 . 4 ?
Al6 Y2 Al7 0.000(1) 16_556 4 ?
Al7 Y2 Al7 180.0 . 4 ?
Y2 Y2 Al6 180.000(2) 16_556 13 ?
Al6 Y2 Al6 0.0 . 13 ?
Al6 Y2 Al6 180.000(2) 16_556 13 ?
Al7 Y2 Al6 0.0 . 13 ?
Al7 Y2 Al6 180.000(1) 4 13 ?
Y2 Y2 Al1 122.99(7) 16_556 . ?
Al6 Y2 Al1 57.01(7) . . ?
Al6 Y2 Al1 122.99(7) 16_556 . ?
Al7 Y2 Al1 57.01(7) . . ?
Al7 Y2 Al1 122.99(7) 4 . ?
Al6 Y2 Al1 57.01(7) 13 . ?
Y2 Y2 Al1 122.99(7) 16_556 3 ?
Al6 Y2 Al1 57.01(7) . 3 ?
Al6 Y2 Al1 122.99(7) 16_556 3 ?
Al7 Y2 Al1 57.01(7) . 3 ?
Al7 Y2 Al1 122.99(7) 4 3 ?
Al6 Y2 Al1 57.01(7) 13 3 ?
Al1 Y2 Al1 93.17(9) . 3 ?
Y2 Y2 Al1 122.99(7) 16_556 2 ?
Al6 Y2 Al1 57.01(7) . 2 ?
Al6 Y2 Al1 122.99(7) 16_556 2 ?
Al7 Y2 Al1 57.01(7) . 2 ?
Al7 Y2 Al1 122.99(7) 4 2 ?
Al6 Y2 Al1 57.01(7) 13 2 ?
Al1 Y2 Al1 93.17(9) . 2 ?
Al1 Y2 Al1 93.17(9) 3 2 ?
Y2 Y2 Al3 84.54(7) 16_556 8 ?
Al6 Y2 Al3 95.46(7) . 8 ?
Al6 Y2 Al3 84.54(7) 16_556 8 ?
Al7 Y2 Al3 95.46(7) . 8 ?
Al7 Y2 Al3 84.54(7) 4 8 ?
Al6 Y2 Al3 95.46(7) 13 8 ?
Al1 Y2 Al3 88.57(4) . 8 ?
Al1 Y2 Al3 50.97(3) 3 8 ?
Al1 Y2 Al3 144.12(11) 2 8 ?
Y2 Y2 Al3 84.54(7) 16_556 2 ?
Al6 Y2 Al3 95.46(7) . 2 ?
Al6 Y2 Al3 84.54(7) 16_556 2 ?
Al7 Y2 Al3 95.46(7) . 2 ?
Al7 Y2 Al3 84.54(7) 4 2 ?
Al6 Y2 Al3 95.46(7) 13 2 ?
Al1 Y2 Al3 144.12(11) . 2 ?
Al1 Y2 Al3 50.97(3) 3 2 ?
Al1 Y2 Al3 88.57(4) 2 2 ?
Al3 Y2 Al3 70.20(4) 8 2 ?
Y2 Y2 Al3 84.54(7) 16_556 7 ?
Al6 Y2 Al3 95.46(7) . 7 ?
Al6 Y2 Al3 84.54(7) 16_556 7 ?
Al7 Y2 Al3 95.46(7) . 7 ?
Al7 Y2 Al3 84.54(7) 4 7 ?
Al6 Y2 Al3 95.46(7) 13 7 ?
Al1 Y2 Al3 50.97(3) . 7 ?
Al1 Y2 Al3 144.12(11) 3 7 ?
Al1 Y2 Al3 88.56(4) 2 7 ?
Al3 Y2 Al3 119.11(2) 8 7 ?
Al3 Y2 Al3 164.81(11) 2 7 ?
Y2 Y2 Al3 84.54(7) 16_556 . ?
Al6 Y2 Al3 95.46(7) . . ?
Al6 Y2 Al3 84.54(7) 16_556 . ?
Al7 Y2 Al3 95.46(7) . . ?
Al7 Y2 Al3 84.54(7) 4 . ?
Al6 Y2 Al3 95.46(7) 13 . ?
Al1 Y2 Al3 88.56(4) . . ?
Al1 Y2 Al3 144.12(11) 3 . ?
Al1 Y2 Al3 50.97(3) 2 . ?
Al3 Y2 Al3 164.81(11) 8 . ?
Al3 Y2 Al3 119.11(2) 2 . ?
Al3 Y2 Al3 49.19(4) 7 . ?
Y2 Y2 Al3 84.54(7) 16_556 9 ?
Al6 Y2 Al3 95.46(7) . 9 ?
Al6 Y2 Al3 84.54(7) 16_556 9 ?
Al7 Y2 Al3 95.46(7) . 9 ?
Al7 Y2 Al3 84.54(7) 4 9 ?
Al6 Y2 Al3 95.46(7) 13 9 ?
Al1 Y2 Al3 144.12(11) . 9 ?
Al1 Y2 Al3 88.56(4) 3 9 ?
Al1 Y2 Al3 50.97(3) 2 9 ?
Al3 Y2 Al3 119.10(2) 8 9 ?
Al3 Y2 Al3 49.19(4) 2 9 ?
Al3 Y2 Al3 119.10(2) 7 9 ?
Al3 Y2 Al3 70.20(4) . 9 ?
Y2 Y2 Al3 84.54(7) 16_556 3 ?
Al6 Y2 Al3 95.46(7) . 3 ?
Al6 Y2 Al3 84.54(7) 16_556 3 ?
Al7 Y2 Al3 95.46(7) . 3 ?
Al7 Y2 Al3 84.54(7) 4 3 ?
Al6 Y2 Al3 95.46(7) 13 3 ?
Al1 Y2 Al3 50.97(3) . 3 ?
Al1 Y2 Al3 88.56(4) 3 3 ?
Al1 Y2 Al3 144.12(11) 2 3 ?
Al3 Y2 Al3 49.19(4) 8 3 ?
Al3 Y2 Al3 119.10(2) 2 3 ?
Al3 Y2 Al3 70.20(4) 7 3 ?
Al3 Y2 Al3 119.10(2) . 3 ?
Al3 Y2 Al3 164.81(11) 9 3 ?
Y2 Y2 Al6 0.000(2) 16_556 4 ?
Al6 Y2 Al6 180.000(1) . 4 ?
Al6 Y2 Al6 0.000(1) 16_556 4 ?
Al7 Y2 Al6 180.000(1) . 4 ?
Al7 Y2 Al6 0.0 4 4 ?
Al6 Y2 Al6 180.000(1) 13 4 ?
Al1 Y2 Al6 122.99(7) . 4 ?
Al1 Y2 Al6 122.99(7) 3 4 ?
Al1 Y2 Al6 122.99(7) 2 4 ?
Al3 Y2 Al6 84.54(7) 8 4 ?
Al3 Y2 Al6 84.54(7) 2 4 ?
Al3 Y2 Al6 84.54(7) 7 4 ?
Al3 Y2 Al6 84.54(7) . 4 ?
Al3 Y2 Al6 84.54(7) 9 4 ?
Al3 Y2 Al6 84.54(7) 3 4 ?
Y2 Y2 Al1 130.23(6) 16_556 14 ?
Al6 Y2 Al1 49.77(6) . 14 ?
Al6 Y2 Al1 130.23(6) 16_556 14 ?
Al7 Y2 Al1 49.77(6) . 14 ?
Al7 Y2 Al1 130.23(6) 4 14 ?
Al6 Y2 Al1 49.77(6) 13 14 ?
Al1 Y2 Al1 47.79(4) . 14 ?
Al1 Y2 Al1 47.79(4) 3 14 ?
Al1 Y2 Al1 106.78(12) 2 14 ?
Al3 Y2 Al1 51.03(3) 8 14 ?
Al3 Y2 Al1 97.55(5) 2 14 ?
Al3 Y2 Al1 97.56(5) 7 14 ?
Al3 Y2 Al1 132.99(9) . 14 ?
Al3 Y2 Al1 132.99(9) 9 14 ?
Al3 Y2 Al1 51.03(3) 3 14 ?
Al6 Y2 Al1 130.23(6) 4 14 ?
Y2 Y2 Al1 130.23(6) 16_556 13 ?
Al6 Y2 Al1 49.77(6) . 13 ?
Al6 Y2 Al1 130.23(6) 16_556 13 ?
Al7 Y2 Al1 49.77(6) . 13 ?
Al7 Y2 Al1 130.23(6) 4 13 ?
Al6 Y2 Al1 49.77(6) 13 13 ?
Al1 Y2 Al1 106.78(12) . 13 ?
Al1 Y2 Al1 47.79(4) 3 13 ?
Al1 Y2 Al1 47.79(4) 2 13 ?
Al3 Y2 Al1 97.55(5) 8 13 ?
Al3 Y2 Al1 51.03(3) 2 13 ?
Al3 Y2 Al1 132.99(9) 7 13 ?
Al3 Y2 Al1 97.55(5) . 13 ?
Al3 Y2 Al1 51.03(3) 9 13 ?
Al3 Y2 Al1 132.99(9) 3 13 ?
Al6 Y2 Al1 130.23(6) 4 13 ?
Al1 Y2 Al1 82.78(9) 14 13 ?
Y2 Y2 Al1 130.23(6) 16_556 15 ?
Al6 Y2 Al1 49.77(6) . 15 ?
Al6 Y2 Al1 130.23(6) 16_556 15 ?
Al7 Y2 Al1 49.77(6) . 15 ?
Al7 Y2 Al1 130.23(6) 4 15 ?
Al6 Y2 Al1 49.77(6) 13 15 ?
Al1 Y2 Al1 47.79(4) . 15 ?
Al1 Y2 Al1 106.78(12) 3 15 ?
Al1 Y2 Al1 47.79(4) 2 15 ?
Al3 Y2 Al1 132.99(9) 8 15 ?
Al3 Y2 Al1 132.99(9) 2 15 ?
Al3 Y2 Al1 51.03(3) 7 15 ?
Al3 Y2 Al1 51.03(3) . 15 ?
Al3 Y2 Al1 97.55(5) 9 15 ?
Al3 Y2 Al1 97.55(5) 3 15 ?
Al6 Y2 Al1 130.23(6) 4 15 ?
Al1 Y2 Al1 82.78(9) 14 15 ?
Al1 Y2 Al1 82.78(9) 13 15 ?
Y2 Y2 Al1 48.48(6) 16_556 17_556 ?
Al6 Y2 Al1 131.52(6) . 17_556 ?
Al6 Y2 Al1 48.48(6) 16_556 17_556 ?
Al7 Y2 Al1 131.52(6) . 17_556 ?
Al7 Y2 Al1 48.48(6) 4 17_556 ?
Al6 Y2 Al1 131.52(6) 13 17_556 ?
Al1 Y2 Al1 132.45(3) . 17_556 ?
Al1 Y2 Al1 132.45(3) 3 17_556 ?
Al1 Y2 Al1 74.51(5) 2 17_556 ?
Al3 Y2 Al1 127.87(11) 8 17_556 ?
Al3 Y2 Al1 82.43(5) 2 17_556 ?
Al3 Y2 Al1 82.43(5) 7 17_556 ?
Al3 Y2 Al1 47.82(3) . 17_556 ?
Al3 Y2 Al1 47.82(3) 9 17_556 ?
Al3 Y2 Al1 127.87(11) 3 17_556 ?
Al6 Y2 Al1 48.48(6) 4 17_556 ?
Al1 Y2 Al1 178.70(11) 14 17_556 ?
Al1 Y2 Al1 98.18(2) 13 17_556 ?
Al1 Y2 Al1 98.18(2) 15 17_556 ?
Y2 Y2 Al1 48.48(6) 16_556 16_556 ?
Al6 Y2 Al1 131.52(6) . 16_556 ?
Al6 Y2 Al1 48.48(6) 16_556 16_556 ?
Al7 Y2 Al1 131.52(6) . 16_556 ?
Al7 Y2 Al1 48.48(6) 4 16_556 ?
Al6 Y2 Al1 131.52(6) 13 16_556 ?
Al1 Y2 Al1 74.51(5) . 16_556 ?
Al1 Y2 Al1 132.45(3) 3 16_556 ?
Al1 Y2 Al1 132.45(3) 2 16_556 ?
Al3 Y2 Al1 82.43(5) 8 16_556 ?
Al3 Y2 Al1 127.87(11) 2 16_556 ?
Al3 Y2 Al1 47.82(3) 7 16_556 ?
Al3 Y2 Al1 82.43(5) . 16_556 ?
Al3 Y2 Al1 127.87(11) 9 16_556 ?
Al3 Y2 Al1 47.82(3) 3 16_556 ?
Al6 Y2 Al1 48.48(6) 4 16_556 ?
Al1 Y2 Al1 98.18(2) 14 16_556 ?
Al1 Y2 Al1 178.70(11) 13 16_556 ?
Al1 Y2 Al1 98.18(2) 15 16_556 ?
Al1 Y2 Al1 80.84(8) 17_556 16_556 ?
Y2 Y2 Al1 48.48(6) 16_556 18_556 ?
Al6 Y2 Al1 131.52(6) . 18_556 ?
Al6 Y2 Al1 48.48(6) 16_556 18_556 ?
Al7 Y2 Al1 131.52(6) . 18_556 ?
Al7 Y2 Al1 48.48(6) 4 18_556 ?
Al6 Y2 Al1 131.52(6) 13 18_556 ?
Al1 Y2 Al1 132.45(3) . 18_556 ?
Al1 Y2 Al1 74.51(5) 3 18_556 ?
Al1 Y2 Al1 132.45(3) 2 18_556 ?
Al3 Y2 Al1 47.82(3) 8 18_556 ?
Al3 Y2 Al1 47.82(3) 2 18_556 ?
Al3 Y2 Al1 127.87(11) 7 18_556 ?
Al3 Y2 Al1 127.87(11) . 18_556 ?
Al3 Y2 Al1 82.43(5) 9 18_556 ?
Al3 Y2 Al1 82.43(5) 3 18_556 ?
Al6 Y2 Al1 48.48(6) 4 18_556 ?
Al1 Y2 Al1 98.18(2) 14 18_556 ?
Al1 Y2 Al1 98.18(2) 13 18_556 ?
Al1 Y2 Al1 178.70(11) 15 18_556 ?
Al1 Y2 Al1 80.84(8) 17_556 18_556 ?
Al1 Y2 Al1 80.84(8) 16_556 18_556 ?
Y2 Y2 Al1 42.74(5) 16_556 6 ?
Al6 Y2 Al1 137.26(5) . 6 ?
Al6 Y2 Al1 42.74(5) 16_556 6 ?
Al7 Y2 Al1 137.26(5) . 6 ?
Al7 Y2 Al1 42.74(5) 4 6 ?
Al6 Y2 Al1 137.26(5) 13 6 ?
Al1 Y2 Al1 96.62(3) . 6 ?
Al1 Y2 Al1 165.74(11) 3 6 ?
Al1 Y2 Al1 96.62(3) 2 6 ?
Al3 Y2 Al1 118.79(10) 8 6 ?
Al3 Y2 Al1 118.79(10) 2 6 ?
Al3 Y2 Al1 46.87(4) 7 6 ?
Al3 Y2 Al1 46.87(4) . 6 ?
Al3 Y2 Al1 89.56(6) 9 6 ?
Al3 Y2 Al1 89.56(6) 3 6 ?
Al6 Y2 Al1 42.74(5) 4 6 ?
Al1 Y2 Al1 137.17(2) 14 6 ?
Al1 Y2 Al1 137.17(2) 13 6 ?
Al1 Y2 Al1 87.48(4) 15 6 ?
Al1 Y2 Al1 42.19(4) 17_556 6 ?
Al1 Y2 Al1 42.19(4) 16_556 6 ?
Al1 Y2 Al1 91.22(10) 18_556 6 ?
Y2 Y2 Al1 42.74(5) 16_556 5 ?
Al6 Y2 Al1 137.26(5) . 5 ?
Al6 Y2 Al1 42.74(5) 16_556 5 ?
Al7 Y2 Al1 137.26(5) . 5 ?
Al7 Y2 Al1 42.74(5) 4 5 ?
Al6 Y2 Al1 137.26(5) 13 5 ?
Al1 Y2 Al1 96.62(3) . 5 ?
Al1 Y2 Al1 96.62(3) 3 5 ?
Al1 Y2 Al1 165.74(11) 2 5 ?
Al3 Y2 Al1 46.87(4) 8 5 ?
Al3 Y2 Al1 89.56(6) 2 5 ?
Al3 Y2 Al1 89.56(6) 7 5 ?
Al3 Y2 Al1 118.79(10) . 5 ?
Al3 Y2 Al1 118.79(10) 9 5 ?
Al3 Y2 Al1 46.87(4) 3 5 ?
Al6 Y2 Al1 42.74(5) 4 5 ?
Al1 Y2 Al1 87.48(4) 14 5 ?
Al1 Y2 Al1 137.17(2) 13 5 ?
Al1 Y2 Al1 137.17(2) 15 5 ?
Al1 Y2 Al1 91.22(10) 17_556 5 ?
Al1 Y2 Al1 42.19(4) 16_556 5 ?
Al1 Y2 Al1 42.19(4) 18_556 5 ?
Al1 Y2 Al1 72.00(7) 6 5 ?
Y2 Y2 Al1 42.74(5) 16_556 4 ?
Al6 Y2 Al1 137.26(5) . 4 ?
Al6 Y2 Al1 42.74(5) 16_556 4 ?
Al7 Y2 Al1 137.26(5) . 4 ?
Al7 Y2 Al1 42.74(5) 4 4 ?
Al6 Y2 Al1 137.26(5) 13 4 ?
Al1 Y2 Al1 165.74(11) . 4 ?
Al1 Y2 Al1 96.62(3) 3 4 ?
Al1 Y2 Al1 96.62(3) 2 4 ?
Al3 Y2 Al1 89.56(6) 8 4 ?
Al3 Y2 Al1 46.87(4) 2 4 ?
Al3 Y2 Al1 118.79(10) 7 4 ?
Al3 Y2 Al1 89.56(6) . 4 ?
Al3 Y2 Al1 46.87(4) 9 4 ?
Al3 Y2 Al1 118.79(10) 3 4 ?
Al6 Y2 Al1 42.74(5) 4 4 ?
Al1 Y2 Al1 137.17(2) 14 4 ?
Al1 Y2 Al1 87.48(4) 13 4 ?
Al1 Y2 Al1 137.17(2) 15 4 ?
Al1 Y2 Al1 42.19(4) 17_556 4 ?
Al1 Y2 Al1 91.22(10) 16_556 4 ?
Al1 Y2 Al1 42.19(4) 18_556 4 ?
Al1 Y2 Al1 72.00(7) 6 4 ?
Al1 Y2 Al1 72.00(7) 5 4 ?
Y2 Y2 Y2 180.0 16_556 13 ?
Al6 Y2 Y2 0.0 . 13 ?
Al6 Y2 Y2 180.000(1) 16_556 13 ?
Al7 Y2 Y2 0.0 . 13 ?
Al7 Y2 Y2 180.0 4 13 ?
Al6 Y2 Y2 0.0 13 13 ?
Al1 Y2 Y2 57.01(7) . 13 ?
Al1 Y2 Y2 57.01(7) 3 13 ?
Al1 Y2 Y2 57.01(7) 2 13 ?
Al3 Y2 Y2 95.46(7) 8 13 ?
Al3 Y2 Y2 95.46(7) 2 13 ?
Al3 Y2 Y2 95.46(7) 7 13 ?
Al3 Y2 Y2 95.46(7) . 13 ?
Al3 Y2 Y2 95.46(7) 9 13 ?
Al3 Y2 Y2 95.46(7) 3 13 ?
Al6 Y2 Y2 180.000(1) 4 13 ?
Al1 Y2 Y2 49.77(6) 14 13 ?
Al1 Y2 Y2 49.77(6) 13 13 ?
Al1 Y2 Y2 49.77(6) 15 13 ?
Al1 Y2 Y2 131.52(6) 17_556 13 ?
Al1 Y2 Y2 131.52(6) 16_556 13 ?
Al1 Y2 Y2 131.52(6) 18_556 13 ?
Al1 Y2 Y2 137.26(5) 6 13 ?
Al1 Y2 Y2 137.26(5) 5 13 ?
Al1 Y2 Y2 137.26(5) 4 13 ?
Y2 Y2 Y3 180.000(1) 16_556 13 ?
Al6 Y2 Y3 0.0 . 13 ?
Al6 Y2 Y3 180.000(1) 16_556 13 ?
Al7 Y2 Y3 0.0 . 13 ?
Al7 Y2 Y3 180.0 4 13 ?
Al6 Y2 Y3 0.0 13 13 ?
Al1 Y2 Y3 57.01(7) . 13 ?
Al1 Y2 Y3 57.01(7) 3 13 ?
Al1 Y2 Y3 57.01(7) 2 13 ?
Al3 Y2 Y3 95.46(7) 8 13 ?
Al3 Y2 Y3 95.46(7) 2 13 ?
Al3 Y2 Y3 95.46(7) 7 13 ?
Al3 Y2 Y3 95.46(7) . 13 ?
Al3 Y2 Y3 95.46(7) 9 13 ?
Al3 Y2 Y3 95.46(7) 3 13 ?
Al6 Y2 Y3 180.000(1) 4 13 ?
Al1 Y2 Y3 49.77(6) 14 13 ?
Al1 Y2 Y3 49.77(6) 13 13 ?
Al1 Y2 Y3 49.77(6) 15 13 ?
Al1 Y2 Y3 131.52(6) 17_556 13 ?
Al1 Y2 Y3 131.52(6) 16_556 13 ?
Al1 Y2 Y3 131.52(6) 18_556 13 ?
Al1 Y2 Y3 137.26(5) 6 13 ?
Al1 Y2 Y3 137.26(5) 5 13 ?
Al1 Y2 Y3 137.26(5) 4 13 ?
Y2 Y2 Y3 0.0 13 13 ?
Y2 Y2 Y2 0.0 16_556 4 ?
Al6 Y2 Y2 180.000(1) . 4 ?
Al6 Y2 Y2 0.000(1) 16_556 4 ?
Al7 Y2 Y2 180.0 . 4 ?
Al7 Y2 Y2 0.0 4 4 ?
Al6 Y2 Y2 180.0 13 4 ?
Al1 Y2 Y2 122.99(7) . 4 ?
Al1 Y2 Y2 122.99(7) 3 4 ?
Al1 Y2 Y2 122.99(7) 2 4 ?
Al3 Y2 Y2 84.54(7) 8 4 ?
Al3 Y2 Y2 84.54(7) 2 4 ?
Al3 Y2 Y2 84.54(7) 7 4 ?
Al3 Y2 Y2 84.54(7) . 4 ?
Al3 Y2 Y2 84.54(7) 9 4 ?
Al3 Y2 Y2 84.54(7) 3 4 ?
Al6 Y2 Y2 0.000(1) 4 4 ?
Al1 Y2 Y2 130.23(6) 14 4 ?
Al1 Y2 Y2 130.23(6) 13 4 ?
Al1 Y2 Y2 130.23(6) 15 4 ?
Al1 Y2 Y2 48.48(6) 17_556 4 ?
Al1 Y2 Y2 48.48(6) 16_556 4 ?
Al1 Y2 Y2 48.48(6) 18_556 4 ?
Al1 Y2 Y2 42.74(5) 6 4 ?
Al1 Y2 Y2 42.74(5) 5 4 ?
Al1 Y2 Y2 42.74(5) 4 4 ?
Y2 Y2 Y2 180.0 13 4 ?
Y3 Y2 Y2 180.0 13 4 ?
Y2 Y2 Y2 180.000(2) 16_556 4_554 ?
Al6 Y2 Y2 0.0 . 4_554 ?
Al6 Y2 Y2 180.000(1) 16_556 4_554 ?
Al7 Y2 Y2 0.0 . 4_554 ?
Al7 Y2 Y2 180.0 4 4_554 ?
Al6 Y2 Y2 0.0 13 4_554 ?
Al1 Y2 Y2 57.01(7) . 4_554 ?
Al1 Y2 Y2 57.01(7) 3 4_554 ?
Al1 Y2 Y2 57.01(7) 2 4_554 ?
Al3 Y2 Y2 95.46(7) 8 4_554 ?
Al3 Y2 Y2 95.46(7) 2 4_554 ?
Al3 Y2 Y2 95.46(7) 7 4_554 ?
Al3 Y2 Y2 95.46(7) . 4_554 ?
Al3 Y2 Y2 95.46(7) 9 4_554 ?
Al3 Y2 Y2 95.46(7) 3 4_554 ?
Al6 Y2 Y2 180.000(1) 4 4_554 ?
Al1 Y2 Y2 49.77(6) 14 4_554 ?
Al1 Y2 Y2 49.77(6) 13 4_554 ?
Al1 Y2 Y2 49.77(6) 15 4_554 ?
Al1 Y2 Y2 131.52(6) 17_556 4_554 ?
Al1 Y2 Y2 131.52(6) 16_556 4_554 ?
Al1 Y2 Y2 131.52(6) 18_556 4_554 ?
Al1 Y2 Y2 137.26(5) 6 4_554 ?
Al1 Y2 Y2 137.26(5) 5 4_554 ?
Al1 Y2 Y2 137.26(5) 4 4_554 ?
Y2 Y2 Y2 0.0 13 4_554 ?
Y3 Y2 Y2 0.0 13 4_554 ?
Y2 Y2 Y2 180.0 4 4_554 ?
Y2 Y2 Y3 0.000(1) 16_556 13_556 ?
Al6 Y2 Y3 180.0 . 13_556 ?
Al6 Y2 Y3 0.000(1) 16_556 13_556 ?
Al7 Y2 Y3 180.0 . 13_556 ?
Al7 Y2 Y3 0.0 4 13_556 ?
Al6 Y2 Y3 180.0 13 13_556 ?
Al1 Y2 Y3 122.99(7) . 13_556 ?
Al1 Y2 Y3 122.99(7) 3 13_556 ?
Al1 Y2 Y3 122.99(7) 2 13_556 ?
Al3 Y2 Y3 84.54(7) 8 13_556 ?
Al3 Y2 Y3 84.54(7) 2 13_556 ?
Al3 Y2 Y3 84.54(7) 7 13_556 ?
Al3 Y2 Y3 84.54(7) . 13_556 ?
Al3 Y2 Y3 84.54(7) 9 13_556 ?
Al3 Y2 Y3 84.54(7) 3 13_556 ?
Al6 Y2 Y3 0.000(1) 4 13_556 ?
Al1 Y2 Y3 130.23(6) 14 13_556 ?
Al1 Y2 Y3 130.23(6) 13 13_556 ?
Al1 Y2 Y3 130.23(6) 15 13_556 ?
Al1 Y2 Y3 48.48(6) 17_556 13_556 ?
Al1 Y2 Y3 48.48(6) 16_556 13_556 ?
Al1 Y2 Y3 48.48(6) 18_556 13_556 ?
Al1 Y2 Y3 42.74(5) 6 13_556 ?
Al1 Y2 Y3 42.74(5) 5 13_556 ?
Al1 Y2 Y3 42.74(5) 4 13_556 ?
Y2 Y2 Y3 180.0 13 13_556 ?
Y3 Y2 Y3 180.0 13 13_556 ?
Y2 Y2 Y3 0.0 4 13_556 ?
Y2 Y2 Y3 180.0 4_554 13_556 ?
Y2 Y3 Al6 180.000(6) 16_556 . ?
Y2 Y3 Al6 0.000(4) 16_556 16_556 ?
Al6 Y3 Al6 180.000(2) . 16_556 ?
Y2 Y3 Al7 0.000(2) 16_556 4 ?
Al6 Y3 Al7 180.0 . 4 ?
Al6 Y3 Al7 0.000(2) 16_556 4 ?
Y2 Y3 Al7 180.000(2) 16_556 . ?
Al6 Y3 Al7 0.0 . . ?
Al6 Y3 Al7 180.000(2) 16_556 . ?
Al7 Y3 Al7 180.0 4 . ?
Y2 Y3 Al6 0.000(4) 16_556 4 ?
Al6 Y3 Al6 180.000(2) . 4 ?
Al6 Y3 Al6 0.000(1) 16_556 4 ?
Al7 Y3 Al6 0.0 4 4 ?
Al7 Y3 Al6 180.000(1) . 4 ?
Y2 Y3 Al6 180.000(5) 16_556 13 ?
Al6 Y3 Al6 0.0 . 13 ?
Al6 Y3 Al6 180.000(3) 16_556 13 ?
Al7 Y3 Al6 180.000(1) 4 13 ?
Al7 Y3 Al6 0.0 . 13 ?
Al6 Y3 Al6 180.0 4 13 ?
Y2 Y3 Al3 90.000(1) 16_556 8 ?
Al6 Y3 Al3 90.000(1) . 8 ?
Al6 Y3 Al3 90.000(1) 16_556 8 ?
Al7 Y3 Al3 90.0 4 8 ?
Al7 Y3 Al3 90.0 . 8 ?
Al6 Y3 Al3 90.0 4 8 ?
Al6 Y3 Al3 90.0 13 8 ?
Y2 Y3 Al3 90.000(1) 16_556 2 ?
Al6 Y3 Al3 90.000(1) . 2 ?
Al6 Y3 Al3 90.000(1) 16_556 2 ?
Al7 Y3 Al3 90.0 4 2 ?
Al7 Y3 Al3 90.0 . 2 ?
Al6 Y3 Al3 90.0 4 2 ?
Al6 Y3 Al3 90.0 13 2 ?
Al3 Y3 Al3 70.57(4) 8 2 ?
Y2 Y3 Al3 90.000(1) 16_556 7 ?
Al6 Y3 Al3 90.000(1) . 7 ?
Al6 Y3 Al3 90.000(1) 16_556 7 ?
Al7 Y3 Al3 90.0 4 7 ?
Al7 Y3 Al3 90.0 . 7 ?
Al6 Y3 Al3 90.0 4 7 ?
Al6 Y3 Al3 90.0 13 7 ?
Al3 Y3 Al3 120.0 8 7 ?
Al3 Y3 Al3 169.43(4) 2 7 ?
Y2 Y3 Al3 90.000(1) 16_556 . ?
Al6 Y3 Al3 90.000(1) . . ?
Al6 Y3 Al3 90.000(1) 16_556 . ?
Al7 Y3 Al3 90.0 4 . ?
Al7 Y3 Al3 90.0 . . ?
Al6 Y3 Al3 90.0 4 . ?
Al6 Y3 Al3 90.0 13 . ?
Al3 Y3 Al3 169.43(4) 8 . ?
Al3 Y3 Al3 120.0 2 . ?
Al3 Y3 Al3 49.43(4) 7 . ?
Y2 Y3 Al3 90.0 16_556 9 ?
Al6 Y3 Al3 90.0 . 9 ?
Al6 Y3 Al3 90.0 16_556 9 ?
Al7 Y3 Al3 90.0 4 9 ?
Al7 Y3 Al3 90.0 . 9 ?
Al6 Y3 Al3 90.0 4 9 ?
Al6 Y3 Al3 90.0 13 9 ?
Al3 Y3 Al3 120.0 8 9 ?
Al3 Y3 Al3 49.43(4) 2 9 ?
Al3 Y3 Al3 120.0 7 9 ?
Al3 Y3 Al3 70.57(4) . 9 ?
Y2 Y3 Al3 90.0 16_556 3 ?
Al6 Y3 Al3 90.0 . 3 ?
Al6 Y3 Al3 90.0 16_556 3 ?
Al7 Y3 Al3 90.0 4 3 ?
Al7 Y3 Al3 90.0 . 3 ?
Al6 Y3 Al3 90.0 4 3 ?
Al6 Y3 Al3 90.0 13 3 ?
Al3 Y3 Al3 49.43(4) 8 3 ?
Al3 Y3 Al3 120.0 2 3 ?
Al3 Y3 Al3 70.57(4) 7 3 ?
Al3 Y3 Al3 120.0 . 3 ?
Al3 Y3 Al3 169.43(4) 9 3 ?
Y2 Y3 Al1 127.50(2) 16_556 . ?
Al6 Y3 Al1 52.50(2) . . ?
Al6 Y3 Al1 127.50(2) 16_556 . ?
Al7 Y3 Al1 127.50(2) 4 . ?
Al7 Y3 Al1 52.50(2) . . ?
Al6 Y3 Al1 127.50(2) 4 . ?
Al6 Y3 Al1 52.50(2) 13 . ?
Al3 Y3 Al1 85.811(17) 8 . ?
Al3 Y3 Al1 136.11(2) 2 . ?
Al3 Y3 Al1 49.638(19) 7 . ?
Al3 Y3 Al1 85.810(17) . . ?
Al3 Y3 Al1 136.11(2) 9 . ?
Al3 Y3 Al1 49.637(19) 3 . ?
Y2 Y3 Al1 127.50(2) 16_556 3 ?
Al6 Y3 Al1 52.50(2) . 3 ?
Al6 Y3 Al1 127.50(2) 16_556 3 ?
Al7 Y3 Al1 127.50(2) 4 3 ?
Al7 Y3 Al1 52.50(2) . 3 ?
Al6 Y3 Al1 127.50(2) 4 3 ?
Al6 Y3 Al1 52.50(2) 13 3 ?
Al3 Y3 Al1 49.637(19) 8 3 ?
Al3 Y3 Al1 49.637(19) 2 3 ?
Al3 Y3 Al1 136.11(2) 7 3 ?
Al3 Y3 Al1 136.11(2) . 3 ?
Al3 Y3 Al1 85.810(17) 9 3 ?
Al3 Y3 Al1 85.810(17) 3 3 ?
Al1 Y3 Al1 86.80(3) . 3 ?
Y2 Y3 Al1 52.50(2) 16_556 17_556 ?
Al6 Y3 Al1 127.50(2) . 17_556 ?
Al6 Y3 Al1 52.50(2) 16_556 17_556 ?
Al7 Y3 Al1 52.50(2) 4 17_556 ?
Al7 Y3 Al1 127.50(2) . 17_556 ?
Al6 Y3 Al1 52.50(2) 4 17_556 ?
Al6 Y3 Al1 127.50(2) 13 17_556 ?
Al3 Y3 Al1 136.11(2) 8 17_556 ?
Al3 Y3 Al1 85.811(17) 2 17_556 ?
Al3 Y3 Al1 85.810(17) 7 17_556 ?
Al3 Y3 Al1 49.637(19) . 17_556 ?
Al3 Y3 Al1 49.637(19) 9 17_556 ?
Al3 Y3 Al1 136.11(2) 3 17_556 ?
Al1 Y3 Al1 133.258(15) . 17_556 ?
Al1 Y3 Al1 133.258(15) 3 17_556 ?
Y2 Y3 Al1 52.50(2) 16_556 16_556 ?
Al6 Y3 Al1 127.50(2) . 16_556 ?
Al6 Y3 Al1 52.50(2) 16_556 16_556 ?
Al7 Y3 Al1 52.50(2) 4 16_556 ?
Al7 Y3 Al1 127.50(2) . 16_556 ?
Al6 Y3 Al1 52.50(2) 4 16_556 ?
Al6 Y3 Al1 127.50(2) 13 16_556 ?
Al3 Y3 Al1 85.811(17) 8 16_556 ?
Al3 Y3 Al1 136.11(2) 2 16_556 ?
Al3 Y3 Al1 49.638(19) 7 16_556 ?
Al3 Y3 Al1 85.810(17) . 16_556 ?
Al3 Y3 Al1 136.11(2) 9 16_556 ?
Al3 Y3 Al1 49.637(19) 3 16_556 ?
Al1 Y3 Al1 75.00(4) . 16_556 ?
Al1 Y3 Al1 133.258(15) 3 16_556 ?
Al1 Y3 Al1 86.80(3) 17_556 16_556 ?
Y2 Y3 Al1 52.50(2) 16_556 18_556 ?
Al6 Y3 Al1 127.50(2) . 18_556 ?
Al6 Y3 Al1 52.50(2) 16_556 18_556 ?
Al7 Y3 Al1 52.50(2) 4 18_556 ?
Al7 Y3 Al1 127.50(2) . 18_556 ?
Al6 Y3 Al1 52.50(2) 4 18_556 ?
Al6 Y3 Al1 127.50(2) 13 18_556 ?
Al3 Y3 Al1 49.637(19) 8 18_556 ?
Al3 Y3 Al1 49.637(19) 2 18_556 ?
Al3 Y3 Al1 136.11(2) 7 18_556 ?
Al3 Y3 Al1 136.11(2) . 18_556 ?
Al3 Y3 Al1 85.810(17) 9 18_556 ?
Al3 Y3 Al1 85.810(17) 3 18_556 ?
Al1 Y3 Al1 133.258(15) . 18_556 ?
Al1 Y3 Al1 75.00(4) 3 18_556 ?
Al1 Y3 Al1 86.80(3) 17_556 18_556 ?
Al1 Y3 Al1 86.80(3) 16_556 18_556 ?
Y2 Y3 Al1 127.50(2) 16_556 2 ?
Al6 Y3 Al1 52.50(2) . 2 ?
Al6 Y3 Al1 127.50(2) 16_556 2 ?
Al7 Y3 Al1 127.50(2) 4 2 ?
Al7 Y3 Al1 52.50(2) . 2 ?
Al6 Y3 Al1 127.50(2) 4 2 ?
Al6 Y3 Al1 52.50(2) 13 2 ?
Al3 Y3 Al1 136.11(2) 8 2 ?
Al3 Y3 Al1 85.811(17) 2 2 ?
Al3 Y3 Al1 85.810(17) 7 2 ?
Al3 Y3 Al1 49.637(19) . 2 ?
Al3 Y3 Al1 49.637(19) 9 2 ?
Al3 Y3 Al1 136.11(2) 3 2 ?
Al1 Y3 Al1 86.80(3) . 2 ?
Al1 Y3 Al1 86.80(3) 3 2 ?
Al1 Y3 Al1 75.00(4) 17_556 2 ?
Al1 Y3 Al1 133.258(15) 16_556 2 ?
Al1 Y3 Al1 133.258(15) 18_556 2 ?
Y2 Y3 Al1 46.05(2) 16_556 6 ?
Al6 Y3 Al1 133.95(2) . 6 ?
Al6 Y3 Al1 46.05(2) 16_556 6 ?
Al7 Y3 Al1 46.05(2) 4 6 ?
Al7 Y3 Al1 133.95(2) . 6 ?
Al6 Y3 Al1 46.05(2) 4 6 ?
Al6 Y3 Al1 133.95(2) 13 6 ?
Al3 Y3 Al1 125.995(18) 8 6 ?
Al3 Y3 Al1 125.995(18) 2 6 ?
Al3 Y3 Al1 49.155(19) 7 6 ?
Al3 Y3 Al1 49.155(19) . 6 ?
Al3 Y3 Al1 93.802(16) 9 6 ?
Al3 Y3 Al1 93.802(16) 3 6 ?
Al1 Y3 Al1 97.87(2) . 6 ?
Al1 Y3 Al1 173.55(3) 3 6 ?
Al1 Y3 Al1 44.922(11) 17_556 6 ?
Al1 Y3 Al1 44.922(11) 16_556 6 ?
Al1 Y3 Al1 98.55(3) 18_556 6 ?
Al1 Y3 Al1 97.87(2) 2 6 ?
Y2 Y3 Al1 133.95(2) 16_556 14 ?
Al6 Y3 Al1 46.05(2) . 14 ?
Al6 Y3 Al1 133.95(2) 16_556 14 ?
Al7 Y3 Al1 133.95(2) 4 14 ?
Al7 Y3 Al1 46.05(2) . 14 ?
Al6 Y3 Al1 133.95(2) 4 14 ?
Al6 Y3 Al1 46.05(2) 13 14 ?
Al3 Y3 Al1 49.155(19) 8 14 ?
Al3 Y3 Al1 93.801(16) 2 14 ?
Al3 Y3 Al1 93.802(16) 7 14 ?
Al3 Y3 Al1 125.995(18) . 14 ?
Al3 Y3 Al1 125.995(18) 9 14 ?
Al3 Y3 Al1 49.155(19) 3 14 ?
Al1 Y3 Al1 44.922(11) . 14 ?
Al1 Y3 Al1 44.922(11) 3 14 ?
Al1 Y3 Al1 173.55(3) 17_556 14 ?
Al1 Y3 Al1 97.87(2) 16_556 14 ?
Al1 Y3 Al1 97.87(2) 18_556 14 ?
Al1 Y3 Al1 98.55(3) 2 14 ?
Al1 Y3 Al1 137.802(15) 6 14 ?
Y2 Y3 Al1 133.95(2) 16_556 13 ?
Al6 Y3 Al1 46.05(2) . 13 ?
Al6 Y3 Al1 133.95(2) 16_556 13 ?
Al7 Y3 Al1 133.95(2) 4 13 ?
Al7 Y3 Al1 46.05(2) . 13 ?
Al6 Y3 Al1 133.95(2) 4 13 ?
Al6 Y3 Al1 46.05(2) 13 13 ?
Al3 Y3 Al1 93.801(16) 8 13 ?
Al3 Y3 Al1 49.155(19) 2 13 ?
Al3 Y3 Al1 125.994(18) 7 13 ?
Al3 Y3 Al1 93.802(16) . 13 ?
Al3 Y3 Al1 49.155(19) 9 13 ?
Al3 Y3 Al1 125.995(18) 3 13 ?
Al1 Y3 Al1 98.55(3) . 13 ?
Al1 Y3 Al1 44.922(11) 3 13 ?
Al1 Y3 Al1 97.87(2) 17_556 13 ?
Al1 Y3 Al1 173.55(3) 16_556 13 ?
Al1 Y3 Al1 97.87(2) 18_556 13 ?
Al1 Y3 Al1 44.922(11) 2 13 ?
Al1 Y3 Al1 137.802(15) 6 13 ?
Al1 Y3 Al1 77.15(3) 14 13 ?
Y2 Y3 Al1 133.95(2) 16_556 15 ?
Al6 Y3 Al1 46.05(2) . 15 ?
Al6 Y3 Al1 133.95(2) 16_556 15 ?
Al7 Y3 Al1 133.95(2) 4 15 ?
Al7 Y3 Al1 46.05(2) . 15 ?
Al6 Y3 Al1 133.95(2) 4 15 ?
Al6 Y3 Al1 46.05(2) 13 15 ?
Al3 Y3 Al1 125.995(18) 8 15 ?
Al3 Y3 Al1 125.995(18) 2 15 ?
Al3 Y3 Al1 49.155(19) 7 15 ?
Al3 Y3 Al1 49.155(19) . 15 ?
Al3 Y3 Al1 93.802(16) 9 15 ?
Al3 Y3 Al1 93.802(16) 3 15 ?
Al1 Y3 Al1 44.922(11) . 15 ?
Al1 Y3 Al1 98.55(3) 3 15 ?
Al1 Y3 Al1 97.87(2) 17_556 15 ?
Al1 Y3 Al1 97.87(2) 16_556 15 ?
Al1 Y3 Al1 173.55(3) 18_556 15 ?
Al1 Y3 Al1 44.922(11) 2 15 ?
Al1 Y3 Al1 87.90(4) 6 15 ?
Al1 Y3 Al1 77.15(3) 14 15 ?
Al1 Y3 Al1 77.15(3) 13 15 ?
Y2 Y3 Al1 46.05(2) 16_556 5 ?
Al6 Y3 Al1 133.95(2) . 5 ?
Al6 Y3 Al1 46.05(2) 16_556 5 ?
Al7 Y3 Al1 46.05(2) 4 5 ?
Al7 Y3 Al1 133.95(2) . 5 ?
Al6 Y3 Al1 46.05(2) 4 5 ?
Al6 Y3 Al1 133.95(2) 13 5 ?
Al3 Y3 Al1 49.156(19) 8 5 ?
Al3 Y3 Al1 93.801(16) 2 5 ?
Al3 Y3 Al1 93.802(16) 7 5 ?
Al3 Y3 Al1 125.995(18) . 5 ?
Al3 Y3 Al1 125.995(18) 9 5 ?
Al3 Y3 Al1 49.155(19) 3 5 ?
Al1 Y3 Al1 97.87(2) . 5 ?
Al1 Y3 Al1 97.87(2) 3 5 ?
Al1 Y3 Al1 98.55(3) 17_556 5 ?
Al1 Y3 Al1 44.922(11) 16_556 5 ?
Al1 Y3 Al1 44.922(11) 18_556 5 ?
Al1 Y3 Al1 173.55(3) 2 5 ?
Al1 Y3 Al1 77.15(3) 6 5 ?
Al1 Y3 Al1 87.90(4) 14 5 ?
Al1 Y3 Al1 137.802(15) 13 5 ?
Al1 Y3 Al1 137.802(15) 15 5 ?
Y2 Y3 Al1 46.05(2) 16_556 4 ?
Al6 Y3 Al1 133.95(2) . 4 ?
Al6 Y3 Al1 46.05(2) 16_556 4 ?
Al7 Y3 Al1 46.05(2) 4 4 ?
Al7 Y3 Al1 133.95(2) . 4 ?
Al6 Y3 Al1 46.05(2) 4 4 ?
Al6 Y3 Al1 133.95(2) 13 4 ?
Al3 Y3 Al1 93.801(16) 8 4 ?
Al3 Y3 Al1 49.156(19) 2 4 ?
Al3 Y3 Al1 125.994(18) 7 4 ?
Al3 Y3 Al1 93.802(16) . 4 ?
Al3 Y3 Al1 49.155(19) 9 4 ?
Al3 Y3 Al1 125.995(18) 3 4 ?
Al1 Y3 Al1 173.55(3) . 4 ?
Al1 Y3 Al1 97.87(2) 3 4 ?
Al1 Y3 Al1 44.922(11) 17_556 4 ?
Al1 Y3 Al1 98.55(3) 16_556 4 ?
Al1 Y3 Al1 44.922(11) 18_556 4 ?
Al1 Y3 Al1 97.87(2) 2 4 ?
Al1 Y3 Al1 77.15(3) 6 4 ?
Al1 Y3 Al1 137.802(15) 14 4 ?
Al1 Y3 Al1 87.90(4) 13 4 ?
Al1 Y3 Al1 137.802(15) 15 4 ?
Al1 Y3 Al1 77.15(3) 5 4 ?
Y2 Y3 Y2 0.0 16_556 4 ?
Al6 Y3 Y2 180.000(1) . 4 ?
Al6 Y3 Y2 0.000(2) 16_556 4 ?
Al7 Y3 Y2 0.0 4 4 ?
Al7 Y3 Y2 180.0 . 4 ?
Al6 Y3 Y2 0.000(1) 4 4 ?
Al6 Y3 Y2 180.0 13 4 ?
Al3 Y3 Y2 90.0 8 4 ?
Al3 Y3 Y2 90.0 2 4 ?
Al3 Y3 Y2 90.0 7 4 ?
Al3 Y3 Y2 90.0 . 4 ?
Al3 Y3 Y2 90.0 9 4 ?
Al3 Y3 Y2 90.0 3 4 ?
Al1 Y3 Y2 127.50(2) . 4 ?
Al1 Y3 Y2 127.50(2) 3 4 ?
Al1 Y3 Y2 52.50(2) 17_556 4 ?
Al1 Y3 Y2 52.50(2) 16_556 4 ?
Al1 Y3 Y2 52.50(2) 18_556 4 ?
Al1 Y3 Y2 127.50(2) 2 4 ?
Al1 Y3 Y2 46.05(2) 6 4 ?
Al1 Y3 Y2 133.95(2) 14 4 ?
Al1 Y3 Y2 133.95(2) 13 4 ?
Al1 Y3 Y2 133.95(2) 15 4 ?
Al1 Y3 Y2 46.05(2) 5 4 ?
Al1 Y3 Y2 46.05(2) 4 4 ?
Y2 Y3 Y2 180.000(3) 16_556 13 ?
Al6 Y3 Y2 0.0 . 13 ?
Al6 Y3 Y2 180.000(2) 16_556 13 ?
Al7 Y3 Y2 180.0 4 13 ?
Al7 Y3 Y2 0.0 . 13 ?
Al6 Y3 Y2 180.000(1) 4 13 ?
Al6 Y3 Y2 0.0 13 13 ?
Al3 Y3 Y2 90.0 8 13 ?
Al3 Y3 Y2 90.0 2 13 ?
Al3 Y3 Y2 90.0 7 13 ?
Al3 Y3 Y2 90.0 . 13 ?
Al3 Y3 Y2 90.0 9 13 ?
Al3 Y3 Y2 90.0 3 13 ?
Al1 Y3 Y2 52.50(2) . 13 ?
Al1 Y3 Y2 52.50(2) 3 13 ?
Al1 Y3 Y2 127.50(2) 17_556 13 ?
Al1 Y3 Y2 127.50(2) 16_556 13 ?
Al1 Y3 Y2 127.50(2) 18_556 13 ?
Al1 Y3 Y2 52.50(2) 2 13 ?
Al1 Y3 Y2 133.95(2) 6 13 ?
Al1 Y3 Y2 46.05(2) 14 13 ?
Al1 Y3 Y2 46.05(2) 13 13 ?
Al1 Y3 Y2 46.05(2) 15 13 ?
Al1 Y3 Y2 133.95(2) 5 13 ?
Al1 Y3 Y2 133.95(2) 4 13 ?
Y2 Y3 Y2 180.0 4 13 ?
Y2 Y3 Y3 0.000(2) 16_556 13_556 ?
Al6 Y3 Y3 180.0 . 13_556 ?
Al6 Y3 Y3 0.000(2) 16_556 13_556 ?
Al7 Y3 Y3 0.0 4 13_556 ?
Al7 Y3 Y3 180.0 . 13_556 ?
Al6 Y3 Y3 0.000(1) 4 13_556 ?
Al6 Y3 Y3 180.0 13 13_556 ?
Al3 Y3 Y3 90.0 8 13_556 ?
Al3 Y3 Y3 90.0 2 13_556 ?
Al3 Y3 Y3 90.0 7 13_556 ?
Al3 Y3 Y3 90.0 . 13_556 ?
Al3 Y3 Y3 90.0 9 13_556 ?
Al3 Y3 Y3 90.0 3 13_556 ?
Al1 Y3 Y3 127.50(2) . 13_556 ?
Al1 Y3 Y3 127.50(2) 3 13_556 ?
Al1 Y3 Y3 52.50(2) 17_556 13_556 ?
Al1 Y3 Y3 52.50(2) 16_556 13_556 ?
Al1 Y3 Y3 52.50(2) 18_556 13_556 ?
Al1 Y3 Y3 127.50(2) 2 13_556 ?
Al1 Y3 Y3 46.05(2) 6 13_556 ?
Al1 Y3 Y3 133.95(2) 14 13_556 ?
Al1 Y3 Y3 133.95(2) 13 13_556 ?
Al1 Y3 Y3 133.95(2) 15 13_556 ?
Al1 Y3 Y3 46.05(2) 5 13_556 ?
Al1 Y3 Y3 46.05(2) 4 13_556 ?
Y2 Y3 Y3 0.0 4 13_556 ?
Y2 Y3 Y3 180.0 13 13_556 ?
Y2 Y3 Y3 180.000(2) 16_556 13 ?
Al6 Y3 Y3 0.0 . 13 ?
Al6 Y3 Y3 180.000(2) 16_556 13 ?
Al7 Y3 Y3 180.0 4 13 ?
Al7 Y3 Y3 0.0 . 13 ?
Al6 Y3 Y3 180.000(1) 4 13 ?
Al6 Y3 Y3 0.0 13 13 ?
Al3 Y3 Y3 90.0 8 13 ?
Al3 Y3 Y3 90.0 2 13 ?
Al3 Y3 Y3 90.0 7 13 ?
Al3 Y3 Y3 90.0 . 13 ?
Al3 Y3 Y3 90.0 9 13 ?
Al3 Y3 Y3 90.0 3 13 ?
Al1 Y3 Y3 52.50(2) . 13 ?
Al1 Y3 Y3 52.50(2) 3 13 ?
Al1 Y3 Y3 127.50(2) 17_556 13 ?
Al1 Y3 Y3 127.50(2) 16_556 13 ?
Al1 Y3 Y3 127.50(2) 18_556 13 ?
Al1 Y3 Y3 52.50(2) 2 13 ?
Al1 Y3 Y3 133.95(2) 6 13 ?
Al1 Y3 Y3 46.05(2) 14 13 ?
Al1 Y3 Y3 46.05(2) 13 13 ?
Al1 Y3 Y3 46.05(2) 15 13 ?
Al1 Y3 Y3 133.95(2) 5 13 ?
Al1 Y3 Y3 133.95(2) 4 13 ?
Y2 Y3 Y3 180.0 4 13 ?
Y2 Y3 Y3 0.0 13 13 ?
Y3 Y3 Y3 180.0 13_556 13 ?
Y2 Y3 Y2 180.0 16_556 4_554 ?
Al6 Y3 Y2 0.0 . 4_554 ?
Al6 Y3 Y2 180.000(2) 16_556 4_554 ?
Al7 Y3 Y2 180.0 4 4_554 ?
Al7 Y3 Y2 0.0 . 4_554 ?
Al6 Y3 Y2 180.000(1) 4 4_554 ?
Al6 Y3 Y2 0.0 13 4_554 ?
Al3 Y3 Y2 90.0 8 4_554 ?
Al3 Y3 Y2 90.0 2 4_554 ?
Al3 Y3 Y2 90.0 7 4_554 ?
Al3 Y3 Y2 90.0 . 4_554 ?
Al3 Y3 Y2 90.0 9 4_554 ?
Al3 Y3 Y2 90.0 3 4_554 ?
Al1 Y3 Y2 52.50(2) . 4_554 ?
Al1 Y3 Y2 52.50(2) 3 4_554 ?
Al1 Y3 Y2 127.50(2) 17_556 4_554 ?
Al1 Y3 Y2 127.50(2) 16_556 4_554 ?
Al1 Y3 Y2 127.50(2) 18_556 4_554 ?
Al1 Y3 Y2 52.50(2) 2 4_554 ?
Al1 Y3 Y2 133.95(2) 6 4_554 ?
Al1 Y3 Y2 46.05(2) 14 4_554 ?
Al1 Y3 Y2 46.05(2) 13 4_554 ?
Al1 Y3 Y2 46.05(2) 15 4_554 ?
Al1 Y3 Y2 133.95(2) 5 4_554 ?
Al1 Y3 Y2 133.95(2) 4 4_554 ?
Y2 Y3 Y2 180.0 4 4_554 ?
Y2 Y3 Y2 0.0 13 4_554 ?
Y3 Y3 Y2 180.0 13_556 4_554 ?
Y3 Y3 Y2 0.0 13 4_554 ?
Al5 Os1 Al5 71.15(4) 15 14_565 ?
Al5 Os1 Al4 63.95(2) 15 . ?
Al5 Os1 Al4 66.88(3) 14_565 . ?
Al5 Os1 Al4 66.88(3) 15 20 ?
Al5 Os1 Al4 63.95(2) 14_565 20 ?
Al4 Os1 Al4 118.50(4) . 20 ?
Al5 Os1 Al3 110.681(19) 15 . ?
Al5 Os1 Al3 118.89(3) 14_565 . ?
Al4 Os1 Al3 61.86(3) . . ?
Al4 Os1 Al3 175.86(4) 20 . ?
Al5 Os1 Al3 118.89(3) 15 20 ?
Al5 Os1 Al3 110.682(19) 14_565 20 ?
Al4 Os1 Al3 175.86(4) . 20 ?
Al4 Os1 Al3 61.86(3) 20 20 ?
Al3 Os1 Al3 118.12(4) . 20 ?
Al5 Os1 Al1 114.88(3) 15 15 ?
Al5 Os1 Al1 171.74(3) 14_565 15 ?
Al4 Os1 Al1 120.42(4) . 15 ?
Al4 Os1 Al1 112.35(3) 20 15 ?
Al3 Os1 Al1 65.25(4) . 15 ?
Al3 Os1 Al1 61.78(3) 20 15 ?
Al5 Os1 Al1 171.74(3) 15 2 ?
Al5 Os1 Al1 114.88(3) 14_565 2 ?
Al4 Os1 Al1 112.35(3) . 2 ?
Al4 Os1 Al1 120.42(4) 20 2 ?
Al3 Os1 Al1 61.78(3) . 2 ?
Al3 Os1 Al1 65.25(4) 20 2 ?
Al1 Os1 Al1 59.77(4) 15 2 ?
Al5 Os1 Al2 61.97(3) 15 3_665 ?
Al5 Os1 Al2 127.96(3) 14_565 3_665 ?
Al4 Os1 Al2 73.02(4) . 3_665 ?
Al4 Os1 Al2 112.54(4) 20 3_665 ?
Al3 Os1 Al2 63.41(3) . 3_665 ?
Al3 Os1 Al2 110.84(3) 20 3_665 ?
Al1 Os1 Al2 60.02(3) 15 3_665 ?
Al1 Os1 Al2 110.17(3) 2 3_665 ?
Al5 Os1 Al2 127.96(3) 15 14_565 ?
Al5 Os1 Al2 61.97(3) 14_565 14_565 ?
Al4 Os1 Al2 112.54(4) . 14_565 ?
Al4 Os1 Al2 73.02(4) 20 14_565 ?
Al3 Os1 Al2 110.84(3) . 14_565 ?
Al3 Os1 Al2 63.41(3) 20 14_565 ?
Al1 Os1 Al2 110.17(3) 15 14_565 ?
Al1 Os1 Al2 60.02(3) 2 14_565 ?
Al2 Os1 Al2 169.76(4) 3_665 14_565 ?
Al5 Os1 Y1 66.521(16) 15 15 ?
Al5 Os1 Y1 118.159(15) 14_565 15 ?
Al4 Os1 Y1 124.17(4) . 15 ?
Al4 Os1 Y1 58.97(3) 20 15 ?
Al3 Os1 Y1 117.15(3) . 15 ?
Al3 Os1 Y1 59.82(3) 20 15 ?
Al1 Os1 Y1 62.06(2) 15 15 ?
Al1 Os1 Y1 112.97(3) 2 15 ?
Al2 Os1 Y1 61.97(3) 3_665 15 ?
Al2 Os1 Y1 117.50(3) 14_565 15 ?
Al5 Os1 Y1 118.158(15) 15 2 ?
Al5 Os1 Y1 66.521(16) 14_565 2 ?
Al4 Os1 Y1 58.97(3) . 2 ?
Al4 Os1 Y1 124.17(4) 20 2 ?
Al3 Os1 Y1 59.82(3) . 2 ?
Al3 Os1 Y1 117.15(3) 20 2 ?
Al1 Os1 Y1 112.97(3) 15 2 ?
Al1 Os1 Y1 62.06(2) 2 2 ?
Al2 Os1 Y1 117.50(3) 3_665 2 ?
Al2 Os1 Y1 61.97(3) 14_565 2 ?
Y1 Os1 Y1 174.821(14) 15 2 ?
Al5 Os1 Al2 73.243(18) 15 18_666 ?
Al5 Os1 Al2 112.175(14) 14_565 18_666 ?
Al4 Os1 Al2 45.79(4) . 18_666 ?
Al4 Os1 Al2 138.88(4) 20 18_666 ?
Al3 Os1 Al2 38.00(2) . 18_666 ?
Al3 Os1 Al2 137.02(2) 20 18_666 ?
Al1 Os1 Al2 75.61(3) 15 18_666 ?
Al1 Os1 Al2 98.83(3) 2 18_666 ?
Al2 Os1 Al2 34.43(3) 3_665 18_666 ?
Al2 Os1 Al2 144.59(3) 14_565 18_666 ?
Y1 Os1 Al2 96.394(18) 15 18_666 ?
Y1 Os1 Al2 83.321(19) 2 18_666 ?
Al5 Os1 Al2 112.174(14) 15 5_564 ?
Al5 Os1 Al2 73.243(18) 14_565 5_564 ?
Al4 Os1 Al2 138.88(4) . 5_564 ?
Al4 Os1 Al2 45.79(4) 20 5_564 ?
Al3 Os1 Al2 137.02(2) . 5_564 ?
Al3 Os1 Al2 38.00(2) 20 5_564 ?
Al1 Os1 Al2 98.83(3) 15 5_564 ?
Al1 Os1 Al2 75.61(3) 2 5_564 ?
Al2 Os1 Al2 144.59(3) 3_665 5_564 ?
Al2 Os1 Al2 34.43(3) 14_565 5_564 ?
Y1 Os1 Al2 83.321(19) 15 5_564 ?
Y1 Os1 Al2 96.394(18) 2 5_564 ?
Al2 Os1 Al2 173.72(3) 18_666 5_564 ?
Al5 Os1 Al3 98.84(2) 15 7 ?
Al5 Os1 Al3 148.081(11) 14_565 7 ?
Al4 Os1 Al3 81.41(3) . 7 ?
Al4 Os1 Al3 141.21(3) 20 7 ?
Al3 Os1 Al3 34.92(4) . 7 ?
Al3 Os1 Al3 100.74(2) 20 7 ?
Al1 Os1 Al3 39.01(3) 15 7 ?
Al1 Os1 Al3 73.05(2) 2 7 ?
Al2 Os1 Al3 37.65(2) 3_665 7 ?
Al2 Os1 Al3 132.97(2) 14_565 7 ?
Y1 Os1 Al3 82.243(16) 15 7 ?
Y1 Os1 Al3 94.548(17) 2 7 ?
Al2 Os1 Al3 37.297(13) 18_666 7 ?
Al2 Os1 Al3 136.718(16) 5_564 7 ?
Al5 Os1 Al3 148.081(11) 15 15 ?
Al5 Os1 Al3 98.84(2) 14_565 15 ?
Al4 Os1 Al3 141.21(3) . 15 ?
Al4 Os1 Al3 81.42(3) 20 15 ?
Al3 Os1 Al3 100.74(3) . 15 ?
Al3 Os1 Al3 34.92(4) 20 15 ?
Al1 Os1 Al3 73.05(2) 15 15 ?
Al1 Os1 Al3 39.01(3) 2 15 ?
Al2 Os1 Al3 132.98(2) 3_665 15 ?
Al2 Os1 Al3 37.65(2) 14_565 15 ?
Y1 Os1 Al3 94.549(17) 15 15 ?
Y1 Os1 Al3 82.242(16) 2 15 ?
Al2 Os1 Al3 136.718(16) 18_666 15 ?
Al2 Os1 Al3 37.297(13) 5_564 15 ?
Al3 Os1 Al3 103.918(19) 7 15 ?
Al5 Os1 Os1 90.0 15 16_556 ?
Al5 Os1 Os1 90.0 14_565 16_556 ?
Al4 Os1 Os1 30.854(19) . 16_556 ?
Al4 Os1 Os1 149.144(19) 20 16_556 ?
Al3 Os1 Os1 31.74(2) . 16_556 ?
Al3 Os1 Os1 148.26(2) 20 16_556 ?
Al1 Os1 Os1 95.52(3) 15 16_556 ?
Al1 Os1 Os1 84.48(3) 2 16_556 ?
Al2 Os1 Os1 69.52(2) 3_665 16_556 ?
Al2 Os1 Os1 110.48(2) 14_565 16_556 ?
Y1 Os1 Os1 131.465(8) 15 16_556 ?
Y1 Os1 Os1 48.535(8) 2 16_556 ?
Al2 Os1 Os1 35.086(12) 18_666 16_556 ?
Al2 Os1 Os1 144.914(12) 5_564 16_556 ?
Al3 Os1 Os1 59.128(11) 7 16_556 ?
Al3 Os1 Os1 120.872(11) 15 16_556 ?
Al5 Os1 Os1 90.0 15 16 ?
Al5 Os1 Os1 90.0 14_565 16 ?
Al4 Os1 Os1 149.145(19) . 16 ?
Al4 Os1 Os1 30.855(19) 20 16 ?
Al3 Os1 Os1 148.26(2) . 16 ?
Al3 Os1 Os1 31.74(2) 20 16 ?
Al1 Os1 Os1 84.48(3) 15 16 ?
Al1 Os1 Os1 95.52(3) 2 16 ?
Al2 Os1 Os1 110.48(2) 3_665 16 ?
Al2 Os1 Os1 69.52(2) 14_565 16 ?
Y1 Os1 Os1 48.537(8) 15 16 ?
Y1 Os1 Os1 131.463(8) 2 16 ?
Al2 Os1 Os1 144.915(12) 18_666 16 ?
Al2 Os1 Os1 35.085(12) 5_564 16 ?
Al3 Os1 Os1 120.873(11) 7 16 ?
Al3 Os1 Os1 59.128(11) 15 16 ?
Os1 Os1 Os1 180.0 16_556 16 ?
Al5 Os1 Al4 32.787(13) 15 19_665 ?
Al5 Os1 Al4 61.88(3) 14_565 19_665 ?
Al4 Os1 Al4 90.173(18) . 19_665 ?
Al4 Os1 Al4 34.12(4) 20 19_665 ?
Al3 Os1 Al4 143.447(19) . 19_665 ?
Al3 Os1 Al4 91.49(3) 20 19_665 ?
Al1 Os1 Al4 119.75(3) 15 19_665 ?
Al1 Os1 Al4 154.48(3) 2 19_665 ?
Al2 Os1 Al4 87.16(3) 3_665 19_665 ?
Al2 Os1 Al4 101.16(3) 14_565 19_665 ?
Y1 Os1 Al4 57.92(2) 15 19_665 ?
Y1 Os1 Al4 127.16(2) 2 19_665 ?
Al2 Os1 Al4 105.70(2) 18_666 19_665 ?
Al2 Os1 Al4 79.498(16) 5_564 19_665 ?
Al3 Os1 Al4 124.28(2) 7 19_665 ?
Al3 Os1 Al4 115.518(16) 15 19_665 ?
Os1 Os1 Al4 119.913(10) 16_556 19_665 ?
Os1 Os1 Al4 60.087(10) 16 19_665 ?
Al5 Os1 Al4 61.87(3) 15 3_565 ?
Al5 Os1 Al4 32.787(13) 14_565 3_565 ?
Al4 Os1 Al4 34.12(4) . 3_565 ?
Al4 Os1 Al4 90.172(19) 20 3_565 ?
Al3 Os1 Al4 91.49(3) . 3_565 ?
Al3 Os1 Al4 143.448(19) 20 3_565 ?
Al1 Os1 Al4 154.48(3) 15 3_565 ?
Al1 Os1 Al4 119.75(3) 2 3_565 ?
Al2 Os1 Al4 101.16(3) 3_665 3_565 ?
Al2 Os1 Al4 87.16(3) 14_565 3_565 ?
Y1 Os1 Al4 127.16(2) 15 3_565 ?
Y1 Os1 Al4 57.92(2) 2 3_565 ?
Al2 Os1 Al4 79.498(16) 18_666 3_565 ?
Al2 Os1 Al4 105.70(2) 5_564 3_565 ?
Al3 Os1 Al4 115.517(16) 7 3_565 ?
Al3 Os1 Al4 124.28(2) 15 3_565 ?
Os1 Os1 Al4 60.086(9) 16_556 3_565 ?
Os1 Os1 Al4 119.912(10) 16 3_565 ?
Al4 Os1 Al4 72.47(3) 19_665 3_565 ?
Al5 Os1 Os1 155.57(2) 15 15 ?
Al5 Os1 Os1 84.43(2) 14_565 15 ?
Al4 Os1 Os1 106.87(3) . 15 ?
Al4 Os1 Os1 102.77(4) 20 15 ?
Al3 Os1 Os1 80.77(2) . 15 ?
Al3 Os1 Os1 69.28(3) 20 15 ?
Al1 Os1 Os1 89.42(2) 15 15 ?
Al1 Os1 Os1 31.03(2) 2 15 ?
Al2 Os1 Os1 139.72(2) 3_665 15 ?
Al2 Os1 Os1 31.55(2) 14_565 15 ?
Y1 Os1 Os1 128.697(9) 15 15 ?
Y1 Os1 Os1 47.904(7) 2 15 ?
Al2 Os1 Os1 117.913(15) 18_666 15 ?
Al2 Os1 Os1 58.472(10) 5_564 15 ?
Al3 Os1 Os1 102.081(11) 7 15 ?
Al3 Os1 Os1 34.357(12) 15 15 ?
Os1 Os1 Os1 90.0 16_556 15 ?
Os1 Os1 Os1 90.0 16 15 ?
Al4 Os1 Os1 132.701(16) 19_665 15 ?
Al4 Os1 Os1 97.38(2) 3_565 15 ?
Al5 Os1 Al7 144.43(2) 15 . ?
Al5 Os1 Al7 144.43(2) 14_565 . ?
Al4 Os1 Al7 120.751(19) . . ?
Al4 Os1 Al7 120.75(2) 20 . ?
Al3 Os1 Al7 59.062(18) . . ?
Al3 Os1 Al7 59.062(18) 20 . ?
Al1 Os1 Al7 29.88(2) 15 . ?
Al1 Os1 Al7 29.88(2) 2 . ?
Al2 Os1 Al7 84.88(2) 3_665 . ?
Al2 Os1 Al7 84.88(2) 14_565 . ?
Y1 Os1 Al7 87.410(7) 15 . ?
Y1 Os1 Al7 87.410(7) 2 . ?
Al2 Os1 Al7 86.860(13) 18_666 . ?
Al2 Os1 Al7 86.860(13) 5_564 . ?
Al3 Os1 Al7 51.958(10) 7 . ?
Al3 Os1 Al7 51.959(10) 15 . ?
Os1 Os1 Al7 90.0 16_556 . ?
Os1 Os1 Al7 90.0 16 . ?
Al4 Os1 Al7 143.764(17) 19_665 . ?
Al4 Os1 Al7 143.764(17) 3_565 . ?
Os1 Os1 Al7 60.0 15 . ?
Al5 Os1 Os1 84.43(2) 15 14 ?
Al5 Os1 Os1 155.57(2) 14_565 14 ?
Al4 Os1 Os1 102.77(4) . 14 ?
Al4 Os1 Os1 106.87(3) 20 14 ?
Al3 Os1 Os1 69.28(3) . 14 ?
Al3 Os1 Os1 80.77(2) 20 14 ?
Al1 Os1 Os1 31.03(2) 15 14 ?
Al1 Os1 Os1 89.42(2) 2 14 ?
Al2 Os1 Os1 31.54(2) 3_665 14 ?
Al2 Os1 Os1 139.73(2) 14_565 14 ?
Y1 Os1 Os1 47.903(7) 15 14 ?
Y1 Os1 Os1 128.697(8) 2 14 ?
Al2 Os1 Os1 58.472(10) 18_666 14 ?
Al2 Os1 Os1 117.913(15) 5_564 14 ?
Al3 Os1 Os1 34.358(12) 7 14 ?
Al3 Os1 Os1 102.082(11) 15 14 ?
Os1 Os1 Os1 90.001(1) 16_556 14 ?
Os1 Os1 Os1 90.0 16 14 ?
Al4 Os1 Os1 97.38(2) 19_665 14 ?
Al4 Os1 Os1 132.700(16) 3_565 14 ?
Os1 Os1 Os1 120.0 15 14 ?
Al7 Os1 Os1 60.0 . 14 ?
Al5 Os1 Al4 33.043(13) 15 2_665 ?
Al5 Os1 Al4 59.70(2) 14_565 2_665 ?
Al4 Os1 Al4 31.69(2) . 2_665 ?
Al4 Os1 Al4 90.38(2) 20 2_665 ?
Al3 Os1 Al4 88.79(2) . 2_665 ?
Al3 Os1 Al4 150.44(2) 20 2_665 ?
Al1 Os1 Al4 128.48(3) 15 2_665 ?
Al1 Os1 Al4 144.02(3) 2 2_665 ?
Al2 Os1 Al4 68.66(3) 3_665 2_665 ?
Al2 Os1 Al4 120.75(3) 14_565 2_665 ?
Y1 Os1 Al4 98.318(15) 15 2_665 ?
Y1 Os1 Al4 85.982(14) 2 2_665 ?
Al2 Os1 Al4 58.89(2) 18_666 2_665 ?
Al2 Os1 Al4 127.38(2) 5_564 2_665 ?
Al3 Os1 Al4 95.04(2) 7 2_665 ?
Al3 Os1 Al4 158.35(2) 15 2_665 ?
Os1 Os1 Al4 60.912(11) 16_556 2_665 ?
Os1 Os1 Al4 119.087(11) 16 2_665 ?
Al4 Os1 Al4 59.042(16) 19_665 2_665 ?
Al4 Os1 Al4 35.193(17) 3_565 2_665 ?
Os1 Os1 Al4 131.385(12) 15 2_665 ?
Al7 Os1 Al4 145.637(16) . 2_665 ?
Os1 Os1 Al4 99.460(16) 14 2_665 ?
Al5 Os1 Al4 59.70(2) 15 21_565 ?
Al5 Os1 Al4 33.044(13) 14_565 21_565 ?
Al4 Os1 Al4 90.39(2) . 21_565 ?
Al4 Os1 Al4 31.69(2) 20 21_565 ?
Al3 Os1 Al4 150.44(2) . 21_565 ?
Al3 Os1 Al4 88.79(2) 20 21_565 ?
Al1 Os1 Al4 144.02(3) 15 21_565 ?
Al1 Os1 Al4 128.48(3) 2 21_565 ?
Al2 Os1 Al4 120.75(3) 3_665 21_565 ?
Al2 Os1 Al4 68.66(3) 14_565 21_565 ?
Y1 Os1 Al4 85.982(14) 15 21_565 ?
Y1 Os1 Al4 98.318(15) 2 21_565 ?
Al2 Os1 Al4 127.38(2) 18_666 21_565 ?
Al2 Os1 Al4 58.89(2) 5_564 21_565 ?
Al3 Os1 Al4 158.36(2) 7 21_565 ?
Al3 Os1 Al4 95.04(2) 15 21_565 ?
Os1 Os1 Al4 119.087(11) 16_556 21_565 ?
Os1 Os1 Al4 60.912(11) 16 21_565 ?
Al4 Os1 Al4 35.193(17) 19_665 21_565 ?
Al4 Os1 Al4 59.042(16) 3_565 21_565 ?
Os1 Os1 Al4 99.461(16) 15 21_565 ?
Al7 Os1 Al4 145.637(15) . 21_565 ?
Os1 Os1 Al4 131.385(12) 14 21_565 ?
Al4 Os1 Al4 68.73(3) 2_665 21_565 ?
Al5 Os1 Al6 143.18(5) 15 13 ?
Al5 Os1 Al6 143.18(5) 14_565 13 ?
Al4 Os1 Al6 130.93(17) . 13 ?
Al4 Os1 Al6 110.57(17) 20 13 ?
Al3 Os1 Al6 69.18(17) . 13 ?
Al3 Os1 Al6 48.96(17) 20 13 ?
Al1 Os1 Al6 29.50(3) 15 13 ?
Al1 Os1 Al6 33.25(8) 2 13 ?
Al2 Os1 Al6 88.51(7) 3_665 13 ?
Al2 Os1 Al6 81.38(6) 14_565 13 ?
Y1 Os1 Al6 80.70(11) 15 13 ?
Y1 Os1 Al6 94.17(11) 2 13 ?
Al2 Os1 Al6 95.22(14) 18_666 13 ?
Al2 Os1 Al6 78.54(14) 5_564 13 ?
Al3 Os1 Al6 58.96(12) 7 13 ?
Al3 Os1 Al6 45.79(10) 15 13 ?
Os1 Os1 Al6 100.20(17) 16_556 13 ?
Os1 Os1 Al6 79.80(17) 16 13 ?
Al4 Os1 Al6 134.88(16) 19_665 13 ?
Al4 Os1 Al6 151.90(13) 3_565 13 ?
Os1 Os1 Al6 60.520(18) 15 13 ?
Al7 Os1 Al6 10.20(17) . 13 ?
Os1 Os1 Al6 60.521(18) 14 13 ?
Al4 Os1 Al6 153.96(13) 2_665 13 ?
Al4 Os1 Al6 136.58(16) 21_565 13 ?
Al5 Os1 Al6 143.18(5) 15 . ?
Al5 Os1 Al6 143.18(5) 14_565 . ?
Al4 Os1 Al6 110.56(17) . . ?
Al4 Os1 Al6 130.94(17) 20 . ?
Al3 Os1 Al6 48.96(17) . . ?
Al3 Os1 Al6 69.18(17) 20 . ?
Al1 Os1 Al6 33.25(8) 15 . ?
Al1 Os1 Al6 29.50(3) 2 . ?
Al2 Os1 Al6 81.38(6) 3_665 . ?
Al2 Os1 Al6 88.51(7) 14_565 . ?
Y1 Os1 Al6 94.17(11) 15 . ?
Y1 Os1 Al6 80.70(11) 2 . ?
Al2 Os1 Al6 78.53(14) 18_666 . ?
Al2 Os1 Al6 95.22(14) 5_564 . ?
Al3 Os1 Al6 45.79(10) 7 . ?
Al3 Os1 Al6 58.96(12) 15 . ?
Os1 Os1 Al6 79.80(17) 16_556 . ?
Os1 Os1 Al6 100.20(17) 16 . ?
Al4 Os1 Al6 151.90(13) 19_665 . ?
Al4 Os1 Al6 134.88(16) 3_565 . ?
Os1 Os1 Al6 60.521(18) 15 . ?
Al7 Os1 Al6 10.20(17) . . ?
Os1 Os1 Al6 60.521(18) 14 . ?
Al4 Os1 Al6 136.58(16) 2_665 . ?
Al4 Os1 Al6 153.96(13) 21_565 . ?
Al6 Os1 Al6 20.4(3) 13 . ?
Al5 Os1 Al5 35.58(2) 15 13_665 ?
Al5 Os1 Al5 35.57(2) 14_565 13_665 ?
Al4 Os1 Al5 59.25(2) . 13_665 ?
Al4 Os1 Al5 59.25(2) 20 13_665 ?
Al3 Os1 Al5 120.938(18) . 13_665 ?
Al3 Os1 Al5 120.938(18) 20 13_665 ?
Al1 Os1 Al5 150.12(2) 15 13_665 ?
Al1 Os1 Al5 150.11(2) 2 13_665 ?
Al2 Os1 Al5 95.12(2) 3_665 13_665 ?
Al2 Os1 Al5 95.12(2) 14_565 13_665 ?
Y1 Os1 Al5 92.590(7) 15 13_665 ?
Y1 Os1 Al5 92.589(7) 2 13_665 ?
Al2 Os1 Al5 93.141(13) 18_666 13_665 ?
Al2 Os1 Al5 93.140(13) 5_564 13_665 ?
Al3 Os1 Al5 128.042(10) 7 13_665 ?
Al3 Os1 Al5 128.040(10) 15 13_665 ?
Os1 Os1 Al5 90.0 16_556 13_665 ?
Os1 Os1 Al5 90.0 16 13_665 ?
Al4 Os1 Al5 36.237(17) 19_665 13_665 ?
Al4 Os1 Al5 36.236(17) 3_565 13_665 ?
Os1 Os1 Al5 120.0 15 13_665 ?
Al7 Os1 Al5 180.0 . 13_665 ?
Os1 Os1 Al5 120.0 14 13_665 ?
Al4 Os1 Al5 34.364(16) 2_665 13_665 ?
Al4 Os1 Al5 34.363(15) 21_565 13_665 ?
Al6 Os1 Al5 169.80(17) 13 13_665 ?
Al6 Os1 Al5 169.80(17) . 13_665 ?
Al5 Os1 Al2 26.28(2) 15 15 ?
Al5 Os1 Al2 94.89(2) 14_565 15 ?
Al4 Os1 Al2 83.16(3) . 15 ?
Al4 Os1 Al2 66.98(4) 20 15 ?
Al3 Os1 Al2 109.29(2) . 15 ?
Al3 Os1 Al2 100.52(3) 20 15 ?
Al1 Os1 Al2 90.05(2) 15 15 ?
Al1 Os1 Al2 149.78(2) 2 15 ?
Al2 Os1 Al2 47.68(3) 3_665 15 ?
Al2 Os1 Al2 139.67(3) 14_565 15 ?
Y1 Os1 Al2 42.308(14) 15 15 ?
Y1 Os1 Al2 141.685(13) 2 15 ?
Al2 Os1 Al2 72.915(16) 18_666 15 ?
Al2 Os1 Al2 110.392(11) 5_564 15 ?
Al3 Os1 Al2 84.528(14) 7 15 ?
Al3 Os1 Al2 135.249(19) 15 15 ?
Os1 Os1 Al2 101.399(13) 16_556 15 ?
Os1 Os1 Al2 78.601(13) 16 15 ?
Al4 Os1 Al2 39.76(2) 19_665 15 ?
Al4 Os1 Al2 87.94(2) 3_565 15 ?
Os1 Os1 Al2 168.586(13) 15 15 ?
Al7 Os1 Al2 119.923(7) . 15 ?
Os1 Os1 Al2 61.224(6) 14 15 ?
Al4 Os1 Al2 56.102(16) 2_665 15 ?
Al4 Os1 Al2 74.583(17) 21_565 15 ?
Al6 Os1 Al2 117.13(6) 13 15 ?
Al6 Os1 Al2 121.73(2) . 15 ?
Al5 Os1 Al2 60.078(7) 13_665 15 ?
Al5 Os1 Al2 94.89(2) 15 2 ?
Al5 Os1 Al2 26.28(2) 14_565 2 ?
Al4 Os1 Al2 66.98(4) . 2 ?
Al4 Os1 Al2 83.16(3) 20 2 ?
Al3 Os1 Al2 100.52(3) . 2 ?
Al3 Os1 Al2 109.29(2) 20 2 ?
Al1 Os1 Al2 149.78(2) 15 2 ?
Al1 Os1 Al2 90.06(2) 2 2 ?
Al2 Os1 Al2 139.67(3) 3_665 2 ?
Al2 Os1 Al2 47.68(3) 14_565 2 ?
Y1 Os1 Al2 141.685(13) 15 2 ?
Y1 Os1 Al2 42.308(14) 2 2 ?
Al2 Os1 Al2 110.392(11) 18_666 2 ?
Al2 Os1 Al2 72.915(15) 5_564 2 ?
Al3 Os1 Al2 135.248(19) 7 2 ?
Al3 Os1 Al2 84.527(14) 15 2 ?
Os1 Os1 Al2 78.600(13) 16_556 2 ?
Os1 Os1 Al2 101.398(13) 16 2 ?
Al4 Os1 Al2 87.94(2) 19_665 2 ?
Al4 Os1 Al2 39.76(2) 3_565 2 ?
Os1 Os1 Al2 61.225(6) 15 2 ?
Al7 Os1 Al2 119.923(7) . 2 ?
Os1 Os1 Al2 168.586(13) 14 2 ?
Al4 Os1 Al2 74.583(17) 2_665 2 ?
Al4 Os1 Al2 56.102(16) 21_565 2 ?
Al6 Os1 Al2 121.73(2) 13 2 ?
Al6 Os1 Al2 117.13(6) . 2 ?
Al5 Os1 Al2 60.076(7) 13_665 2 ?
Al2 Os1 Al2 120.153(14) 15 2 ?
Al7 Al1 Os1 119.64(2) . 3 ?
Al7 Al1 Os1 119.64(2) . 14 ?
Os1 Al1 Os1 117.94(4) 3 14 ?
Al7 Al1 Al2 147.86(6) . 13_655 ?
Os1 Al1 Al2 60.26(2) 3 13_655 ?
Os1 Al1 Al2 60.26(2) 14 13_655 ?
Al7 Al1 Al1 59.528(4) . 14 ?
Os1 Al1 Al1 60.12(2) 3 14 ?
Os1 Al1 Al1 163.35(8) 14 14 ?
Al2 Al1 Al1 110.66(4) 13_655 14 ?
Al7 Al1 Al1 59.528(5) . 15 ?
Os1 Al1 Al1 163.35(8) 3 15 ?
Os1 Al1 Al1 60.12(2) 14 15 ?
Al2 Al1 Al1 110.66(4) 13_655 15 ?
Al1 Al1 Al1 116.37(3) 14 15 ?
Al7 Al1 Al6 17.9(3) . . ?
Os1 Al1 Al6 121.02(2) 3 . ?
Os1 Al1 Al6 121.02(2) 14 . ?
Al2 Al1 Al6 165.7(3) 13_655 . ?
Al1 Al1 Al6 63.99(10) 14 . ?
Al1 Al1 Al6 63.99(10) 15 . ?
Al7 Al1 Al3 94.54(4) . 7 ?
Os1 Al1 Al3 130.54(5) 3 7 ?
Os1 Al1 Al3 58.88(2) 14 7 ?
Al2 Al1 Al3 108.68(4) 13_655 7 ?
Al1 Al1 Al3 136.35(6) 14 7 ?
Al1 Al1 Al3 64.31(4) 15 7 ?
Al6 Al1 Al3 81.5(2) . 7 ?
Al7 Al1 Al3 94.54(4) . 3 ?
Os1 Al1 Al3 58.88(2) 3 3 ?
Os1 Al1 Al3 130.54(5) 14 3 ?
Al2 Al1 Al3 108.68(4) 13_655 3 ?
Al1 Al1 Al3 64.31(4) 14 3 ?
Al1 Al1 Al3 136.35(6) 15 3 ?
Al6 Al1 Al3 81.5(2) . 3 ?
Al3 Al1 Al3 85.81(5) 7 3 ?
Al7 Al1 Al6 16.9(3) . 13 ?
Os1 Al1 Al6 115.55(9) 3 13 ?
Os1 Al1 Al6 115.55(9) 14 13 ?
Al2 Al1 Al6 131.0(3) 13_655 13 ?
Al1 Al1 Al6 58.191(17) 14 13 ?
Al1 Al1 Al6 58.191(17) 15 13 ?
Al6 Al1 Al6 34.7(6) . 13 ?
Al3 Al1 Al6 106.67(19) 7 13 ?
Al3 Al1 Al6 106.67(19) 3 13 ?
Al7 Al1 Al3 91.39(4) . 14 ?
Os1 Al1 Al3 105.18(4) 3 14 ?
Os1 Al1 Al3 57.16(3) 14 14 ?
Al2 Al1 Al3 60.65(4) 13_655 14 ?
Al1 Al1 Al3 106.49(7) 14 14 ?
Al1 Al1 Al3 59.10(5) 15 14 ?
Al6 Al1 Al3 107.1(3) . 14 ?
Al3 Al1 Al3 108.75(3) 7 14 ?
Al3 Al1 Al3 163.81(4) 3 14 ?
Al6 Al1 Al3 76.5(2) 13 14 ?
Al7 Al1 Al3 91.39(4) . 21 ?
Os1 Al1 Al3 57.16(3) 3 21 ?
Os1 Al1 Al3 105.18(4) 14 21 ?
Al2 Al1 Al3 60.65(3) 13_655 21 ?
Al1 Al1 Al3 59.10(5) 14 21 ?
Al1 Al1 Al3 106.50(7) 15 21 ?
Al6 Al1 Al3 107.1(3) . 21 ?
Al3 Al1 Al3 163.81(4) 7 21 ?
Al3 Al1 Al3 108.75(3) 3 21 ?
Al6 Al1 Al3 76.5(2) 13 21 ?
Al3 Al1 Al3 55.97(5) 14 21 ?
Al7 Al1 Y2 38.61(7) . . ?
Os1 Al1 Y2 118.50(3) 3 . ?
Os1 Al1 Y2 118.50(3) 14 . ?
Al2 Al1 Y2 173.53(8) 13_655 . ?
Al1 Al1 Y2 72.16(4) 14 . ?
Al1 Al1 Y2 72.16(4) 15 . ?
Al6 Al1 Y2 20.8(3) . . ?
Al3 Al1 Y2 66.89(5) 7 . ?
Al3 Al1 Y2 66.89(5) 3 . ?
Al6 Al1 Y2 55.5(3) 13 . ?
Al3 Al1 Y2 124.73(7) 14 . ?
Al3 Al1 Y2 124.74(7) 21 . ?
Al7 Al1 Y1 146.86(5) . . ?
Os1 Al1 Y1 70.44(2) 3 . ?
Os1 Al1 Y1 70.44(2) 14 . ?
Al2 Al1 Y1 65.28(4) 13_655 . ?
Al1 Al1 Y1 120.22(4) 14 . ?
Al1 Al1 Y1 120.22(4) 15 . ?
Al6 Al1 Y1 129.0(3) . . ?
Al3 Al1 Y1 62.33(4) 7 . ?
Al3 Al1 Y1 62.33(4) 3 . ?
Al6 Al1 Y1 163.7(3) 13 . ?
Al3 Al1 Y1 117.54(4) 14 . ?
Al3 Al1 Y1 117.54(4) 21 . ?
Y2 Al1 Y1 108.25(8) . . ?
Al7 Al1 Y3 43.11(2) . . ?
Os1 Al1 Y3 117.41(2) 3 . ?
Os1 Al1 Y3 117.41(2) 14 . ?
Al2 Al1 Y3 169.02(5) 13_655 . ?
Al1 Al1 Y3 74.23(3) 14 . ?
Al1 Al1 Y3 74.23(3) 15 . ?
Al6 Al1 Y3 25.3(3) . . ?
Al3 Al1 Y3 63.90(3) 7 . ?
Al3 Al1 Y3 63.90(3) 3 . ?
Al6 Al1 Y3 60.0(3) 13 . ?
Al3 Al1 Y3 128.39(4) 14 . ?
Al3 Al1 Y3 128.39(4) 21 . ?
Y2 Al1 Y3 4.51(6) . . ?
Y1 Al1 Y3 103.74(4) . . ?
Al7 Al1 Y2 34.61(6) . 13 ?
Os1 Al1 Y2 108.94(4) 3 13 ?
Os1 Al1 Y2 108.94(4) 14 13 ?
Al2 Al1 Y2 113.25(7) 13_655 13 ?
Al1 Al1 Y2 60.05(3) 14 13 ?
Al1 Al1 Y2 60.05(3) 15 13 ?
Al6 Al1 Y2 52.5(3) . 13 ?
Al3 Al1 Y2 118.60(5) 7 13 ?
Al3 Al1 Y2 118.61(5) 3 13 ?
Al6 Al1 Y2 17.8(3) 13 13 ?
Al3 Al1 Y2 61.22(5) 14 13 ?
Al3 Al1 Y2 61.22(5) 21 13 ?
Y2 Al1 Y2 73.22(12) . 13 ?
Y1 Al1 Y2 178.53(7) . 13 ?
Y3 Al1 Y2 77.73(6) . 13 ?
Al7 Al1 Y2 47.14(6) . 16_556 ?
Os1 Al1 Y2 116.29(3) 3 16_556 ?
Os1 Al1 Y2 116.29(3) 14 16_556 ?
Al2 Al1 Y2 165.00(7) 13_655 16_556 ?
Al1 Al1 Y2 76.15(4) 14 16_556 ?
Al1 Al1 Y2 76.15(4) 15 16_556 ?
Al6 Al1 Y2 29.3(3) . 16_556 ?
Al3 Al1 Y2 61.32(4) 7 16_556 ?
Al3 Al1 Y2 61.32(4) 3 16_556 ?
Al6 Al1 Y2 64.0(3) 13 16_556 ?
Al3 Al1 Y2 131.57(5) 14 16_556 ?
Al3 Al1 Y2 131.57(5) 21 16_556 ?
Y2 Al1 Y2 8.53(12) . 16_556 ?
Y1 Al1 Y2 99.72(6) . 16_556 ?
Y3 Al1 Y2 4.02(5) . 16_556 ?
Y2 Al1 Y2 81.75(3) 13 16_556 ?
Al7 Al1 Y3 38.333(17) . 13 ?
Os1 Al1 Y3 107.33(3) 3 13 ?
Os1 Al1 Y3 107.33(3) 14 13 ?
Al2 Al1 Y3 109.53(5) 13_655 13 ?
Al1 Al1 Y3 60.85(3) 14 13 ?
Al1 Al1 Y3 60.85(3) 15 13 ?
Al6 Al1 Y3 56.2(3) . 13 ?
Al3 Al1 Y3 120.91(4) 7 13 ?
Al3 Al1 Y3 120.91(4) 3 13 ?
Al6 Al1 Y3 21.5(3) 13 13 ?
Al3 Al1 Y3 58.10(3) 14 13 ?
Al3 Al1 Y3 58.10(3) 21 13 ?
Y2 Al1 Y3 76.94(7) . 13 ?
Y1 Al1 Y3 174.81(4) . 13 ?
Y3 Al1 Y3 81.45(3) . 13 ?
Y2 Al1 Y3 3.72(5) 13 13 ?
Y2 Al1 Y3 85.47(6) 16_556 13 ?
Al7 Al1 Y2 41.64(5) . 4_554 ?
Os1 Al1 Y2 105.85(3) 3 4_554 ?
Os1 Al1 Y2 105.85(3) 14 4_554 ?
Al2 Al1 Y2 106.22(6) 13_655 4_554 ?
Al1 Al1 Y2 61.66(4) 14 4_554 ?
Al1 Al1 Y2 61.66(4) 15 4_554 ?
Al6 Al1 Y2 59.5(3) . 4_554 ?
Al3 Al1 Y2 122.89(5) 7 4_554 ?
Al3 Al1 Y2 122.89(5) 3 4_554 ?
Al6 Al1 Y2 24.8(3) 13 4_554 ?
Al3 Al1 Y2 55.36(4) 14 4_554 ?
Al3 Al1 Y2 55.36(4) 21 4_554 ?
Y2 Al1 Y2 80.25(4) . 4_554 ?
Y1 Al1 Y2 171.50(6) . 4_554 ?
Y3 Al1 Y2 84.76(5) . 4_554 ?
Y2 Al1 Y2 7.03(10) 13 4_554 ?
Y2 Al1 Y2 88.78(10) 16_556 4_554 ?
Y3 Al1 Y2 3.31(4) 13 4_554 ?
Al7 Al1 Al1 95.62(3) . 16_556 ?
Os1 Al1 Al1 95.52(3) 3 16_556 ?
Os1 Al1 Al1 95.52(3) 14 16_556 ?
Al2 Al1 Al1 116.52(4) 13_655 16_556 ?
Al1 Al1 Al1 101.13(5) 14 16_556 ?
Al1 Al1 Al1 101.13(5) 15 16_556 ?
Al6 Al1 Al1 77.8(3) . 16_556 ?
Al3 Al1 Al1 42.91(2) 7 16_556 ?
Al3 Al1 Al1 42.91(2) 3 16_556 ?
Al6 Al1 Al1 112.5(3) 13 16_556 ?
Al3 Al1 Al1 151.18(3) 14 16_556 ?
Al3 Al1 Al1 151.18(3) 21 16_556 ?
Y2 Al1 Al1 57.01(7) . 16_556 ?
Y1 Al1 Al1 51.24(2) . 16_556 ?
Y3 Al1 Al1 52.50(2) . 16_556 ?
Y2 Al1 Al1 130.23(6) 13 16_556 ?
Y2 Al1 Al1 48.48(6) 16_556 16_556 ?
Y3 Al1 Al1 133.95(2) 13 16_556 ?
Y2 Al1 Al1 137.26(5) 4_554 16_556 ?
Al7 Al1 Al6 58.42(12) . 16_556 ?
Os1 Al1 Al6 112.50(5) 3 16_556 ?
Os1 Al1 Al6 112.50(5) 14 16_556 ?
Al2 Al1 Al6 153.72(12) 13_655 16_556 ?
Al1 Al1 Al6 81.79(7) 14 16_556 ?
Al1 Al1 Al6 81.79(7) 15 16_556 ?
Al6 Al1 Al6 40.6(4) . 16_556 ?
Al3 Al1 Al6 54.63(7) 7 16_556 ?
Al3 Al1 Al6 54.63(7) 3 16_556 ?
Al6 Al1 Al6 75.27(15) 13 16_556 ?
Al3 Al1 Al6 139.88(9) 14 16_556 ?
Al3 Al1 Al6 139.88(9) 21 16_556 ?
Y2 Al1 Al6 19.81(13) . 16_556 ?
Y1 Al1 Al6 88.44(12) . 16_556 ?
Y3 Al1 Al6 15.31(11) . 16_556 ?
Y2 Al1 Al6 93.03(13) 13 16_556 ?
Y2 Al1 Al6 11.28(13) 16_556 16_556 ?
Y3 Al1 Al6 96.75(12) 13 16_556 ?
Y2 Al1 Al6 100.06(12) 4_554 16_556 ?
Al1 Al1 Al6 37.20(12) 16_556 16_556 ?
Al7 Al1 Al2 89.480(17) . 3_665 ?
Os1 Al1 Al2 150.87(4) 3 3_665 ?
Os1 Al1 Al2 35.024(12) 14 3_665 ?
Al2 Al1 Al2 95.24(2) 13_655 3_665 ?
Al1 Al1 Al2 149.003(17) 14 3_665 ?
Al1 Al1 Al2 34.80(3) 15 3_665 ?
Al6 Al1 Al2 86.74(5) . 3_665 ?
Al3 Al1 Al2 38.19(2) 7 3_665 ?
Al3 Al1 Al2 123.96(4) 3 3_665 ?
Al6 Al1 Al2 92.11(4) 13 3_665 ?
Al3 Al1 Al2 71.07(3) 14 3_665 ?
Al3 Al1 Al2 127.04(4) 21 3_665 ?
Y2 Al1 Al2 83.97(2) . 3_665 ?
Y1 Al1 Al2 85.509(19) . 3_665 ?
Y3 Al1 Al2 83.454(19) . 3_665 ?
Y2 Al1 Al2 94.69(2) 13 3_665 ?
Y2 Al1 Al2 83.03(2) 16_556 3_665 ?
Y3 Al1 Al2 95.183(19) 13 3_665 ?
Y2 Al1 Al2 95.60(2) 4_554 3_665 ?
Al1 Al1 Al2 81.06(2) 16_556 3_665 ?
Al6 Al1 Al2 82.03(2) 16_556 3_665 ?
Al7 Al1 Al2 89.480(17) . 2_545 ?
Os1 Al1 Al2 35.023(12) 3 2_545 ?
Os1 Al1 Al2 150.87(4) 14 2_545 ?
Al2 Al1 Al2 95.24(2) 13_655 2_545 ?
Al1 Al1 Al2 34.80(3) 14 2_545 ?
Al1 Al1 Al2 149.003(17) 15 2_545 ?
Al6 Al1 Al2 86.74(5) . 2_545 ?
Al3 Al1 Al2 123.96(4) 7 2_545 ?
Al3 Al1 Al2 38.19(2) 3 2_545 ?
Al6 Al1 Al2 92.11(4) 13 2_545 ?
Al3 Al1 Al2 127.04(4) 14 2_545 ?
Al3 Al1 Al2 71.07(3) 21 2_545 ?
Y2 Al1 Al2 83.97(2) . 2_545 ?
Y1 Al1 Al2 85.509(19) . 2_545 ?
Y3 Al1 Al2 83.454(19) . 2_545 ?
Y2 Al1 Al2 94.69(2) 13 2_545 ?
Y2 Al1 Al2 83.03(2) 16_556 2_545 ?
Y3 Al1 Al2 95.183(19) 13 2_545 ?
Y2 Al1 Al2 95.60(2) 4_554 2_545 ?
Al1 Al1 Al2 81.06(2) 16_556 2_545 ?
Al6 Al1 Al2 82.03(2) 16_556 2_545 ?
Al2 Al1 Al2 161.89(4) 3_665 2_545 ?
Al7 Al1 Al5 151.038(17) . . ?
Os1 Al1 Al5 86.69(3) 3 . ?
Os1 Al1 Al5 31.813(18) 14 . ?
Al2 Al1 Al5 35.14(2) 13_655 . ?
Al1 Al1 Al5 144.65(3) 14 . ?
Al1 Al1 Al5 91.728(14) 15 . ?
Al6 Al1 Al5 151.29(8) . . ?
Al3 Al1 Al5 73.82(3) 7 . ?
Al3 Al1 Al5 110.52(4) 3 . ?
Al6 Al1 Al5 142.70(17) 13 . ?
Al3 Al1 Al5 68.55(3) 14 . ?
Al3 Al1 Al5 93.90(3) 21 . ?
Y2 Al1 Al5 140.70(5) . . ?
Y1 Al1 Al5 49.187(17) . . ?
Y3 Al1 Al5 137.51(3) . . ?
Y2 Al1 Al5 129.65(5) 13 . ?
Y2 Al1 Al5 134.51(5) 16_556 . ?
Y3 Al1 Al5 126.63(3) 13 . ?
Y2 Al1 Al5 123.91(4) 4_554 . ?
Al1 Al1 Al5 93.335(16) 16_556 . ?
Al6 Al1 Al5 125.54(10) 16_556 . ?
Al2 Al1 Al5 64.800(15) 3_665 . ?
Al2 Al1 Al5 119.15(3) 2_545 . ?
Al7 Al1 Al5 151.037(17) . 13_655 ?
Os1 Al1 Al5 31.813(18) 3 13_655 ?
Os1 Al1 Al5 86.69(3) 14 13_655 ?
Al2 Al1 Al5 35.14(2) 13_655 13_655 ?
Al1 Al1 Al5 91.727(14) 14 13_655 ?
Al1 Al1 Al5 144.65(3) 15 13_655 ?
Al6 Al1 Al5 151.29(8) . 13_655 ?
Al3 Al1 Al5 110.52(4) 7 13_655 ?
Al3 Al1 Al5 73.81(3) 3 13_655 ?
Al6 Al1 Al5 142.70(17) 13 13_655 ?
Al3 Al1 Al5 93.91(3) 14 13_655 ?
Al3 Al1 Al5 68.55(3) 21 13_655 ?
Y2 Al1 Al5 140.70(5) . 13_655 ?
Y1 Al1 Al5 49.188(17) . 13_655 ?
Y3 Al1 Al5 137.51(3) . 13_655 ?
Y2 Al1 Al5 129.64(5) 13 13_655 ?
Y2 Al1 Al5 134.51(5) 16_556 13_655 ?
Y3 Al1 Al5 126.63(3) 13 13_655 ?
Y2 Al1 Al5 123.91(4) 4_554 13_655 ?
Al1 Al1 Al5 93.335(16) 16_556 13_655 ?
Al6 Al1 Al5 125.54(10) 16_556 13_655 ?
Al2 Al1 Al5 119.15(3) 3_665 13_655 ?
Al2 Al1 Al5 64.799(15) 2_545 13_655 ?
Al5 Al1 Al5 55.06(3) . 13_655 ?
Al7 Al1 Al4 126.97(3) . 7 ?
Os1 Al1 Al4 110.73(4) 3 7 ?
Os1 Al1 Al4 33.551(18) 14 7 ?
Al2 Al1 Al4 72.68(3) 13_655 7 ?
Al1 Al1 Al4 162.00(6) 14 7 ?
Al1 Al1 Al4 76.91(3) 15 7 ?
Al6 Al1 Al4 116.78(19) . 7 ?
Al3 Al1 Al4 36.01(3) 7 7 ?
Al3 Al1 Al4 97.72(4) 3 7 ?
Al6 Al1 Al4 133.71(8) 13 7 ?
Al3 Al1 Al4 90.66(3) 14 7 ?
Al3 Al1 Al4 131.42(4) 21 7 ?
Y2 Al1 Al4 102.81(5) . 7 ?
Y1 Al1 Al4 43.86(2) . 7 ?
Y3 Al1 Al4 99.62(3) . 7 ?
Y2 Al1 Al4 136.13(2) 13 7 ?
Y2 Al1 Al4 96.75(5) 16_556 7 ?
Y3 Al1 Al4 135.93(2) 13 7 ?
Y2 Al1 Al4 135.54(2) 4_554 7 ?
Al1 Al1 Al4 62.952(17) 16_556 7 ?
Al6 Al1 Al4 88.63(9) 16_556 7 ?
Al2 Al1 Al4 42.16(2) 3_665 7 ?
Al2 Al1 Al4 128.84(3) 2_545 7 ?
Al5 Al1 Al4 37.911(18) . 7 ?
Al5 Al1 Al4 81.46(3) 13_655 7 ?
Al7 Al1 Al4 126.97(3) . 3 ?
Os1 Al1 Al4 33.551(18) 3 3 ?
Os1 Al1 Al4 110.73(4) 14 3 ?
Al2 Al1 Al4 72.68(3) 13_655 3 ?
Al1 Al1 Al4 76.91(3) 14 3 ?
Al1 Al1 Al4 162.00(6) 15 3 ?
Al6 Al1 Al4 116.78(19) . 3 ?
Al3 Al1 Al4 97.72(4) 7 3 ?
Al3 Al1 Al4 36.00(3) 3 3 ?
Al6 Al1 Al4 133.71(8) 13 3 ?
Al3 Al1 Al4 131.43(4) 14 3 ?
Al3 Al1 Al4 90.65(3) 21 3 ?
Y2 Al1 Al4 102.81(5) . 3 ?
Y1 Al1 Al4 43.86(2) . 3 ?
Y3 Al1 Al4 99.62(3) . 3 ?
Y2 Al1 Al4 136.13(2) 13 3 ?
Y2 Al1 Al4 96.75(5) 16_556 3 ?
Y3 Al1 Al4 135.93(2) 13 3 ?
Y2 Al1 Al4 135.54(2) 4_554 3 ?
Al1 Al1 Al4 62.952(17) 16_556 3 ?
Al6 Al1 Al4 88.63(9) 16_556 3 ?
Al2 Al1 Al4 128.84(3) 3_665 3 ?
Al2 Al1 Al4 42.16(2) 2_545 3 ?
Al5 Al1 Al4 81.46(3) . 3 ?
Al5 Al1 Al4 37.910(18) 13_655 3 ?
Al4 Al1 Al4 87.71(5) 7 3 ?
Al7 Al1 Al3 61.64(2) . . ?
Os1 Al1 Al3 158.10(4) 3 . ?
Os1 Al1 Al3 71.789(16) 14 . ?
Al2 Al1 Al3 131.953(18) 13_655 . ?
Al1 Al1 Al3 116.50(3) 14 . ?
Al1 Al1 Al3 38.39(4) 15 . ?
Al6 Al1 Al3 52.73(13) . . ?
Al3 Al1 Al3 34.95(4) 7 . ?
Al3 Al1 Al3 99.55(4) 3 . ?
Al6 Al1 Al3 71.97(17) 13 . ?
Al3 Al1 Al3 96.53(3) 14 . ?
Al3 Al1 Al3 142.47(4) 21 . ?
Y2 Al1 Al3 46.879(17) . . ?
Y1 Al1 Al3 97.13(3) . . ?
Y3 Al1 Al3 46.459(15) . . ?
Y2 Al1 Al3 83.88(4) 13 . ?
Y2 Al1 Al3 46.367(14) 16_556 . ?
Y3 Al1 Al3 86.44(2) 13 . ?
Y2 Al1 Al3 88.72(4) 4_554 . ?
Al1 Al1 Al3 63.149(17) 16_556 . ?
Al6 Al1 Al3 47.53(3) 16_556 . ?
Al2 Al1 Al3 37.092(15) 3_665 . ?
Al2 Al1 Al3 129.18(3) 2_545 . ?
Al5 Al1 Al3 98.827(17) . . ?
Al5 Al1 Al3 145.33(3) 13_655 . ?
Al4 Al1 Al3 65.49(3) 7 . ?
Al4 Al1 Al3 126.02(3) 3 . ?
Al7 Al1 Al3 61.64(2) . 8 ?
Os1 Al1 Al3 71.789(16) 3 8 ?
Os1 Al1 Al3 158.10(4) 14 8 ?
Al2 Al1 Al3 131.953(18) 13_655 8 ?
Al1 Al1 Al3 38.39(4) 14 8 ?
Al1 Al1 Al3 116.50(3) 15 8 ?
Al6 Al1 Al3 52.73(13) . 8 ?
Al3 Al1 Al3 99.55(4) 7 8 ?
Al3 Al1 Al3 34.96(4) 3 8 ?
Al6 Al1 Al3 71.97(17) 13 8 ?
Al3 Al1 Al3 142.47(4) 14 8 ?
Al3 Al1 Al3 96.53(3) 21 8 ?
Y2 Al1 Al3 46.878(17) . 8 ?
Y1 Al1 Al3 97.13(3) . 8 ?
Y3 Al1 Al3 46.458(15) . 8 ?
Y2 Al1 Al3 83.88(4) 13 8 ?
Y2 Al1 Al3 46.367(14) 16_556 8 ?
Y3 Al1 Al3 86.44(2) 13 8 ?
Y2 Al1 Al3 88.72(4) 4_554 8 ?
Al1 Al1 Al3 63.149(17) 16_556 8 ?
Al6 Al1 Al3 47.53(3) 16_556 8 ?
Al2 Al1 Al3 129.18(3) 3_665 8 ?
Al2 Al1 Al3 37.092(15) 2_545 8 ?
Al5 Al1 Al3 145.33(3) . 8 ?
Al5 Al1 Al3 98.826(17) 13_655 8 ?
Al4 Al1 Al3 126.02(3) 7 8 ?
Al4 Al1 Al3 65.49(3) 3 8 ?
Al3 Al1 Al3 92.73(3) . 8 ?
Al7 Al1 Al2 116.37(4) . 4_654 ?
Os1 Al1 Al2 69.52(2) 3 4_654 ?
Os1 Al1 Al2 69.52(2) 14 4_654 ?
Al2 Al1 Al2 31.49(3) 13_655 4_654 ?
Al1 Al1 Al2 95.52(5) 14 4_654 ?
Al1 Al1 Al2 95.52(5) 15 4_654 ?
Al6 Al1 Al2 134.2(3) . 4_654 ?
Al3 Al1 Al2 128.11(3) 7 4_654 ?
Al3 Al1 Al2 128.11(3) 3 4_654 ?
Al6 Al1 Al2 99.5(3) 13 4_654 ?
Al3 Al1 Al2 36.71(3) 14 4_654 ?
Al3 Al1 Al2 36.71(3) 21 4_654 ?
Y2 Al1 Al2 154.98(8) . 4_654 ?
Y1 Al1 Al2 96.77(3) . 4_654 ?
Y3 Al1 Al2 159.49(4) . 4_654 ?
Y2 Al1 Al2 81.76(6) 13 4_654 ?
Y2 Al1 Al2 163.51(6) 16_556 4_654 ?
Y3 Al1 Al2 78.04(3) 13 4_654 ?
Y2 Al1 Al2 74.73(5) 4_554 4_654 ?
Al1 Al1 Al2 148.01(2) 16_556 4_654 ?
Al6 Al1 Al2 174.79(12) 16_556 4_654 ?
Al2 Al1 Al2 98.33(2) 3_665 4_654 ?
Al2 Al1 Al2 98.33(2) 2_545 4_654 ?
Al5 Al1 Al2 58.796(19) . 4_654 ?
Al5 Al1 Al2 58.796(19) 13_655 4_654 ?
Al4 Al1 Al2 95.12(3) 7 4_654 ?
Al4 Al1 Al2 95.12(3) 3 4_654 ?
Al3 Al1 Al2 131.259(16) . 4_654 ?
Al3 Al1 Al2 131.260(16) 8 4_654 ?
Al2 Al2 Al1 116.53(4) 16_556 13_655 ?
Al2 Al2 Os1 110.48(2) 16_556 2_655 ?
Al1 Al2 Os1 59.72(2) 13_655 2_655 ?
Al2 Al2 Os1 110.48(2) 16_556 15_655 ?
Al1 Al2 Os1 59.72(2) 13_655 15_655 ?
Os1 Al2 Os1 116.91(4) 2_655 15_655 ?
Al2 Al2 Al5 110.33(2) 16_556 . ?
Al1 Al2 Al5 110.10(3) 13_655 . ?
Os1 Al2 Al5 137.55(4) 2_655 . ?
Os1 Al2 Al5 56.813(14) 15_655 . ?
Al2 Al2 Al5 110.33(2) 16_556 13_655 ?
Al1 Al2 Al5 110.10(3) 13_655 13_655 ?
Os1 Al2 Al5 56.813(14) 2_655 13_655 ?
Os1 Al2 Al5 137.55(4) 15_655 13_655 ?
Al5 Al2 Al5 97.88(4) . 13_655 ?
Al2 Al2 Al3 61.94(2) 16_556 9_655 ?
Al1 Al2 Al3 63.10(4) 13_655 9_655 ?
Os1 Al2 Al3 106.60(4) 2_655 9_655 ?
Os1 Al2 Al3 57.82(3) 15_655 9_655 ?
Al5 Al2 Al3 102.36(3) . 9_655 ?
Al5 Al2 Al3 159.75(4) 13_655 9_655 ?
Al2 Al2 Al3 61.94(2) 16_556 2_655 ?
Al1 Al2 Al3 63.10(4) 13_655 2_655 ?
Os1 Al2 Al3 57.82(3) 2_655 2_655 ?
Os1 Al2 Al3 106.60(4) 15_655 2_655 ?
Al5 Al2 Al3 159.74(4) . 2_655 ?
Al5 Al2 Al3 102.37(3) 13_655 2_655 ?
Al3 Al2 Al3 57.38(5) 9_655 2_655 ?
Al2 Al2 Al4 65.33(2) 16_556 9_655 ?
Al1 Al2 Al4 103.63(3) 13_655 9_655 ?
Os1 Al2 Al4 160.13(4) 2_655 9_655 ?
Os1 Al2 Al4 52.73(2) 15_655 9_655 ?
Al5 Al2 Al4 55.273(19) . 9_655 ?
Al5 Al2 Al4 142.97(4) 13_655 9_655 ?
Al3 Al2 Al4 53.77(3) 9_655 9_655 ?
Al3 Al2 Al4 106.25(4) 2_655 9_655 ?
Al2 Al2 Al4 65.33(2) 16_556 2_655 ?
Al1 Al2 Al4 103.63(3) 13_655 2_655 ?
Os1 Al2 Al4 52.73(2) 2_655 2_655 ?
Os1 Al2 Al4 160.13(4) 15_655 2_655 ?
Al5 Al2 Al4 142.97(4) . 2_655 ?
Al5 Al2 Al4 55.27(2) 13_655 2_655 ?
Al3 Al2 Al4 106.26(4) 9_655 2_655 ?
Al3 Al2 Al4 53.77(3) 2_655 2_655 ?
Al4 Al2 Al4 130.21(5) 9_655 2_655 ?
Al2 Al2 Y1 178.23(2) 16_556 13_655 ?
Al1 Al2 Y1 65.24(4) 13_655 13_655 ?
Os1 Al2 Y1 70.26(2) 2_655 13_655 ?
Os1 Al2 Y1 70.26(2) 15_655 13_655 ?
Al5 Al2 Y1 68.63(2) . 13_655 ?
Al5 Al2 Y1 68.63(2) 13_655 13_655 ?
Al3 Al2 Y1 119.54(3) 9_655 13_655 ?
Al3 Al2 Y1 119.54(3) 2_655 13_655 ?
Al4 Al2 Y1 114.55(2) 9_655 13_655 ?
Al4 Al2 Y1 114.55(2) 2_655 13_655 ?
Al2 Al2 Y1 65.64(2) 16_556 . ?
Al1 Al2 Y1 177.84(5) 13_655 . ?
Os1 Al2 Y1 119.91(2) 2_655 . ?
Os1 Al2 Y1 119.91(2) 15_655 . ?
Al5 Al2 Y1 68.63(2) . . ?
Al5 Al2 Y1 68.62(2) 13_655 . ?
Al3 Al2 Y1 118.72(4) 9_655 . ?
Al3 Al2 Y1 118.72(4) 2_655 . ?
Al4 Al2 Y1 77.16(3) 9_655 . ?
Al4 Al2 Y1 77.16(3) 2_655 . ?
Y1 Al2 Y1 112.60(3) 13_655 . ?
Al2 Al2 Al2 121.93(4) 16_556 13_655 ?
Al1 Al2 Al2 121.54(6) 13_655 13_655 ?
Os1 Al2 Al2 98.34(3) 2_655 13_655 ?
Os1 Al2 Al2 98.34(3) 15_655 13_655 ?
Al5 Al2 Al2 48.94(2) . 13_655 ?
Al5 Al2 Al2 48.94(2) 13_655 13_655 ?
Al3 Al2 Al2 151.30(3) 9_655 13_655 ?
Al3 Al2 Al2 151.31(3) 2_655 13_655 ?
Al4 Al2 Al2 100.02(3) 9_655 13_655 ?
Al4 Al2 Al2 100.02(3) 2_655 13_655 ?
Y1 Al2 Al2 56.30(3) 13_655 13_655 ?
Y1 Al2 Al2 56.30(3) . 13_655 ?
Al2 Al2 Os1 35.085(12) 16_556 17_656 ?
Al1 Al2 Os1 98.74(3) 13_655 17_656 ?
Os1 Al2 Os1 75.40(2) 2_655 17_656 ?
Os1 Al2 Os1 129.73(3) 15_655 17_656 ?
Al5 Al2 Os1 144.25(3) . 17_656 ?
Al5 Al2 Os1 91.318(19) 13_655 17_656 ?
Al3 Al2 Os1 71.91(3) 9_655 17_656 ?
Al3 Al2 Os1 35.647(17) 2_655 17_656 ?
Al4 Al2 Os1 98.39(3) 9_655 17_656 ?
Al4 Al2 Os1 36.610(15) 2_655 17_656 ?
Y1 Al2 Os1 145.616(16) 13_655 17_656 ?
Y1 Al2 Os1 83.10(2) . 17_656 ?
Al2 Al2 Os1 129.44(3) 13_655 17_656 ?
Al2 Al2 Os1 35.086(12) 16_556 6_655 ?
Al1 Al2 Os1 98.74(3) 13_655 6_655 ?
Os1 Al2 Os1 129.73(3) 2_655 6_655 ?
Os1 Al2 Os1 75.40(2) 15_655 6_655 ?
Al5 Al2 Os1 91.318(19) . 6_655 ?
Al5 Al2 Os1 144.25(3) 13_655 6_655 ?
Al3 Al2 Os1 35.645(17) 9_655 6_655 ?
Al3 Al2 Os1 71.91(3) 2_655 6_655 ?
Al4 Al2 Os1 36.610(15) 9_655 6_655 ?
Al4 Al2 Os1 98.39(3) 2_655 6_655 ?
Y1 Al2 Os1 145.616(16) 13_655 6_655 ?
Y1 Al2 Os1 83.10(2) . 6_655 ?
Al2 Al2 Os1 129.45(3) 13_655 6_655 ?
Os1 Al2 Os1 63.06(2) 17_656 6_655 ?
Al2 Al2 Al5 35.305(15) 16_556 16_556 ?
Al1 Al2 Al5 132.21(3) 13_655 16_556 ?
Os1 Al2 Al5 144.61(3) 2_655 16_556 ?
Os1 Al2 Al5 91.324(19) 15_655 16_556 ?
Al5 Al2 Al5 75.02(2) . 16_556 ?
Al5 Al2 Al5 116.26(3) 13_655 16_556 ?
Al3 Al2 Al5 69.35(2) 9_655 16_556 ?
Al3 Al2 Al5 95.37(3) 2_655 16_556 ?
Al4 Al2 Al5 38.64(2) 9_655 16_556 ?
Al4 Al2 Al5 93.56(3) 2_655 16_556 ?
Y1 Al2 Al5 143.62(2) 13_655 16_556 ?
Y1 Al2 Al5 49.488(15) . 16_556 ?
Al2 Al2 Al5 98.05(4) 13_655 16_556 ?
Os1 Al2 Al5 69.95(2) 17_656 16_556 ?
Os1 Al2 Al5 34.021(10) 6_655 16_556 ?
Al2 Al2 Al5 35.306(15) 16_556 4_655 ?
Al1 Al2 Al5 132.21(3) 13_655 4_655 ?
Os1 Al2 Al5 91.324(19) 2_655 4_655 ?
Os1 Al2 Al5 144.61(3) 15_655 4_655 ?
Al5 Al2 Al5 116.26(3) . 4_655 ?
Al5 Al2 Al5 75.02(2) 13_655 4_655 ?
Al3 Al2 Al5 95.38(3) 9_655 4_655 ?
Al3 Al2 Al5 69.36(2) 2_655 4_655 ?
Al4 Al2 Al5 93.56(3) 9_655 4_655 ?
Al4 Al2 Al5 38.64(2) 2_655 4_655 ?
Y1 Al2 Al5 143.62(2) 13_655 4_655 ?
Y1 Al2 Al5 49.486(15) . 4_655 ?
Al2 Al2 Al5 98.05(4) 13_655 4_655 ?
Os1 Al2 Al5 34.022(10) 17_656 4_655 ?
Os1 Al2 Al5 69.95(2) 6_655 4_655 ?
Al5 Al2 Al5 55.39(3) 16_556 4_655 ?
Al2 Al2 Al1 98.94(2) 16_556 2_655 ?
Al1 Al2 Al1 34.54(3) 13_655 2_655 ?
Os1 Al2 Al1 93.24(3) 2_655 2_655 ?
Os1 Al2 Al1 34.80(2) 15_655 2_655 ?
Al5 Al2 Al1 91.58(2) . 2_655 ?
Al5 Al2 Al1 143.53(4) 13_655 2_655 ?
Al3 Al2 Al1 37.03(2) 9_655 2_655 ?
Al3 Al2 Al1 72.31(3) 2_655 2_655 ?
Al4 Al2 Al1 69.16(3) 9_655 2_655 ?
Al4 Al2 Al1 125.33(4) 2_655 2_655 ?
Y1 Al2 Al1 82.57(3) 13_655 2_655 ?
Y1 Al2 Al1 146.31(2) . 2_655 ?
Al2 Al2 Al1 129.29(4) 13_655 2_655 ?
Os1 Al2 Al1 101.26(3) 17_656 2_655 ?
Os1 Al2 Al1 69.93(2) 6_655 2_655 ?
Al5 Al2 Al1 100.21(2) 16_556 2_655 ?
Al5 Al2 Al1 130.98(3) 4_655 2_655 ?
Al2 Al2 Al1 98.95(2) 16_556 3_655 ?
Al1 Al2 Al1 34.54(3) 13_655 3_655 ?
Os1 Al2 Al1 34.81(2) 2_655 3_655 ?
Os1 Al2 Al1 93.24(3) 15_655 3_655 ?
Al5 Al2 Al1 143.53(4) . 3_655 ?
Al5 Al2 Al1 91.59(2) 13_655 3_655 ?
Al3 Al2 Al1 72.31(3) 9_655 3_655 ?
Al3 Al2 Al1 37.03(2) 2_655 3_655 ?
Al4 Al2 Al1 125.33(4) 9_655 3_655 ?
Al4 Al2 Al1 69.16(3) 2_655 3_655 ?
Y1 Al2 Al1 82.57(3) 13_655 3_655 ?
Y1 Al2 Al1 146.31(2) . 3_655 ?
Al2 Al2 Al1 129.29(4) 13_655 3_655 ?
Os1 Al2 Al1 69.93(2) 17_656 3_655 ?
Os1 Al2 Al1 101.26(3) 6_655 3_655 ?
Al5 Al2 Al1 130.98(3) 16_556 3_655 ?
Al5 Al2 Al1 100.21(2) 4_655 3_655 ?
Al1 Al2 Al1 61.98(3) 2_655 3_655 ?
Al2 Al2 Al3 136.666(19) 16_556 15_655 ?
Al1 Al2 Al3 36.09(2) 13_655 15_655 ?
Os1 Al2 Al3 84.04(3) 2_655 15_655 ?
Os1 Al2 Al3 34.375(17) 15_655 15_655 ?
Al5 Al2 Al3 74.29(2) . 15_655 ?
Al5 Al2 Al3 111.57(3) 13_655 15_655 ?
Al3 Al2 Al3 74.87(2) 9_655 15_655 ?
Al3 Al2 Al3 98.36(4) 2_655 15_655 ?
Al4 Al2 Al3 87.09(3) 9_655 15_655 ?
Al4 Al2 Al3 135.83(3) 2_655 15_655 ?
Y1 Al2 Al3 44.74(2) 13_655 15_655 ?
Y1 Al2 Al3 142.38(3) . 15_655 ?
Al2 Al2 Al3 94.22(4) 13_655 15_655 ?
Os1 Al2 Al3 133.45(3) 17_656 15_655 ?
Os1 Al2 Al3 104.18(2) 6_655 15_655 ?
Al5 Al2 Al3 125.620(18) 16_556 15_655 ?
Al5 Al2 Al3 167.39(3) 4_655 15_655 ?
Al1 Al2 Al3 38.15(2) 2_655 15_655 ?
Al1 Al2 Al3 69.49(2) 3_655 15_655 ?
Al2 Al2 Al3 136.666(19) 16_556 19_655 ?
Al1 Al2 Al3 36.09(2) 13_655 19_655 ?
Os1 Al2 Al3 34.376(17) 2_655 19_655 ?
Os1 Al2 Al3 84.04(3) 15_655 19_655 ?
Al5 Al2 Al3 111.57(3) . 19_655 ?
Al5 Al2 Al3 74.29(2) 13_655 19_655 ?
Al3 Al2 Al3 98.36(4) 9_655 19_655 ?
Al3 Al2 Al3 74.87(3) 2_655 19_655 ?
Al4 Al2 Al3 135.83(3) 9_655 19_655 ?
Al4 Al2 Al3 87.09(3) 2_655 19_655 ?
Y1 Al2 Al3 44.74(2) 13_655 19_655 ?
Y1 Al2 Al3 142.38(3) . 19_655 ?
Al2 Al2 Al3 94.23(4) 13_655 19_655 ?
Os1 Al2 Al3 104.18(2) 17_656 19_655 ?
Os1 Al2 Al3 133.44(3) 6_655 19_655 ?
Al5 Al2 Al3 167.39(3) 16_556 19_655 ?
Al5 Al2 Al3 125.621(18) 4_655 19_655 ?
Al1 Al2 Al3 69.48(2) 2_655 19_655 ?
Al1 Al2 Al3 38.15(2) 3_655 19_655 ?
Al3 Al2 Al3 50.09(2) 15_655 19_655 ?
Al2 Al2 Al4 136.342(18) 16_556 19_655 ?
Al1 Al2 Al4 71.99(3) 13_655 19_655 ?
Os1 Al2 Al4 33.36(2) 2_655 19_655 ?
Os1 Al2 Al4 109.94(3) 15_655 19_655 ?
Al5 Al2 Al4 105.09(4) . 19_655 ?
Al5 Al2 Al4 38.699(18) 13_655 19_655 ?
Al3 Al2 Al4 133.09(4) 9_655 19_655 ?
Al3 Al2 Al4 91.17(3) 2_655 19_655 ?
Al4 Al2 Al4 157.99(4) 9_655 19_655 ?
Al4 Al2 Al4 71.037(18) 2_655 19_655 ?
Y1 Al2 Al4 43.647(18) 13_655 19_655 ?
Y1 Al2 Al4 106.51(3) . 19_655 ?
Al2 Al2 Al4 66.68(3) 13_655 19_655 ?
Os1 Al2 Al4 103.58(2) 17_656 19_655 ?
Os1 Al2 Al4 163.07(3) 6_655 19_655 ?
Al5 Al2 Al4 154.93(3) 16_556 19_655 ?
Al5 Al2 Al4 105.33(2) 4_655 19_655 ?
Al1 Al2 Al4 104.84(3) 2_655 19_655 ?
Al1 Al2 Al4 62.95(3) 3_655 19_655 ?
Al3 Al2 Al4 76.96(3) 15_655 19_655 ?
Al3 Al2 Al4 35.91(2) 19_655 19_655 ?
Al2 Al2 Al4 136.342(18) 16_556 15_655 ?
Al1 Al2 Al4 71.99(3) 13_655 15_655 ?
Os1 Al2 Al4 109.94(3) 2_655 15_655 ?
Os1 Al2 Al4 33.36(2) 15_655 15_655 ?
Al5 Al2 Al4 38.697(18) . 15_655 ?
Al5 Al2 Al4 105.09(4) 13_655 15_655 ?
Al3 Al2 Al4 91.17(3) 9_655 15_655 ?
Al3 Al2 Al4 133.09(4) 2_655 15_655 ?
Al4 Al2 Al4 71.037(18) 9_655 15_655 ?
Al4 Al2 Al4 157.99(4) 2_655 15_655 ?
Y1 Al2 Al4 43.647(18) 13_655 15_655 ?
Y1 Al2 Al4 106.51(3) . 15_655 ?
Al2 Al2 Al4 66.68(3) 13_655 15_655 ?
Os1 Al2 Al4 163.07(3) 17_656 15_655 ?
Os1 Al2 Al4 103.58(2) 6_655 15_655 ?
Al5 Al2 Al4 105.33(2) 16_556 15_655 ?
Al5 Al2 Al4 154.93(3) 4_655 15_655 ?
Al1 Al2 Al4 62.95(3) 2_655 15_655 ?
Al1 Al2 Al4 104.84(3) 3_655 15_655 ?
Al3 Al2 Al4 35.91(2) 15_655 15_655 ?
Al3 Al2 Al4 76.96(3) 19_655 15_655 ?
Al4 Al2 Al4 87.29(4) 19_655 15_655 ?
Al2 Al2 Al4 72.707(16) 16_556 3 ?
Al1 Al2 Al4 136.553(15) 13_655 3 ?
Os1 Al2 Al4 77.079(15) 2_655 3 ?
Os1 Al2 Al4 161.33(3) 15_655 3 ?
Al5 Al2 Al4 104.58(3) . 3 ?
Al5 Al2 Al4 38.335(17) 13_655 3 ?
Al3 Al2 Al4 132.92(4) 9_655 3 ?
Al3 Al2 Al4 91.22(3) 2_655 3 ?
Al4 Al2 Al4 117.56(3) 9_655 3 ?
Al4 Al2 Al4 38.40(3) 2_655 3 ?
Y1 Al2 Al4 106.06(2) 13_655 3 ?
Y1 Al2 Al4 43.395(15) . 3 ?
Al2 Al2 Al4 66.08(3) 13_655 3 ?
Os1 Al2 Al4 63.624(14) 17_656 3 ?
Os1 Al2 Al4 105.92(3) 6_655 3 ?
Al5 Al2 Al4 81.31(2) 16_556 3 ?
Al5 Al2 Al4 37.845(12) 4_655 3 ?
Al1 Al2 Al4 163.53(3) 2_655 3 ?
Al1 Al2 Al4 104.563(19) 3_655 3 ?
Al3 Al2 Al4 149.90(3) 15_655 3 ?
Al3 Al2 Al4 106.470(17) 19_655 3 ?
Al4 Al2 Al4 74.37(2) 19_655 3 ?
Al4 Al2 Al4 132.76(3) 15_655 3 ?
Al2 Al2 Al4 72.707(16) 16_556 7 ?
Al1 Al2 Al4 136.553(15) 13_655 7 ?
Os1 Al2 Al4 161.33(3) 2_655 7 ?
Os1 Al2 Al4 77.080(15) 15_655 7 ?
Al5 Al2 Al4 38.337(17) . 7 ?
Al5 Al2 Al4 104.58(3) 13_655 7 ?
Al3 Al2 Al4 91.22(3) 9_655 7 ?
Al3 Al2 Al4 132.92(4) 2_655 7 ?
Al4 Al2 Al4 38.40(3) 9_655 7 ?
Al4 Al2 Al4 117.56(3) 2_655 7 ?
Y1 Al2 Al4 106.06(2) 13_655 7 ?
Y1 Al2 Al4 43.395(15) . 7 ?
Al2 Al2 Al4 66.08(3) 13_655 7 ?
Os1 Al2 Al4 105.92(3) 17_656 7 ?
Os1 Al2 Al4 63.625(14) 6_655 7 ?
Al5 Al2 Al4 37.847(12) 16_556 7 ?
Al5 Al2 Al4 81.31(2) 4_655 7 ?
Al1 Al2 Al4 104.563(19) 2_655 7 ?
Al1 Al2 Al4 163.53(3) 3_655 7 ?
Al3 Al2 Al4 106.470(17) 15_655 7 ?
Al3 Al2 Al4 149.90(3) 19_655 7 ?
Al4 Al2 Al4 132.76(3) 19_655 7 ?
Al4 Al2 Al4 74.37(2) 15_655 7 ?
Al4 Al2 Al4 86.79(3) 3 7 ?
Al2 Al2 Al1 31.99(2) 16_556 4_655 ?
Al1 Al2 Al1 84.54(5) 13_655 4_655 ?
Os1 Al2 Al1 95.21(3) 2_655 4_655 ?
Os1 Al2 Al1 95.21(3) 15_655 4_655 ?
Al5 Al2 Al1 126.15(2) . 4_655 ?
Al5 Al2 Al1 126.15(2) 13_655 4_655 ?
Al3 Al2 Al1 37.70(2) 9_655 4_655 ?
Al3 Al2 Al1 37.71(2) 2_655 4_655 ?
Al4 Al2 Al1 71.04(2) 9_655 4_655 ?
Al4 Al2 Al1 71.04(2) 2_655 4_655 ?
Y1 Al2 Al1 149.78(4) 13_655 4_655 ?
Y1 Al2 Al1 97.62(3) . 4_655 ?
Al2 Al2 Al1 153.92(5) 13_655 4_655 ?
Os1 Al2 Al1 34.868(12) 17_656 4_655 ?
Os1 Al2 Al1 34.867(12) 6_655 4_655 ?
Al5 Al2 Al1 59.32(2) 16_556 4_655 ?
Al5 Al2 Al1 59.32(2) 4_655 4_655 ?
Al1 Al2 Al1 71.66(2) 2_655 4_655 ?
Al1 Al2 Al1 71.66(2) 3_655 4_655 ?
Al3 Al2 Al1 109.32(3) 15_655 4_655 ?
Al3 Al2 Al1 109.32(3) 19_655 4_655 ?
Al4 Al2 Al1 128.45(3) 19_655 4_655 ?
Al4 Al2 Al1 128.45(3) 15_655 4_655 ?
Al4 Al2 Al1 95.69(2) 3 4_655 ?
Al4 Al2 Al1 95.69(2) 7 4_655 ?
Al2 Al2 Al5 101.488(13) 16_556 15_545 ?
Al1 Al2 Al5 85.070(17) 13_655 15_545 ?
Os1 Al2 Al5 25.373(11) 2_655 15_545 ?
Os1 Al2 Al5 140.06(3) 15_655 15_545 ?
Al5 Al2 Al5 131.90(3) . 15_545 ?
Al5 Al2 Al5 35.91(2) 13_655 15_545 ?
Al3 Al2 Al5 124.52(4) 9_655 15_545 ?
Al3 Al2 Al5 68.02(3) 2_655 15_545 ?
Al4 Al2 Al5 166.37(3) 9_655 15_545 ?
Al4 Al2 Al5 36.297(17) 2_655 15_545 ?
Y1 Al2 Al5 78.511(13) 13_655 15_545 ?
Y1 Al2 Al5 94.537(16) . 15_545 ?
Al2 Al2 Al5 83.789(17) 13_655 15_545 ?
Os1 Al2 Al5 69.595(12) 17_656 15_545 ?
Os1 Al2 Al5 132.55(2) 6_655 15_545 ?
Al5 Al2 Al5 128.08(2) 16_556 15_545 ?
Al5 Al2 Al5 72.900(17) 4_655 15_545 ?
Al1 Al2 Al5 118.45(3) 2_655 15_545 ?
Al1 Al2 Al5 57.811(19) 3_655 15_545 ?
Al3 Al2 Al5 105.77(2) 15_655 15_545 ?
Al3 Al2 Al5 56.090(13) 19_655 15_545 ?
Al4 Al2 Al5 34.866(15) 19_655 15_545 ?
Al4 Al2 Al5 122.15(3) 15_655 15_545 ?
Al4 Al2 Al5 51.955(14) 3 15_545 ?
Al4 Al2 Al5 136.90(3) 7 15_545 ?
Al1 Al2 Al5 99.829(15) 4_655 15_545 ?
Al2 Al2 Al5 101.488(13) 16_556 2_655 ?
Al1 Al2 Al5 85.071(17) 13_655 2_655 ?
Os1 Al2 Al5 140.07(3) 2_655 2_655 ?
Os1 Al2 Al5 25.376(11) 15_655 2_655 ?
Al5 Al2 Al5 35.90(2) . 2_655 ?
Al5 Al2 Al5 131.90(3) 13_655 2_655 ?
Al3 Al2 Al5 68.02(3) 9_655 2_655 ?
Al3 Al2 Al5 124.52(4) 2_655 2_655 ?
Al4 Al2 Al5 36.297(17) 9_655 2_655 ?
Al4 Al2 Al5 166.37(3) 2_655 2_655 ?
Y1 Al2 Al5 78.512(13) 13_655 2_655 ?
Y1 Al2 Al5 94.536(16) . 2_655 ?
Al2 Al2 Al5 83.788(17) 13_655 2_655 ?
Os1 Al2 Al5 132.55(2) 17_656 2_655 ?
Os1 Al2 Al5 69.595(11) 6_655 2_655 ?
Al5 Al2 Al5 72.899(17) 16_556 2_655 ?
Al5 Al2 Al5 128.08(2) 4_655 2_655 ?
Al1 Al2 Al5 57.812(19) 2_655 2_655 ?
Al1 Al2 Al5 118.46(3) 3_655 2_655 ?
Al3 Al2 Al5 56.090(13) 15_655 2_655 ?
Al3 Al2 Al5 105.77(2) 19_655 2_655 ?
Al4 Al2 Al5 122.15(3) 19_655 2_655 ?
Al4 Al2 Al5 34.867(15) 15_655 2_655 ?
Al4 Al2 Al5 136.90(3) 3 2_655 ?
Al4 Al2 Al5 51.954(14) 7 2_655 ?
Al1 Al2 Al5 99.829(15) 4_655 2_655 ?
Al5 Al2 Al5 157.02(3) 15_545 2_655 ?
Al2 Al2 Os1 101.398(13) 16_556 14 ?
Al1 Al2 Os1 132.52(3) 13_655 14 ?
Os1 Al2 Os1 132.32(3) 2_655 14 ?
Os1 Al2 Os1 81.532(17) 15_655 14 ?
Al5 Al2 Os1 24.818(15) . 14 ?
Al5 Al2 Os1 79.53(3) 13_655 14 ?
Al3 Al2 Os1 119.61(3) 9_655 14 ?
Al3 Al2 Os1 163.01(4) 2_655 14 ?
Al4 Al2 Os1 66.35(2) 9_655 14 ?
Al4 Al2 Os1 118.17(3) 2_655 14 ?
Y1 Al2 Os1 77.06(2) 13_655 14 ?
Y1 Al2 Os1 45.865(14) . 14 ?
Al2 Al2 Os1 33.978(14) 13_655 14 ?
Os1 Al2 Os1 128.11(2) 17_656 14 ?
Os1 Al2 Os1 96.535(14) 6_655 14 ?
Al5 Al2 Os1 69.158(16) 16_556 14 ?
Al5 Al2 Os1 95.26(2) 4_655 14 ?
Al1 Al2 Os1 116.187(17) 2_655 14 ?
Al1 Al2 Os1 159.56(3) 3_655 14 ?
Al3 Al2 Os1 96.53(2) 15_655 14 ?
Al3 Al2 Os1 121.42(3) 19_655 14 ?
Al4 Al2 Os1 100.13(3) 19_655 14 ?
Al4 Al2 Os1 60.755(19) 15_655 14 ?
Al4 Al2 Os1 79.82(2) 3 14 ?
Al4 Al2 Os1 33.051(12) 7 14 ?
Al1 Al2 Os1 128.31(2) 4_655 14 ?
Al5 Al2 Os1 115.44(2) 15_545 14 ?
Al5 Al2 Os1 59.071(12) 2_655 14 ?
Al2 Al2 Os1 101.398(13) 16_556 3 ?
Al1 Al2 Os1 132.52(3) 13_655 3 ?
Os1 Al2 Os1 81.531(17) 2_655 3 ?
Os1 Al2 Os1 132.32(3) 15_655 3 ?
Al5 Al2 Os1 79.53(3) . 3 ?
Al5 Al2 Os1 24.816(15) 13_655 3 ?
Al3 Al2 Os1 163.01(4) 9_655 3 ?
Al3 Al2 Os1 119.62(3) 2_655 3 ?
Al4 Al2 Os1 118.17(3) 9_655 3 ?
Al4 Al2 Os1 66.35(2) 2_655 3 ?
Y1 Al2 Os1 77.06(2) 13_655 3 ?
Y1 Al2 Os1 45.864(14) . 3 ?
Al2 Al2 Os1 33.978(14) 13_655 3 ?
Os1 Al2 Os1 96.534(14) 17_656 3 ?
Os1 Al2 Os1 128.11(2) 6_655 3 ?
Al5 Al2 Os1 95.26(2) 16_556 3 ?
Al5 Al2 Os1 69.156(16) 4_655 3 ?
Al1 Al2 Os1 159.56(3) 2_655 3 ?
Al1 Al2 Os1 116.188(17) 3_655 3 ?
Al3 Al2 Os1 121.42(3) 15_655 3 ?
Al3 Al2 Os1 96.530(19) 19_655 3 ?
Al4 Al2 Os1 60.756(19) 19_655 3 ?
Al4 Al2 Os1 100.13(3) 15_655 3 ?
Al4 Al2 Os1 33.051(12) 3 3 ?
Al4 Al2 Os1 79.82(2) 7 3 ?
Al1 Al2 Os1 128.31(2) 4_655 3 ?
Al5 Al2 Os1 59.072(12) 15_545 3 ?
Al5 Al2 Os1 115.43(2) 2_655 3 ?
Os1 Al2 Os1 57.550(13) 14 3 ?
Os1 Al3 Os1 116.51(4) . 16_556 ?
Os1 Al3 Al3 110.72(3) . 7 ?
Os1 Al3 Al3 110.72(3) 16_556 7 ?
Os1 Al3 Al4 58.62(2) . . ?
Os1 Al3 Al4 58.62(2) 16_556 . ?
Al3 Al3 Al4 124.04(4) 7 . ?
Os1 Al3 Al1 59.34(3) . 2 ?
Os1 Al3 Al1 137.37(5) 16_556 2 ?
Al3 Al3 Al1 109.50(4) 7 2 ?
Al4 Al3 Al1 107.74(5) . 2 ?
Os1 Al3 Al1 137.37(5) . 17_556 ?
Os1 Al3 Al1 59.34(3) 16_556 17_556 ?
Al3 Al3 Al1 109.50(4) 7 17_556 ?
Al4 Al3 Al1 107.74(5) . 17_556 ?
Al1 Al3 Al1 94.18(5) 2 17_556 ?
Os1 Al3 Al2 106.35(3) . 18_666 ?
Os1 Al3 Al2 58.77(2) 16_556 18_666 ?
Al3 Al3 Al2 61.31(3) 7 18_666 ?
Al4 Al3 Al2 69.83(4) . 18_666 ?
Al1 Al3 Al2 160.76(4) 2 18_666 ?
Al1 Al3 Al2 104.78(3) 17_556 18_666 ?
Os1 Al3 Al2 58.77(2) . 3_665 ?
Os1 Al3 Al2 106.35(3) 16_556 3_665 ?
Al3 Al3 Al2 61.31(3) 7 3_665 ?
Al4 Al3 Al2 69.83(4) . 3_665 ?
Al1 Al3 Al2 104.78(3) 2 3_665 ?
Al1 Al3 Al2 160.76(4) 17_556 3_665 ?
Al2 Al3 Al2 56.11(5) 18_666 3_665 ?
Os1 Al3 Al1 57.59(2) . 15 ?
Os1 Al3 Al1 162.58(4) 16_556 15 ?
Al3 Al3 Al1 62.02(3) 7 15 ?
Al4 Al3 Al1 110.75(3) . 15 ?
Al1 Al3 Al1 56.59(3) 2 15 ?
Al1 Al3 Al1 137.12(5) 17_556 15 ?
Al2 Al3 Al1 105.58(4) 18_666 15 ?
Al2 Al3 Al1 56.25(3) 3_665 15 ?
Os1 Al3 Al1 162.58(4) . 6 ?
Os1 Al3 Al1 57.59(2) 16_556 6 ?
Al3 Al3 Al1 62.02(3) 7 6 ?
Al4 Al3 Al1 110.75(3) . 6 ?
Al1 Al3 Al1 137.12(5) 2 6 ?
Al1 Al3 Al1 56.59(3) 17_556 6 ?
Al2 Al3 Al1 56.25(3) 18_666 6 ?
Al2 Al3 Al1 105.58(4) 3_665 6 ?
Al1 Al3 Al1 122.36(5) 15 6 ?
Os1 Al3 Y1 72.30(3) . 2 ?
Os1 Al3 Y1 72.30(3) 16_556 2 ?
Al3 Al3 Y1 173.040(15) 7 2 ?
Al4 Al3 Y1 62.92(4) . 2 ?
Al1 Al3 Y1 66.21(3) 2 2 ?
Al1 Al3 Y1 66.21(3) 17_556 2 ?
Al2 Al3 Y1 124.49(3) 18_666 2 ?
Al2 Al3 Y1 124.49(3) 3_665 2 ?
Al1 Al3 Y1 116.90(3) 15 2 ?
Al1 Al3 Y1 116.90(3) 6 2 ?
Os1 Al3 Y3 120.108(17) . . ?
Os1 Al3 Y3 120.109(17) 16_556 . ?
Al3 Al3 Y3 65.28(2) 7 . ?
Al4 Al3 Y3 170.67(6) . . ?
Al1 Al3 Y3 66.46(3) 2 . ?
Al1 Al3 Y3 66.46(3) 17_556 . ?
Al2 Al3 Y3 118.16(4) 18_666 . ?
Al2 Al3 Y3 118.16(4) 3_665 . ?
Al1 Al3 Y3 72.75(3) 15 . ?
Al1 Al3 Y3 72.75(3) 6 . ?
Y1 Al3 Y3 107.76(3) 2 . ?
Os1 Al3 Y2 114.73(7) . . ?
Os1 Al3 Y2 125.47(7) 16_556 . ?
Al3 Al3 Y2 65.40(2) 7 . ?
Al4 Al3 Y2 169.20(6) . . ?
Al1 Al3 Y2 62.14(6) 2 . ?
Al1 Al3 Y2 70.86(7) 17_556 . ?
Al2 Al3 Y2 120.97(6) 18_666 . ?
Al2 Al3 Y2 115.15(6) 3_665 . ?
Al1 Al3 Y2 67.75(7) 15 . ?
Al1 Al3 Y2 77.77(7) 6 . ?
Y1 Al3 Y2 107.67(3) 2 . ?
Y3 Al3 Y2 5.46(7) . . ?
Os1 Al3 Y2 125.47(7) . 16_556 ?
Os1 Al3 Y2 114.73(7) 16_556 16_556 ?
Al3 Al3 Y2 65.40(2) 7 16_556 ?
Al4 Al3 Y2 169.20(6) . 16_556 ?
Al1 Al3 Y2 70.86(7) 2 16_556 ?
Al1 Al3 Y2 62.14(6) 17_556 16_556 ?
Al2 Al3 Y2 115.15(6) 18_666 16_556 ?
Al2 Al3 Y2 120.97(6) 3_665 16_556 ?
Al1 Al3 Y2 77.77(8) 15 16_556 ?
Al1 Al3 Y2 67.75(7) 6 16_556 ?
Y1 Al3 Y2 107.67(3) 2 16_556 ?
Y3 Al3 Y2 5.46(7) . 16_556 ?
Y2 Al3 Y2 10.93(15) . 16_556 ?
Os1 Al3 Al6 96.4(2) . . ?
Os1 Al3 Al6 143.6(2) 16_556 . ?
Al3 Al3 Al6 67.55(4) 7 . ?
Al4 Al3 Al6 154.3(2) . . ?
Al1 Al3 Al6 48.47(15) 2 . ?
Al1 Al3 Al6 86.18(18) 17_556 . ?
Al2 Al3 Al6 128.50(8) 18_666 . ?
Al2 Al3 Al6 103.86(14) 3_665 . ?
Al1 Al3 Al6 51.13(19) 15 . ?
Al1 Al3 Al6 94.9(2) 6 . ?
Y1 Al3 Al6 106.17(4) 2 . ?
Y3 Al3 Al6 24.0(2) . . ?
Y2 Al3 Al6 18.6(2) . . ?
Y2 Al3 Al6 29.5(2) 16_556 . ?
Os1 Al3 Al6 143.6(2) . 16_556 ?
Os1 Al3 Al6 96.4(2) 16_556 16_556 ?
Al3 Al3 Al6 67.55(4) 7 16_556 ?
Al4 Al3 Al6 154.3(2) . 16_556 ?
Al1 Al3 Al6 86.18(18) 2 16_556 ?
Al1 Al3 Al6 48.47(15) 17_556 16_556 ?
Al2 Al3 Al6 103.86(14) 18_666 16_556 ?
Al2 Al3 Al6 128.50(8) 3_665 16_556 ?
Al1 Al3 Al6 94.9(2) 15 16_556 ?
Al1 Al3 Al6 51.13(19) 6 16_556 ?
Y1 Al3 Al6 106.17(4) 2 16_556 ?
Y3 Al3 Al6 24.0(2) . 16_556 ?
Y2 Al3 Al6 29.5(2) . 16_556 ?
Y2 Al3 Al6 18.6(2) 16_556 16_556 ?
Al6 Al3 Al6 48.0(4) . 16_556 ?
Os1 Al3 Al3 99.22(2) . 9 ?
Os1 Al3 Al3 99.22(2) 16_556 9 ?
Al3 Al3 Al3 120.0 7 9 ?
Al4 Al3 Al3 115.96(4) . 9 ?
Al1 Al3 Al3 47.09(2) 2 9 ?
Al1 Al3 Al3 47.09(2) 17_556 9 ?
Al2 Al3 Al3 151.80(2) 18_666 9 ?
Al2 Al3 Al3 151.80(2) 3_665 9 ?
Al1 Al3 Al3 97.98(3) 15 9 ?
Al1 Al3 Al3 97.98(3) 6 9 ?
Y1 Al3 Al3 53.039(15) 2 9 ?
Y3 Al3 Al3 54.72(2) . 9 ?
Y2 Al3 Al3 54.90(2) . 9 ?
Y2 Al3 Al3 54.90(2) 16_556 9 ?
Al6 Al3 Al3 58.16(6) . 9 ?
Al6 Al3 Al3 58.16(6) 16_556 9 ?
Os1 Al3 Al7 85.559(17) . . ?
Os1 Al3 Al7 154.02(2) 16_556 . ?
Al3 Al3 Al7 69.979(18) 7 . ?
Al4 Al3 Al7 143.901(18) . . ?
Al1 Al3 Al7 41.63(3) 2 . ?
Al1 Al3 Al7 95.36(3) 17_556 . ?
Al2 Al3 Al7 131.03(4) 18_666 . ?
Al2 Al3 Al7 96.69(3) 3_665 . ?
Al1 Al3 Al7 41.77(3) 15 . ?
Al1 Al3 Al7 105.07(4) 6 . ?
Y1 Al3 Al7 104.46(2) 2 . ?
Y3 Al3 Al7 35.033(10) . . ?
Y2 Al3 Al7 29.57(7) . . ?
Y2 Al3 Al7 40.50(7) 16_556 . ?
Al6 Al3 Al7 11.0(2) . . ?
Al6 Al3 Al7 59.1(2) 16_556 . ?
Al3 Al3 Al7 61.773(16) 9 . ?
Os1 Al3 Al7 154.02(2) . 4 ?
Os1 Al3 Al7 85.560(17) 16_556 4 ?
Al3 Al3 Al7 69.979(18) 7 4 ?
Al4 Al3 Al7 143.901(18) . 4 ?
Al1 Al3 Al7 95.36(3) 2 4 ?
Al1 Al3 Al7 41.63(3) 17_556 4 ?
Al2 Al3 Al7 96.69(3) 18_666 4 ?
Al2 Al3 Al7 131.03(4) 3_665 4 ?
Al1 Al3 Al7 105.07(4) 15 4 ?
Al1 Al3 Al7 41.77(3) 6 4 ?
Y1 Al3 Al7 104.46(2) 2 4 ?
Y3 Al3 Al7 35.033(10) . 4 ?
Y2 Al3 Al7 40.50(7) . 4 ?
Y2 Al3 Al7 29.57(7) 16_556 4 ?
Al6 Al3 Al7 59.1(2) . 4 ?
Al6 Al3 Al7 11.0(2) 16_556 4 ?
Al3 Al3 Al7 61.773(16) 9 4 ?
Al7 Al3 Al7 70.07(2) . 4 ?
Os1 Al3 Al5 93.75(3) . 6 ?
Os1 Al3 Al5 33.949(11) 16_556 6 ?
Al3 Al3 Al5 99.26(2) 7 6 ?
Al4 Al3 Al5 38.56(2) . 6 ?
Al1 Al3 Al5 145.80(5) 2 6 ?
Al1 Al3 Al5 93.23(3) 17_556 6 ?
Al2 Al3 Al5 37.951(19) 18_666 6 ?
Al2 Al3 Al5 72.93(3) 3_665 6 ?
Al1 Al3 Al5 128.96(3) 15 6 ?
Al1 Al3 Al5 72.95(3) 6 6 ?
Y1 Al3 Al5 86.64(3) 2 6 ?
Y3 Al3 Al5 145.669(19) . 6 ?
Y2 Al3 Al5 150.71(7) . 6 ?
Y2 Al3 Al5 140.53(7) 16_556 6 ?
Al6 Al3 Al5 165.58(13) . 6 ?
Al6 Al3 Al5 122.7(2) 16_556 6 ?
Al3 Al3 Al5 129.991(17) 9 6 ?
Al7 Al3 Al5 168.02(3) . 6 ?
Al7 Al3 Al5 111.970(15) 4 6 ?
Os1 Al3 Al5 33.948(11) . 15 ?
Os1 Al3 Al5 93.75(3) 16_556 15 ?
Al3 Al3 Al5 99.26(2) 7 15 ?
Al4 Al3 Al5 38.56(2) . 15 ?
Al1 Al3 Al5 93.23(3) 2 15 ?
Al1 Al3 Al5 145.80(5) 17_556 15 ?
Al2 Al3 Al5 72.93(3) 18_666 15 ?
Al2 Al3 Al5 37.951(19) 3_665 15 ?
Al1 Al3 Al5 72.95(3) 15 15 ?
Al1 Al3 Al5 128.96(3) 6 15 ?
Y1 Al3 Al5 86.64(3) 2 15 ?
Y3 Al3 Al5 145.669(19) . 15 ?
Y2 Al3 Al5 140.53(7) . 15 ?
Y2 Al3 Al5 150.71(7) 16_556 15 ?
Al6 Al3 Al5 122.7(2) . 15 ?
Al6 Al3 Al5 165.58(13) 16_556 15 ?
Al3 Al3 Al5 129.991(17) 9 15 ?
Al7 Al3 Al5 111.970(15) . 15 ?
Al7 Al3 Al5 168.02(3) 4 15 ?
Al5 Al3 Al5 63.495(18) 6 15 ?
Os1 Al3 Al2 34.780(16) . 14_565 ?
Os1 Al3 Al2 114.57(4) 16_556 14_565 ?
Al3 Al3 Al2 132.80(2) 7 14_565 ?
Al4 Al3 Al2 72.52(3) . 14_565 ?
Al1 Al3 Al2 35.23(3) 2 14_565 ?
Al1 Al3 Al2 104.40(4) 17_556 14_565 ?
Al2 Al3 Al2 137.71(4) 18_666 14_565 ?
Al2 Al3 Al2 93.185(19) 3_665 14_565 ?
Al1 Al3 Al2 70.78(2) 15 14_565 ?
Al1 Al3 Al2 160.98(4) 6 14_565 ?
Y1 Al3 Al2 46.676(19) 2 14_565 ?
Y3 Al3 Al2 101.326(19) . 14_565 ?
Y2 Al3 Al2 97.25(6) . 14_565 ?
Y2 Al3 Al2 105.35(6) 16_556 14_565 ?
Al6 Al3 Al2 83.30(16) . 14_565 ?
Al6 Al3 Al2 118.39(14) 16_556 14_565 ?
Al3 Al3 Al2 64.955(12) 9 14_565 ?
Al7 Al3 Al2 75.124(18) . 14_565 ?
Al7 Al3 Al2 125.33(2) 4 14_565 ?
Al5 Al3 Al2 110.73(3) 6 14_565 ?
Al5 Al3 Al2 65.704(17) 15 14_565 ?
Os1 Al3 Al2 114.57(4) . 5_565 ?
Os1 Al3 Al2 34.779(16) 16_556 5_565 ?
Al3 Al3 Al2 132.80(2) 7 5_565 ?
Al4 Al3 Al2 72.52(3) . 5_565 ?
Al1 Al3 Al2 104.40(4) 2 5_565 ?
Al1 Al3 Al2 35.23(3) 17_556 5_565 ?
Al2 Al3 Al2 93.185(19) 18_666 5_565 ?
Al2 Al3 Al2 137.71(4) 3_665 5_565 ?
Al1 Al3 Al2 160.98(4) 15 5_565 ?
Al1 Al3 Al2 70.78(2) 6 5_565 ?
Y1 Al3 Al2 46.676(19) 2 5_565 ?
Y3 Al3 Al2 101.326(19) . 5_565 ?
Y2 Al3 Al2 105.35(6) . 5_565 ?
Y2 Al3 Al2 97.25(6) 16_556 5_565 ?
Al6 Al3 Al2 118.39(14) . 5_565 ?
Al6 Al3 Al2 83.30(16) 16_556 5_565 ?
Al3 Al3 Al2 64.955(12) 9 5_565 ?
Al7 Al3 Al2 125.33(2) . 5_565 ?
Al7 Al3 Al2 75.124(18) 4 5_565 ?
Al5 Al3 Al2 65.704(16) 6 5_565 ?
Al5 Al3 Al2 110.73(3) 15 5_565 ?
Al2 Al3 Al2 93.33(4) 14_565 5_565 ?
Os1 Al3 Os1 129.57(3) . 5 ?
Os1 Al3 Os1 76.36(2) 16_556 5 ?
Al3 Al3 Os1 34.357(12) 7 5 ?
Al4 Al3 Os1 105.51(4) . 5 ?
Al1 Al3 Os1 142.27(4) 2 5 ?
Al1 Al3 Os1 92.25(3) 17_556 5 ?
Al2 Al3 Os1 35.74(2) 18_666 5 ?
Al2 Al3 Os1 70.80(3) 3_665 5 ?
Al1 Al3 Os1 95.06(4) 15 5 ?
Al1 Al3 Os1 35.81(2) 6 5 ?
Y1 Al3 Os1 147.987(13) 2 5 ?
Y3 Al3 Os1 82.43(2) . 5 ?
Y2 Al3 Os1 85.28(5) . 5 ?
Y2 Al3 Os1 79.63(4) 16_556 5 ?
Al6 Al3 Os1 95.08(11) . 5 ?
Al6 Al3 Os1 70.78(9) 16_556 5 ?
Al3 Al3 Os1 128.042(10) 9 5 ?
Al7 Al3 Os1 100.76(3) . 5 ?
Al7 Al3 Os1 66.269(16) 4 5 ?
Al5 Al3 Os1 70.529(17) 6 5 ?
Al5 Al3 Os1 101.93(2) 15 5 ?
Al2 Al3 Os1 163.10(2) 14_565 5 ?
Al2 Al3 Os1 102.143(19) 5_565 5 ?
Os1 Al3 Os1 76.36(2) . 14 ?
Os1 Al3 Os1 129.57(3) 16_556 14 ?
Al3 Al3 Os1 34.357(12) 7 14 ?
Al4 Al3 Os1 105.51(4) . 14 ?
Al1 Al3 Os1 92.25(3) 2 14 ?
Al1 Al3 Os1 142.27(4) 17_556 14 ?
Al2 Al3 Os1 70.80(3) 18_666 14 ?
Al2 Al3 Os1 35.74(2) 3_665 14 ?
Al1 Al3 Os1 35.81(2) 15 14 ?
Al1 Al3 Os1 95.06(4) 6 14 ?
Y1 Al3 Os1 147.987(13) 2 14 ?
Y3 Al3 Os1 82.43(2) . 14 ?
Y2 Al3 Os1 79.63(4) . 14 ?
Y2 Al3 Os1 85.28(5) 16_556 14 ?
Al6 Al3 Os1 70.78(9) . 14 ?
Al6 Al3 Os1 95.08(11) 16_556 14 ?
Al3 Al3 Os1 128.042(10) 9 14 ?
Al7 Al3 Os1 66.269(16) . 14 ?
Al7 Al3 Os1 100.76(3) 4 14 ?
Al5 Al3 Os1 101.93(2) 6 14 ?
Al5 Al3 Os1 70.529(17) 15 14 ?
Al2 Al3 Os1 102.143(19) 14_565 14 ?
Al2 Al3 Os1 163.10(2) 5_565 14 ?
Os1 Al3 Os1 61.74(2) 5 14 ?
Os1 Al3 Al6 76.98(13) . 13 ?
Os1 Al3 Al6 161.86(12) 16_556 13 ?
Al3 Al3 Al6 72.41(4) 7 13 ?
Al4 Al3 Al6 135.49(13) . 13 ?
Al1 Al3 Al6 37.36(6) 2 13 ?
Al1 Al3 Al6 102.57(11) 17_556 13 ?
Al2 Al3 Al6 131.77(4) 18_666 13 ?
Al2 Al3 Al6 90.91(9) 3_665 13 ?
Al1 Al3 Al6 34.92(10) 15 13 ?
Al1 Al3 Al6 113.03(13) 6 13 ?
Y1 Al3 Al6 102.73(3) 2 13 ?
Y3 Al3 Al6 43.72(13) . 13 ?
Y2 Al3 Al6 38.26(15) . 13 ?
Y2 Al3 Al6 49.19(15) 16_556 13 ?
Al6 Al3 Al6 19.7(3) . 13 ?
Al6 Al3 Al6 67.75(8) 16_556 13 ?
Al3 Al3 Al6 65.33(6) 9 13 ?
Al7 Al3 Al6 8.69(13) . 13 ?
Al7 Al3 Al6 78.76(13) 4 13 ?
Al5 Al3 Al6 163.84(9) 6 13 ?
Al5 Al3 Al6 103.48(13) 15 13 ?
Al2 Al3 Al6 68.85(10) 14_565 13 ?
Al2 Al3 Al6 130.14(7) 5_565 13 ?
Os1 Al3 Al6 105.04(7) 5 13 ?
Os1 Al3 Al6 63.26(4) 14 13 ?
Os1 Al3 Al6 161.86(12) . 4 ?
Os1 Al3 Al6 76.98(13) 16_556 4 ?
Al3 Al3 Al6 72.41(4) 7 4 ?
Al4 Al3 Al6 135.49(13) . 4 ?
Al1 Al3 Al6 102.57(11) 2 4 ?
Al1 Al3 Al6 37.36(6) 17_556 4 ?
Al2 Al3 Al6 90.91(9) 18_666 4 ?
Al2 Al3 Al6 131.77(4) 3_665 4 ?
Al1 Al3 Al6 113.03(13) 15 4 ?
Al1 Al3 Al6 34.92(10) 6 4 ?
Y1 Al3 Al6 102.73(3) 2 4 ?
Y3 Al3 Al6 43.72(13) . 4 ?
Y2 Al3 Al6 49.19(15) . 4 ?
Y2 Al3 Al6 38.26(15) 16_556 4 ?
Al6 Al3 Al6 67.75(8) . 4 ?
Al6 Al3 Al6 19.7(3) 16_556 4 ?
Al3 Al3 Al6 65.33(6) 9 4 ?
Al7 Al3 Al6 78.76(13) . 4 ?
Al7 Al3 Al6 8.69(13) 4 4 ?
Al5 Al3 Al6 103.48(13) 6 4 ?
Al5 Al3 Al6 163.84(9) 15 4 ?
Al2 Al3 Al6 130.14(7) 14_565 4 ?
Al2 Al3 Al6 68.85(10) 5_565 4 ?
Os1 Al3 Al6 63.26(4) 5 4 ?
Os1 Al3 Al6 105.04(7) 14 4 ?
Al6 Al3 Al6 87.4(3) 13 4 ?
Os1 Al3 Al1 92.65(3) . . ?
Os1 Al3 Al1 144.54(4) 16_556 . ?
Al3 Al3 Al1 35.542(19) 7 . ?
Al4 Al3 Al1 139.35(4) . . ?
Al1 Al3 Al1 73.96(4) 2 . ?
Al1 Al3 Al1 112.67(4) 17_556 . ?
Al2 Al3 Al1 95.32(4) 18_666 . ?
Al2 Al3 Al1 70.60(3) 3_665 . ?
Al1 Al3 Al1 35.12(3) 15 . ?
Al1 Al3 Al1 88.48(3) 6 . ?
Y1 Al3 Al1 139.76(2) 2 . ?
Y3 Al3 Al1 47.731(18) . . ?
Y2 Al3 Al1 44.56(4) . . ?
Y2 Al3 Al1 51.20(5) 16_556 . ?
Al6 Al3 Al1 37.04(5) . . ?
Al6 Al3 Al1 64.50(16) 16_556 . ?
Al3 Al3 Al1 95.162(17) 9 . ?
Al7 Al3 Al1 35.900(17) . . ?
Al7 Al3 Al1 73.05(2) 4 . ?
Al5 Al3 Al1 132.39(3) 6 . ?
Al5 Al3 Al1 101.47(2) 15 . ?
Al2 Al3 Al1 100.89(3) 14_565 . ?
Al2 Al3 Al1 147.79(2) 5_565 . ?
Os1 Al3 Al1 69.27(3) 5 . ?
Os1 Al3 Al1 35.162(14) 14 . ?
Al6 Al3 Al1 37.03(3) 13 . ?
Al6 Al3 Al1 79.98(11) 4 . ?
Os1 Al3 Al1 144.54(4) . 16_556 ?
Os1 Al3 Al1 92.65(3) 16_556 16_556 ?
Al3 Al3 Al1 35.542(19) 7 16_556 ?
Al4 Al3 Al1 139.35(4) . 16_556 ?
Al1 Al3 Al1 112.67(4) 2 16_556 ?
Al1 Al3 Al1 73.96(4) 17_556 16_556 ?
Al2 Al3 Al1 70.60(3) 18_666 16_556 ?
Al2 Al3 Al1 95.32(4) 3_665 16_556 ?
Al1 Al3 Al1 88.48(3) 15 16_556 ?
Al1 Al3 Al1 35.12(3) 6 16_556 ?
Y1 Al3 Al1 139.76(2) 2 16_556 ?
Y3 Al3 Al1 47.731(18) . 16_556 ?
Y2 Al3 Al1 51.20(5) . 16_556 ?
Y2 Al3 Al1 44.56(4) 16_556 16_556 ?
Al6 Al3 Al1 64.50(16) . 16_556 ?
Al6 Al3 Al1 37.04(5) 16_556 16_556 ?
Al3 Al3 Al1 95.162(17) 9 16_556 ?
Al7 Al3 Al1 73.05(2) . 16_556 ?
Al7 Al3 Al1 35.901(17) 4 16_556 ?
Al5 Al3 Al1 101.47(2) 6 16_556 ?
Al5 Al3 Al1 132.39(3) 15 16_556 ?
Al2 Al3 Al1 147.79(2) 14_565 16_556 ?
Al2 Al3 Al1 100.89(2) 5_565 16_556 ?
Os1 Al3 Al1 35.162(14) 5 16_556 ?
Os1 Al3 Al1 69.27(3) 14 16_556 ?
Al6 Al3 Al1 79.98(11) 13 16_556 ?
Al6 Al3 Al1 37.03(3) 4 16_556 ?
Al1 Al3 Al1 53.70(3) . 16_556 ?
Os1 Al3 Al5 89.33(3) . 5_565 ?
Os1 Al3 Al5 29.945(16) 16_556 5_565 ?
Al3 Al3 Al5 136.738(15) 7 5_565 ?
Al4 Al3 Al5 37.47(3) . 5_565 ?
Al1 Al3 Al5 113.67(5) 2 5_565 ?
Al1 Al3 Al5 70.44(3) 17_556 5_565 ?
Al2 Al3 Al5 76.60(2) 18_666 5_565 ?
Al2 Al3 Al5 103.95(3) 3_665 5_565 ?
Al1 Al3 Al5 146.47(3) 15 5_565 ?
Al1 Al3 Al5 87.30(2) 6 5_565 ?
Y1 Al3 Al5 48.210(18) 2 5_565 ?
Y3 Al3 Al5 136.69(2) . 5_565 ?
Y2 Al3 Al5 140.56(6) . 5_565 ?
Y2 Al3 Al5 132.57(6) 16_556 5_565 ?
Al6 Al3 Al5 150.38(8) . 5_565 ?
Al6 Al3 Al5 117.39(18) 16_556 5_565 ?
Al3 Al3 Al5 92.255(17) 9 5_565 ?
Al7 Al3 Al5 152.18(3) . 5_565 ?
Al7 Al3 Al5 107.898(18) 4 5_565 ?
Al5 Al3 Al5 39.58(2) 6 5_565 ?
Al5 Al3 Al5 76.01(3) 15 5_565 ?
Al2 Al3 Al5 85.17(3) 14_565 5_565 ?
Al2 Al3 Al5 35.374(16) 5_565 5_565 ?
Os1 Al3 Al5 103.522(15) 5 5_565 ?
Os1 Al3 Al5 138.56(2) 14 5_565 ?
Al6 Al3 Al5 150.84(5) 13 5_565 ?
Al6 Al3 Al5 100.28(12) 4 5_565 ?
Al1 Al3 Al5 171.91(3) . 5_565 ?
Al1 Al3 Al5 122.412(19) 16_556 5_565 ?
Os1 Al4 Os1 118.29(4) 16_556 . ?
Os1 Al4 Al3 59.522(19) 16_556 . ?
Os1 Al4 Al3 59.52(2) . . ?
Os1 Al4 Al5 56.809(16) 16_556 6 ?
Os1 Al4 Al5 149.58(7) . 6 ?
Al3 Al4 Al5 103.44(4) . 6 ?
Os1 Al4 Al5 149.58(7) 16_556 15 ?
Os1 Al4 Al5 56.809(16) . 15 ?
Al3 Al4 Al5 103.44(4) . 15 ?
Al5 Al4 Al5 110.39(5) 6 15 ?
Os1 Al4 Al4 118.44(3) 16_556 2_665 ?
Os1 Al4 Al4 118.44(3) . 2_665 ?
Al3 Al4 Al4 149.72(10) . 2_665 ?
Al5 Al4 Al4 62.38(3) 6 2_665 ?
Al5 Al4 Al4 62.38(3) 15 2_665 ?
Os1 Al4 Al4 113.76(5) 16_556 3_565 ?
Os1 Al4 Al4 113.76(5) . 3_565 ?
Al3 Al4 Al4 150.29(10) . 3_565 ?
Al5 Al4 Al4 93.24(3) 6 3_565 ?
Al5 Al4 Al4 93.24(3) 15 3_565 ?
Al4 Al4 Al4 60.0 2_665 3_565 ?
Os1 Al4 Al5 141.91(6) 16_556 14_565 ?
Os1 Al4 Al5 55.408(17) . 14_565 ?
Al3 Al4 Al5 107.26(3) . 14_565 ?
Al5 Al4 Al5 149.25(5) 6 14_565 ?
Al5 Al4 Al5 64.12(3) 15 14_565 ?
Al4 Al4 Al5 90.86(3) 2_665 14_565 ?
Al4 Al4 Al5 58.38(4) 3_565 14_565 ?
Os1 Al4 Al5 55.407(16) 16_556 5_565 ?
Os1 Al4 Al5 141.91(6) . 5_565 ?
Al3 Al4 Al5 107.26(3) . 5_565 ?
Al5 Al4 Al5 64.12(3) 6 5_565 ?
Al5 Al4 Al5 149.25(5) 15 5_565 ?
Al4 Al4 Al5 90.86(4) 2_665 5_565 ?
Al4 Al4 Al5 58.38(4) 3_565 5_565 ?
Al5 Al4 Al5 104.20(6) 14_565 5_565 ?
Os1 Al4 Y1 73.37(3) 16_556 2 ?
Os1 Al4 Y1 73.38(3) . 2 ?
Al3 Al4 Y1 64.60(3) . 2 ?
Al5 Al4 Y1 124.80(3) 6 2 ?
Al5 Al4 Y1 124.80(3) 15 2 ?
Al4 Al4 Y1 145.68(8) 2_665 2 ?
Al4 Al4 Y1 85.68(8) 3_565 2 ?
Al5 Al4 Y1 68.98(4) 14_565 2 ?
Al5 Al4 Y1 68.98(4) 5_565 2 ?
Os1 Al4 Al2 97.60(5) 16_556 3_665 ?
Os1 Al4 Al2 54.25(3) . 3_665 ?
Al3 Al4 Al2 56.40(4) . 3_665 ?
Al5 Al4 Al2 95.48(6) 6 3_665 ?
Al5 Al4 Al2 53.85(4) 15 3_665 ?
Al4 Al4 Al2 96.57(7) 2_665 3_665 ?
Al4 Al4 Al2 146.92(5) 3_565 3_665 ?
Al5 Al4 Al2 102.86(3) 14_565 3_665 ?
Al5 Al4 Al2 151.79(4) 5_565 3_665 ?
Y1 Al4 Al2 114.45(3) 2 3_665 ?
Os1 Al4 Al2 54.25(3) 16_556 18_666 ?
Os1 Al4 Al2 97.60(5) . 18_666 ?
Al3 Al4 Al2 56.40(4) . 18_666 ?
Al5 Al4 Al2 53.85(4) 6 18_666 ?
Al5 Al4 Al2 95.48(6) 15 18_666 ?
Al4 Al4 Al2 96.57(7) 2_665 18_666 ?
Al4 Al4 Al2 146.92(5) 3_565 18_666 ?
Al5 Al4 Al2 151.79(4) 14_565 18_666 ?
Al5 Al4 Al2 102.86(3) 5_565 18_666 ?
Y1 Al4 Al2 114.45(3) 2 18_666 ?
Al2 Al4 Al2 49.34(5) 3_665 18_666 ?
Os1 Al4 Y1 99.20(4) 16_556 3_665 ?
Os1 Al4 Y1 99.20(4) . 3_665 ?
Al3 Al4 Y1 99.65(5) . 3_665 ?
Al5 Al4 Y1 56.43(3) 6 3_665 ?
Al5 Al4 Y1 56.43(3) 15 3_665 ?
Al4 Al4 Y1 50.07(5) 2_665 3_665 ?
Al4 Al4 Y1 110.07(5) 3_565 3_665 ?
Al5 Al4 Y1 118.72(3) 14_565 3_665 ?
Al5 Al4 Y1 118.72(3) 5_565 3_665 ?
Y1 Al4 Y1 164.25(4) 2 3_665 ?
Al2 Al4 Y1 51.84(3) 3_665 3_665 ?
Al2 Al4 Y1 51.84(3) 18_666 3_665 ?
Os1 Al4 Al5 86.497(19) 16_556 4_665 ?
Os1 Al4 Al5 154.72(3) . 4_665 ?
Al3 Al4 Al5 145.725(14) . 4_665 ?
Al5 Al4 Al5 47.90(3) 6 4_665 ?
Al5 Al4 Al5 104.65(3) 15 4_665 ?
Al4 Al4 Al5 43.13(2) 2_665 4_665 ?
Al4 Al4 Al5 45.433(19) 3_565 4_665 ?
Al5 Al4 Al5 102.46(4) 14_565 4_665 ?
Al5 Al4 Al5 47.81(2) 5_565 4_665 ?
Y1 Al4 Al5 112.55(4) 2 4_665 ?
Al2 Al4 Al5 131.97(5) 3_665 4_665 ?
Al2 Al4 Al5 101.50(3) 18_666 4_665 ?
Y1 Al4 Al5 80.20(2) 3_665 4_665 ?
Os1 Al4 Al5 154.72(3) 16_556 13_665 ?
Os1 Al4 Al5 86.498(19) . 13_665 ?
Al3 Al4 Al5 145.725(14) . 13_665 ?
Al5 Al4 Al5 104.65(3) 6 13_665 ?
Al5 Al4 Al5 47.90(3) 15 13_665 ?
Al4 Al4 Al5 43.13(2) 2_665 13_665 ?
Al4 Al4 Al5 45.433(19) 3_565 13_665 ?
Al5 Al4 Al5 47.81(2) 14_565 13_665 ?
Al5 Al4 Al5 102.46(4) 5_565 13_665 ?
Y1 Al4 Al5 112.55(4) 2 13_665 ?
Al2 Al4 Al5 101.50(3) 3_665 13_665 ?
Al2 Al4 Al5 131.97(5) 18_666 13_665 ?
Y1 Al4 Al5 80.20(2) 3_665 13_665 ?
Al5 Al4 Al5 68.42(3) 4_665 13_665 ?
Os1 Al4 Al1 87.29(3) 16_556 2 ?
Os1 Al4 Al1 34.096(19) . 2 ?
Al3 Al4 Al1 36.25(2) . 2 ?
Al5 Al4 Al1 139.28(4) 6 2 ?
Al5 Al4 Al1 90.64(2) 15 2 ?
Al4 Al4 Al1 152.50(2) 2_665 2 ?
Al4 Al4 Al1 120.87(7) 3_565 2 ?
Al5 Al4 Al1 71.16(3) 14_565 2 ?
Al5 Al4 Al1 113.25(4) 5_565 2 ?
Y1 Al4 Al1 46.581(17) 2 2 ?
Al2 Al4 Al1 68.68(3) 3_665 2 ?
Al2 Al4 Al1 90.92(3) 18_666 2 ?
Y1 Al4 Al1 120.52(4) 3_665 2 ?
Al5 Al4 Al1 159.10(5) 4_665 2 ?
Al5 Al4 Al1 115.02(2) 13_665 2 ?
Os1 Al4 Al1 34.096(19) 16_556 17_556 ?
Os1 Al4 Al1 87.29(3) . 17_556 ?
Al3 Al4 Al1 36.25(2) . 17_556 ?
Al5 Al4 Al1 90.64(2) 6 17_556 ?
Al5 Al4 Al1 139.28(4) 15 17_556 ?
Al4 Al4 Al1 152.50(2) 2_665 17_556 ?
Al4 Al4 Al1 120.87(7) 3_565 17_556 ?
Al5 Al4 Al1 113.25(4) 14_565 17_556 ?
Al5 Al4 Al1 71.16(3) 5_565 17_556 ?
Y1 Al4 Al1 46.581(17) 2 17_556 ?
Al2 Al4 Al1 90.92(3) 3_665 17_556 ?
Al2 Al4 Al1 68.68(3) 18_666 17_556 ?
Y1 Al4 Al1 120.52(4) 3_665 17_556 ?
Al5 Al4 Al1 115.02(2) 4_665 17_556 ?
Al5 Al4 Al1 159.10(5) 13_665 17_556 ?
Al1 Al4 Al1 54.10(3) 2 17_556 ?
Os1 Al4 Al2 114.47(4) 16_556 14_565 ?
Os1 Al4 Al2 34.11(2) . 14_565 ?
Al3 Al4 Al2 71.57(3) . 14_565 ?
Al5 Al4 Al2 170.92(3) 6 14_565 ?
Al5 Al4 Al2 78.43(2) 15 14_565 ?
Al4 Al4 Al2 125.62(3) 2_665 14_565 ?
Al4 Al4 Al2 88.30(6) 3_565 14_565 ?
Al5 Al4 Al2 36.18(2) 14_565 14_565 ?
Al5 Al4 Al2 109.55(5) 5_565 14_565 ?
Y1 Al4 Al2 46.370(18) 2 14_565 ?
Al2 Al4 Al2 88.02(3) 3_665 14_565 ?
Al2 Al4 Al2 124.71(4) 18_666 14_565 ?
Y1 Al4 Al2 131.15(2) 3_665 14_565 ?
Al5 Al4 Al2 133.45(4) 4_665 14_565 ?
Al5 Al4 Al2 82.77(2) 13_665 14_565 ?
Al1 Al4 Al2 35.32(2) 2 14_565 ?
Al1 Al4 Al2 80.91(3) 17_556 14_565 ?
Os1 Al4 Al2 34.11(2) 16_556 5_565 ?
Os1 Al4 Al2 114.47(4) . 5_565 ?
Al3 Al4 Al2 71.57(3) . 5_565 ?
Al5 Al4 Al2 78.43(2) 6 5_565 ?
Al5 Al4 Al2 170.92(3) 15 5_565 ?
Al4 Al4 Al2 125.62(3) 2_665 5_565 ?
Al4 Al4 Al2 88.30(6) 3_565 5_565 ?
Al5 Al4 Al2 109.55(5) 14_565 5_565 ?
Al5 Al4 Al2 36.18(2) 5_565 5_565 ?
Y1 Al4 Al2 46.370(18) 2 5_565 ?
Al2 Al4 Al2 124.71(4) 3_665 5_565 ?
Al2 Al4 Al2 88.02(3) 18_666 5_565 ?
Y1 Al4 Al2 131.15(2) 3_665 5_565 ?
Al5 Al4 Al2 82.77(2) 4_665 5_565 ?
Al5 Al4 Al2 133.45(4) 13_665 5_565 ?
Al1 Al4 Al2 80.91(3) 2 5_565 ?
Al1 Al4 Al2 35.32(2) 17_556 5_565 ?
Al2 Al4 Al2 92.68(4) 14_565 5_565 ?
Os1 Al4 Al2 109.64(5) 16_556 2 ?
Os1 Al4 Al2 79.97(4) . 2 ?
Al3 Al4 Al2 107.19(4) . 2 ?
Al5 Al4 Al2 130.45(5) 6 2 ?
Al5 Al4 Al2 99.24(4) 15 2 ?
Al4 Al4 Al2 101.70(6) 2_665 2 ?
Al4 Al4 Al2 45.04(6) 3_565 2 ?
Al5 Al4 Al2 35.85(3) 14_565 2 ?
Al5 Al4 Al2 70.03(4) 5_565 2 ?
Y1 Al4 Al2 46.10(3) 2 2 ?
Al2 Al4 Al2 133.94(3) 3_665 2 ?
Al2 Al4 Al2 160.39(3) 18_666 2 ?
Y1 Al4 Al2 147.73(2) 3_665 2 ?
Al5 Al4 Al2 87.26(3) 4_665 2 ?
Al5 Al4 Al2 67.54(2) 13_665 2 ?
Al1 Al4 Al2 76.11(3) 2 2 ?
Al1 Al4 Al2 91.73(3) 17_556 2 ?
Al2 Al4 Al2 47.24(3) 14_565 2 ?
Al2 Al4 Al2 75.59(3) 5_565 2 ?
Os1 Al4 Al2 79.97(4) 16_556 17_556 ?
Os1 Al4 Al2 109.64(5) . 17_556 ?
Al3 Al4 Al2 107.19(4) . 17_556 ?
Al5 Al4 Al2 99.24(4) 6 17_556 ?
Al5 Al4 Al2 130.45(5) 15 17_556 ?
Al4 Al4 Al2 101.70(6) 2_665 17_556 ?
Al4 Al4 Al2 45.04(6) 3_565 17_556 ?
Al5 Al4 Al2 70.03(4) 14_565 17_556 ?
Al5 Al4 Al2 35.85(3) 5_565 17_556 ?
Y1 Al4 Al2 46.10(3) 2 17_556 ?
Al2 Al4 Al2 160.39(3) 3_665 17_556 ?
Al2 Al4 Al2 133.94(3) 18_666 17_556 ?
Y1 Al4 Al2 147.73(2) 3_665 17_556 ?
Al5 Al4 Al2 67.54(2) 4_665 17_556 ?
Al5 Al4 Al2 87.26(3) 13_665 17_556 ?
Al1 Al4 Al2 91.73(3) 2 17_556 ?
Al1 Al4 Al2 76.11(3) 17_556 17_556 ?
Al2 Al4 Al2 75.59(3) 14_565 17_556 ?
Al2 Al4 Al2 47.24(3) 5_565 17_556 ?
Al2 Al4 Al2 34.58(3) 2 17_556 ?
Os1 Al4 Al4 148.837(19) 16_556 20 ?
Os1 Al4 Al4 30.75(2) . 20 ?
Al3 Al4 Al4 90.188(2) . 20 ?
Al5 Al4 Al4 147.52(6) 6 20 ?
Al5 Al4 Al4 37.18(2) 15 20 ?
Al4 Al4 Al4 91.177(17) 2_665 20 ?
Al4 Al4 Al4 88.52(3) 3_565 20 ?
Al5 Al4 Al4 35.498(17) 14_565 20 ?
Al5 Al4 Al4 139.67(7) 5_565 20 ?
Y1 Al4 Al4 87.68(4) 2 20 ?
Al2 Al4 Al4 67.56(3) 3_665 20 ?
Al2 Al4 Al4 116.88(5) 18_666 20 ?
Y1 Al4 Al4 92.59(4) 3_665 20 ?
Al5 Al4 Al4 124.084(15) 4_665 20 ?
Al5 Al4 Al4 55.747(13) 13_665 20 ?
Al1 Al4 Al4 62.02(2) 2 20 ?
Al1 Al4 Al4 116.06(3) 17_556 20 ?
Al2 Al4 Al4 41.40(3) 14_565 20 ?
Al2 Al4 Al4 134.05(5) 5_565 20 ?
Al2 Al4 Al4 70.12(4) 2 20 ?
Al2 Al4 Al4 104.71(5) 17_556 20 ?
Os1 Al4 Al4 30.75(2) 16_556 20_556 ?
Os1 Al4 Al4 148.836(19) . 20_556 ?
Al3 Al4 Al4 90.188(2) . 20_556 ?
Al5 Al4 Al4 37.18(2) 6 20_556 ?
Al5 Al4 Al4 147.52(6) 15 20_556 ?
Al4 Al4 Al4 91.177(17) 2_665 20_556 ?
Al4 Al4 Al4 88.52(3) 3_565 20_556 ?
Al5 Al4 Al4 139.67(7) 14_565 20_556 ?
Al5 Al4 Al4 35.498(18) 5_565 20_556 ?
Y1 Al4 Al4 87.68(4) 2 20_556 ?
Al2 Al4 Al4 116.88(5) 3_665 20_556 ?
Al2 Al4 Al4 67.56(3) 18_666 20_556 ?
Y1 Al4 Al4 92.59(4) 3_665 20_556 ?
Al5 Al4 Al4 55.747(13) 4_665 20_556 ?
Al5 Al4 Al4 124.084(14) 13_665 20_556 ?
Al1 Al4 Al4 116.06(3) 2 20_556 ?
Al1 Al4 Al4 62.02(2) 17_556 20_556 ?
Al2 Al4 Al4 134.05(5) 14_565 20_556 ?
Al2 Al4 Al4 41.40(3) 5_565 20_556 ?
Al2 Al4 Al4 104.71(5) 2 20_556 ?
Al2 Al4 Al4 70.12(4) 17_556 20_556 ?
Al4 Al4 Al4 174.67(9) 20 20_556 ?
Os1 Al4 Os1 86.57(2) 16_556 17_666 ?
Os1 Al4 Os1 142.79(4) . 17_666 ?
Al3 Al4 Os1 129.67(5) . 17_666 ?
Al5 Al4 Os1 30.289(12) 6 17_666 ?
Al5 Al4 Os1 87.44(3) 15 17_666 ?
Al4 Al4 Os1 32.12(2) 2_665 17_666 ?
Al4 Al4 Os1 74.70(3) 3_565 17_666 ?
Al5 Al4 Os1 121.29(3) 14_565 17_666 ?
Al5 Al4 Os1 74.48(2) 5_565 17_666 ?
Y1 Al4 Os1 143.46(3) 2 17_666 ?
Al2 Al4 Os1 97.98(4) 3_665 17_666 ?
Al2 Al4 Os1 73.89(3) 18_666 17_666 ?
Y1 Al4 Os1 46.764(14) 3_665 17_666 ?
Al5 Al4 Os1 34.229(7) 4_665 17_666 ?
Al5 Al4 Os1 74.57(2) 13_665 17_666 ?
Al1 Al4 Os1 164.41(4) 2 17_666 ?
Al1 Al4 Os1 120.64(2) 17_556 17_666 ?
Al2 Al4 Os1 157.28(3) 14_565 17_666 ?
Al2 Al4 Os1 101.586(18) 5_565 17_666 ?
Al2 Al4 Os1 119.47(3) 2 17_666 ?
Al2 Al4 Os1 101.27(2) 17_556 17_666 ?
Al4 Al4 Os1 121.55(3) 20 17_666 ?
Al4 Al4 Os1 61.77(2) 20_556 17_666 ?
Os1 Al4 Os1 142.79(4) 16_556 2_665 ?
Os1 Al4 Os1 86.57(2) . 2_665 ?
Al3 Al4 Os1 129.67(5) . 2_665 ?
Al5 Al4 Os1 87.44(3) 6 2_665 ?
Al5 Al4 Os1 30.289(12) 15 2_665 ?
Al4 Al4 Os1 32.12(2) 2_665 2_665 ?
Al4 Al4 Os1 74.70(3) 3_565 2_665 ?
Al5 Al4 Os1 74.48(2) 14_565 2_665 ?
Al5 Al4 Os1 121.29(3) 5_565 2_665 ?
Y1 Al4 Os1 143.46(3) 2 2_665 ?
Al2 Al4 Os1 73.89(3) 3_665 2_665 ?
Al2 Al4 Os1 97.98(4) 18_666 2_665 ?
Y1 Al4 Os1 46.764(14) 3_665 2_665 ?
Al5 Al4 Os1 74.57(2) 4_665 2_665 ?
Al5 Al4 Os1 34.229(8) 13_665 2_665 ?
Al1 Al4 Os1 120.64(2) 2 2_665 ?
Al1 Al4 Os1 164.41(4) 17_556 2_665 ?
Al2 Al4 Os1 101.586(18) 14_565 2_665 ?
Al2 Al4 Os1 157.28(3) 5_565 2_665 ?
Al2 Al4 Os1 101.27(2) 2 2_665 ?
Al2 Al4 Os1 119.47(3) 17_556 2_665 ?
Al4 Al4 Os1 61.77(2) 20 2_665 ?
Al4 Al4 Os1 121.55(3) 20_556 2_665 ?
Os1 Al4 Os1 59.826(19) 17_666 2_665 ?
Os1 Al4 Al1 94.19(3) 16_556 15 ?
Os1 Al4 Al1 30.02(2) . 15 ?
Al3 Al4 Al1 35.71(2) . 15 ?
Al5 Al4 Al1 122.09(5) 6 15 ?
Al5 Al4 Al1 68.49(3) 15 15 ?
Al4 Al4 Al1 126.74(6) 2_665 15 ?
Al4 Al4 Al1 143.74(4) 3_565 15 ?
Al5 Al4 Al1 85.36(2) 14_565 15 ?
Al5 Al4 Al1 141.46(3) 5_565 15 ?
Y1 Al4 Al1 80.57(2) 2 15 ?
Al2 Al4 Al1 34.45(2) 3_665 15 ?
Al2 Al4 Al1 68.40(3) 18_666 15 ?
Y1 Al4 Al1 86.27(3) 3_665 15 ?
Al5 Al4 Al1 166.38(5) 4_665 15 ?
Al5 Al4 Al1 110.91(2) 13_665 15 ?
Al1 Al4 Al1 34.28(2) 2 15 ?
Al1 Al4 Al1 70.79(3) 17_556 15 ?
Al2 Al4 Al1 58.193(19) 14_565 15 ?
Al2 Al4 Al1 105.32(3) 5_565 15 ?
Al2 Al4 Al1 105.23(2) 2 15 ?
Al2 Al4 Al1 126.00(3) 17_556 15 ?
Al4 Al4 Al1 57.714(18) 20 15 ?
Al4 Al4 Al1 123.95(2) 20_556 15 ?
Os1 Al4 Al1 132.18(4) 17_666 15 ?
Os1 Al4 Al1 97.24(3) 2_665 15 ?
Os1 Al4 Al1 30.02(2) 16_556 6 ?
Os1 Al4 Al1 94.19(3) . 6 ?
Al3 Al4 Al1 35.71(2) . 6 ?
Al5 Al4 Al1 68.49(3) 6 6 ?
Al5 Al4 Al1 122.09(5) 15 6 ?
Al4 Al4 Al1 126.74(6) 2_665 6 ?
Al4 Al4 Al1 143.74(4) 3_565 6 ?
Al5 Al4 Al1 141.46(3) 14_565 6 ?
Al5 Al4 Al1 85.36(2) 5_565 6 ?
Y1 Al4 Al1 80.57(2) 2 6 ?
Al2 Al4 Al1 68.40(3) 3_665 6 ?
Al2 Al4 Al1 34.45(2) 18_666 6 ?
Y1 Al4 Al1 86.27(3) 3_665 6 ?
Al5 Al4 Al1 110.91(2) 4_665 6 ?
Al5 Al4 Al1 166.38(5) 13_665 6 ?
Al1 Al4 Al1 70.79(3) 2 6 ?
Al1 Al4 Al1 34.28(2) 17_556 6 ?
Al2 Al4 Al1 105.32(3) 14_565 6 ?
Al2 Al4 Al1 58.193(19) 5_565 6 ?
Al2 Al4 Al1 126.00(3) 2 6 ?
Al2 Al4 Al1 105.23(2) 17_556 6 ?
Al4 Al4 Al1 123.95(2) 20 6 ?
Al4 Al4 Al1 57.714(18) 20_556 6 ?
Os1 Al4 Al1 97.24(3) 17_666 6 ?
Os1 Al4 Al1 132.18(4) 2_665 6 ?
Al1 Al4 Al1 66.30(3) 15 6 ?
Os1 Al4 Os1 84.14(3) 16_556 18_566 ?
Os1 Al4 Os1 137.10(5) . 18_566 ?
Al3 Al4 Os1 134.41(4) . 18_566 ?
Al5 Al4 Os1 73.21(3) 6 18_566 ?
Al5 Al4 Os1 120.63(3) 15 18_566 ?
Al4 Al4 Os1 70.10(4) 2_665 18_566 ?
Al4 Al4 Os1 29.86(2) 3_565 18_566 ?
Al5 Al4 Os1 83.94(4) 14_565 18_566 ?
Al5 Al4 Os1 29.216(15) 5_565 18_566 ?
Y1 Al4 Os1 80.05(3) 2 18_566 ?
Al2 Al4 Os1 165.34(4) 3_665 18_566 ?
Al2 Al4 Os1 124.17(2) 18_666 18_566 ?
Y1 Al4 Os1 113.500(19) 3_665 18_566 ?
Al5 Al4 Os1 33.411(10) 4_665 18_566 ?
Al5 Al4 Os1 73.26(2) 13_665 18_566 ?
Al1 Al4 Os1 125.98(4) 2 18_566 ?
Al1 Al4 Os1 98.36(3) 17_556 18_566 ?
Al2 Al4 Os1 104.57(4) 14_565 18_566 ?
Al2 Al4 Os1 63.14(2) 5_565 18_566 ?
Al2 Al4 Os1 57.49(3) 2 18_566 ?
Al2 Al4 Os1 34.257(15) 17_556 18_566 ?
Al4 Al4 Os1 117.33(4) 20 18_566 ?
Al4 Al4 Os1 59.19(2) 20_556 18_566 ?
Os1 Al4 Os1 67.525(12) 17_666 18_566 ?
Os1 Al4 Os1 95.887(19) 2_665 18_566 ?
Al1 Al4 Os1 160.20(4) 15 18_566 ?
Al1 Al4 Os1 114.15(2) 6 18_566 ?
Os1 Al4 Os1 137.10(5) 16_556 3_565 ?
Os1 Al4 Os1 84.14(3) . 3_565 ?
Al3 Al4 Os1 134.41(4) . 3_565 ?
Al5 Al4 Os1 120.63(3) 6 3_565 ?
Al5 Al4 Os1 73.21(3) 15 3_565 ?
Al4 Al4 Os1 70.10(4) 2_665 3_565 ?
Al4 Al4 Os1 29.863(19) 3_565 3_565 ?
Al5 Al4 Os1 29.216(15) 14_565 3_565 ?
Al5 Al4 Os1 83.94(4) 5_565 3_565 ?
Y1 Al4 Os1 80.05(3) 2 3_565 ?
Al2 Al4 Os1 124.17(2) 3_665 3_565 ?
Al2 Al4 Os1 165.34(4) 18_666 3_565 ?
Y1 Al4 Os1 113.500(19) 3_665 3_565 ?
Al5 Al4 Os1 73.26(2) 4_665 3_565 ?
Al5 Al4 Os1 33.411(10) 13_665 3_565 ?
Al1 Al4 Os1 98.36(3) 2 3_565 ?
Al1 Al4 Os1 125.98(4) 17_556 3_565 ?
Al2 Al4 Os1 63.14(2) 14_565 3_565 ?
Al2 Al4 Os1 104.57(4) 5_565 3_565 ?
Al2 Al4 Os1 34.257(15) 2 3_565 ?
Al2 Al4 Os1 57.49(3) 17_556 3_565 ?
Al4 Al4 Os1 59.19(2) 20 3_565 ?
Al4 Al4 Os1 117.33(4) 20_556 3_565 ?
Os1 Al4 Os1 95.887(19) 17_666 3_565 ?
Os1 Al4 Os1 67.525(12) 2_665 3_565 ?
Al1 Al4 Os1 114.15(2) 15 3_565 ?
Al1 Al4 Os1 160.20(4) 6 3_565 ?
Os1 Al4 Os1 58.17(2) 18_566 3_565 ?
Os1 Al4 Al3 65.61(3) 16_556 7 ?
Os1 Al4 Al3 65.60(3) . 7 ?
Al3 Al4 Al3 27.85(4) . 7 ?
Al5 Al4 Al3 87.82(4) 6 7 ?
Al5 Al4 Al3 87.82(4) 15 7 ?
Al4 Al4 Al3 121.87(8) 2_665 7 ?
Al4 Al4 Al3 178.13(8) 3_565 7 ?
Al5 Al4 Al3 120.90(2) 14_565 7 ?
Al5 Al4 Al3 120.90(2) 5_565 7 ?
Y1 Al4 Al3 92.45(3) 2 7 ?
Al2 Al4 Al3 34.31(2) 3_665 7 ?
Al2 Al4 Al3 34.31(2) 18_666 7 ?
Y1 Al4 Al3 71.80(3) 3_665 7 ?
Al5 Al4 Al3 135.69(3) 4_665 7 ?
Al5 Al4 Al3 135.69(3) 13_665 7 ?
Al1 Al4 Al3 57.56(2) 2 7 ?
Al1 Al4 Al3 57.56(2) 17_556 7 ?
Al2 Al4 Al3 90.41(2) 14_565 7 ?
Al2 Al4 Al3 90.41(2) 5_565 7 ?
Al2 Al4 Al3 133.26(3) 2 7 ?
Al2 Al4 Al3 133.26(3) 17_556 7 ?
Al4 Al4 Al3 91.41(2) 20 7 ?
Al4 Al4 Al3 91.41(2) 20_556 7 ?
Os1 Al4 Al3 106.90(3) 17_666 7 ?
Os1 Al4 Al3 106.90(3) 2_665 7 ?
Al1 Al4 Al3 35.584(17) 15 7 ?
Al1 Al4 Al3 35.584(17) 6 7 ?
Os1 Al4 Al3 149.683(10) 18_566 7 ?
Os1 Al4 Al3 149.683(10) 3_565 7 ?
Os1 Al5 Os1 168.85(4) 14 15_655 ?
Os1 Al5 Al2 61.21(2) 14 13_655 ?
Os1 Al5 Al2 128.91(3) 15_655 13_655 ?
Os1 Al5 Al2 128.90(3) 14 . ?
Os1 Al5 Al2 61.21(2) 15_655 . ?
Al2 Al5 Al2 82.12(4) 13_655 . ?
Os1 Al5 Al4 116.92(2) 14 9_655 ?
Os1 Al5 Al4 59.242(19) 15_655 9_655 ?
Al2 Al5 Al4 141.53(5) 13_655 9_655 ?
Al2 Al5 Al4 70.88(4) . 9_655 ?
Os1 Al5 Al4 59.239(19) 14 14 ?
Os1 Al5 Al4 116.92(2) 15_655 14 ?
Al2 Al5 Al4 70.88(4) 13_655 14 ?
Al2 Al5 Al4 141.53(5) . 14 ?
Al4 Al5 Al4 144.85(7) 9_655 14 ?
Os1 Al5 Al4 57.71(2) 14 7 ?
Os1 Al5 Al4 117.74(3) 15_655 7 ?
Al2 Al5 Al4 105.12(3) 13_655 7 ?
Al2 Al5 Al4 105.82(4) . 7 ?
Al4 Al5 Al4 59.24(4) 9_655 7 ?
Al4 Al5 Al4 107.32(3) 14 7 ?
Os1 Al5 Al4 117.74(3) 14 15_655 ?
Os1 Al5 Al4 57.71(2) 15_655 15_655 ?
Al2 Al5 Al4 105.82(4) 13_655 15_655 ?
Al2 Al5 Al4 105.13(3) . 15_655 ?
Al4 Al5 Al4 107.33(3) 9_655 15_655 ?
Al4 Al5 Al4 59.24(4) 14 15_655 ?
Al4 Al5 Al4 138.57(6) 7 15_655 ?
Os1 Al5 Al5 114.42(2) 14 2_655 ?
Os1 Al5 Al5 54.43(2) 15_655 2_655 ?
Al2 Al5 Al5 158.71(2) 13_655 2_655 ?
Al2 Al5 Al5 111.99(2) . 2_655 ?
Al4 Al5 Al5 59.76(4) 9_655 2_655 ?
Al4 Al5 Al5 88.89(3) 14 2_655 ?
Al4 Al5 Al5 86.83(2) 7 2_655 ?
Al4 Al5 Al5 56.12(3) 15_655 2_655 ?
Os1 Al5 Al5 54.42(2) 14 3_665 ?
Os1 Al5 Al5 114.43(2) 15_655 3_665 ?
Al2 Al5 Al5 111.98(2) 13_655 3_665 ?
Al2 Al5 Al5 158.71(2) . 3_665 ?
Al4 Al5 Al5 88.90(3) 9_655 3_665 ?
Al4 Al5 Al5 59.75(4) 14 3_665 ?
Al4 Al5 Al5 56.12(3) 7 3_665 ?
Al4 Al5 Al5 86.83(2) 15_655 3_665 ?
Al5 Al5 Al5 60.0 2_655 3_665 ?
Os1 Al5 Y1 118.492(18) 14 13_655 ?
Os1 Al5 Y1 68.966(12) 15_655 13_655 ?
Al2 Al5 Y1 62.72(3) 13_655 13_655 ?
Al2 Al5 Y1 62.71(3) . 13_655 ?
Al4 Al5 Y1 122.24(3) 9_655 13_655 ?
Al4 Al5 Y1 80.43(3) 14 13_655 ?
Al4 Al5 Y1 163.27(4) 7 13_655 ?
Al4 Al5 Y1 58.16(3) 15_655 13_655 ?
Al5 Al5 Y1 108.454(12) 2_655 13_655 ?
Al5 Al5 Y1 137.432(12) 3_665 13_655 ?
Os1 Al5 Y1 68.963(12) 14 . ?
Os1 Al5 Y1 118.495(18) 15_655 . ?
Al2 Al5 Y1 62.71(3) 13_655 . ?
Al2 Al5 Y1 62.72(3) . . ?
Al4 Al5 Y1 80.43(3) 9_655 . ?
Al4 Al5 Y1 122.23(3) 14 . ?
Al4 Al5 Y1 58.16(3) 7 . ?
Al4 Al5 Y1 163.27(4) 15_655 . ?
Al5 Al5 Y1 137.433(13) 2_655 . ?
Al5 Al5 Y1 108.448(13) 3_665 . ?
Y1 Al5 Y1 105.12(3) 13_655 . ?
Os1 Al5 Al4 86.89(3) 14 8_665 ?
Os1 Al5 Al4 83.90(3) 15_655 8_665 ?
Al2 Al5 Al4 146.42(3) 13_655 8_665 ?
Al2 Al5 Al4 114.42(3) . 8_665 ?
Al4 Al5 Al4 43.62(3) 9_655 8_665 ?
Al4 Al5 Al4 102.99(5) 14 8_665 ?
Al4 Al5 Al4 43.71(3) 7 8_665 ?
Al4 Al5 Al4 97.94(5) 15_655 8_665 ?
Al5 Al5 Al4 43.21(2) 2_655 8_665 ?
Al5 Al5 Al4 45.353(18) 3_665 8_665 ?
Y1 Al5 Al4 150.50(3) 13_655 8_665 ?
Y1 Al5 Al4 97.74(2) . 8_665 ?
Os1 Al5 Al4 83.90(3) 14 13_665 ?
Os1 Al5 Al4 86.89(3) 15_655 13_665 ?
Al2 Al5 Al4 114.42(3) 13_655 13_665 ?
Al2 Al5 Al4 146.43(3) . 13_665 ?
Al4 Al5 Al4 102.99(5) 9_655 13_665 ?
Al4 Al5 Al4 43.62(3) 14 13_665 ?
Al4 Al5 Al4 97.94(5) 7 13_665 ?
Al4 Al5 Al4 43.71(3) 15_655 13_665 ?
Al5 Al5 Al4 45.351(18) 2_655 13_665 ?
Al5 Al5 Al4 43.21(2) 3_665 13_665 ?
Y1 Al5 Al4 97.74(2) 13_655 13_665 ?
Y1 Al5 Al4 150.50(3) . 13_665 ?
Al4 Al5 Al4 68.51(3) 8_665 13_665 ?
Os1 Al5 Al5 95.57(2) 14 13_655 ?
Os1 Al5 Al5 95.58(2) 15_655 13_655 ?
Al2 Al5 Al5 41.06(2) 13_655 13_655 ?
Al2 Al5 Al5 41.06(2) . 13_655 ?
Al4 Al5 Al5 107.58(4) 9_655 13_655 ?
Al4 Al5 Al5 107.57(4) 14 13_655 ?
Al4 Al5 Al5 110.71(3) 7 13_655 ?
Al4 Al5 Al5 110.72(3) 15_655 13_655 ?
Al5 Al5 Al5 150.0 2_655 13_655 ?
Al5 Al5 Al5 150.0 3_665 13_655 ?
Y1 Al5 Al5 52.560(14) 13_655 13_655 ?
Y1 Al5 Al5 52.559(14) . 13_655 ?
Al4 Al5 Al5 145.747(13) 8_665 13_655 ?
Al4 Al5 Al5 145.747(13) 13_665 13_655 ?
Os1 Al5 Al3 147.852(9) 14 9_655 ?
Os1 Al5 Al3 35.372(11) 15_655 9_655 ?
Al2 Al5 Al3 121.80(3) 13_655 9_655 ?
Al2 Al5 Al3 39.68(2) . 9_655 ?
Al4 Al5 Al3 38.01(3) 9_655 9_655 ?
Al4 Al5 Al3 152.27(2) 14 9_655 ?
Al4 Al5 Al3 93.50(3) 7 9_655 ?
Al4 Al5 Al3 93.03(3) 15_655 9_655 ?
Al5 Al5 Al3 73.85(2) 2_655 9_655 ?
Al5 Al5 Al3 123.84(2) 3_665 9_655 ?
Y1 Al5 Al3 84.61(2) 13_655 9_655 ?
Y1 Al5 Al3 84.164(19) . 9_655 ?
Al4 Al5 Al3 79.36(3) 8_665 9_655 ?
Al4 Al5 Al3 116.79(3) 13_665 9_655 ?
Al5 Al5 Al3 80.74(2) 13_655 9_655 ?
Os1 Al5 Al3 35.370(11) 14 14 ?
Os1 Al5 Al3 147.854(10) 15_655 14 ?
Al2 Al5 Al3 39.68(2) 13_655 14 ?
Al2 Al5 Al3 121.80(3) . 14 ?
Al4 Al5 Al3 152.26(2) 9_655 14 ?
Al4 Al5 Al3 38.01(3) 14 14 ?
Al4 Al5 Al3 93.02(3) 7 14 ?
Al4 Al5 Al3 93.50(3) 15_655 14 ?
Al5 Al5 Al3 123.84(2) 2_655 14 ?
Al5 Al5 Al3 73.85(2) 3_665 14 ?
Y1 Al5 Al3 84.163(19) 13_655 14 ?
Y1 Al5 Al3 84.61(2) . 14 ?
Al4 Al5 Al3 116.79(3) 8_665 14 ?
Al4 Al5 Al3 79.36(3) 13_665 14 ?
Al5 Al5 Al3 80.74(2) 13_655 14 ?
Al3 Al5 Al3 161.48(4) 9_655 14 ?
Os1 Al5 Al2 72.734(16) 14 4_654 ?
Os1 Al5 Al2 112.773(18) 15_655 4_654 ?
Al2 Al5 Al2 34.37(3) 13_655 4_654 ?
Al2 Al5 Al2 97.16(3) . 4_654 ?
Al4 Al5 Al2 167.64(4) 9_655 4_654 ?
Al4 Al5 Al2 45.88(4) 14 4_654 ?
Al4 Al5 Al2 129.48(3) 7 4_654 ?
Al4 Al5 Al2 72.12(3) 15_655 4_654 ?
Al5 Al5 Al2 125.047(15) 2_655 4_654 ?
Al5 Al5 Al2 103.336(13) 3_665 4_654 ?
Y1 Al5 Al2 46.517(17) 13_655 4_654 ?
Y1 Al5 Al2 97.07(2) . 4_654 ?
Al4 Al5 Al2 148.42(2) 8_665 4_654 ?
Al4 Al5 Al2 85.199(18) 13_665 4_654 ?
Al5 Al5 Al2 62.306(13) 13_655 4_654 ?
Al3 Al5 Al2 129.91(2) 9_655 4_654 ?
Al3 Al5 Al2 37.715(17) 14 4_654 ?
Os1 Al5 Al2 112.771(18) 14 16_556 ?
Os1 Al5 Al2 72.736(16) 15_655 16_556 ?
Al2 Al5 Al2 97.16(3) 13_655 16_556 ?
Al2 Al5 Al2 34.37(3) . 16_556 ?
Al4 Al5 Al2 45.88(4) 9_655 16_556 ?
Al4 Al5 Al2 167.64(4) 14 16_556 ?
Al4 Al5 Al2 72.12(3) 7 16_556 ?
Al4 Al5 Al2 129.48(3) 15_655 16_556 ?
Al5 Al5 Al2 103.340(13) 2_655 16_556 ?
Al5 Al5 Al2 125.047(15) 3_665 16_556 ?
Y1 Al5 Al2 97.07(3) 13_655 16_556 ?
Y1 Al5 Al2 46.518(17) . 16_556 ?
Al4 Al5 Al2 85.200(18) 8_665 16_556 ?
Al4 Al5 Al2 148.43(2) 13_665 16_556 ?
Al5 Al5 Al2 62.308(14) 13_655 16_556 ?
Al3 Al5 Al2 37.715(17) 9_655 16_556 ?
Al3 Al5 Al2 129.90(2) 14 16_556 ?
Al2 Al5 Al2 124.61(3) 4_654 16_556 ?
Os1 Al5 Al1 157.76(3) 14 13_655 ?
Os1 Al5 Al1 33.302(12) 15_655 13_655 ?
Al2 Al5 Al1 97.15(3) 13_655 13_655 ?
Al2 Al5 Al1 34.76(3) . 13_655 ?
Al4 Al5 Al1 76.04(3) 9_655 13_655 ?
Al4 Al5 Al1 121.36(3) 14 13_655 ?
Al4 Al5 Al1 130.83(3) 7 13_655 ?
Al4 Al5 Al1 70.93(2) 15_655 13_655 ?
Al5 Al5 Al1 87.586(13) 2_655 13_655 ?
Al5 Al5 Al1 147.429(13) 3_665 13_655 ?
Y1 Al5 Al1 46.227(18) 13_655 13_655 ?
Y1 Al5 Al1 97.46(2) . 13_655 ?
Al4 Al5 Al1 113.06(3) 8_665 13_655 ?
Al4 Al5 Al1 111.87(3) 13_665 13_655 ?
Al5 Al5 Al1 62.474(13) 13_655 13_655 ?
Al3 Al5 Al1 38.50(2) 9_655 13_655 ?
Al3 Al5 Al1 129.34(2) 14 13_655 ?
Al2 Al5 Al1 92.39(2) 4_654 13_655 ?
Al2 Al5 Al1 61.88(2) 16_556 13_655 ?
Os1 Al5 Al1 33.301(12) 14 . ?
Os1 Al5 Al1 157.76(3) 15_655 . ?
Al2 Al5 Al1 34.76(3) 13_655 . ?
Al2 Al5 Al1 97.15(3) . . ?
Al4 Al5 Al1 121.36(3) 9_655 . ?
Al4 Al5 Al1 76.03(3) 14 . ?
Al4 Al5 Al1 70.92(2) 7 . ?
Al4 Al5 Al1 130.83(3) 15_655 . ?
Al5 Al5 Al1 147.423(13) 2_655 . ?
Al5 Al5 Al1 87.580(13) 3_665 . ?
Y1 Al5 Al1 97.46(2) 13_655 . ?
Y1 Al5 Al1 46.225(18) . . ?
Al4 Al5 Al1 111.87(3) 8_665 . ?
Al4 Al5 Al1 113.05(3) 13_665 . ?
Al5 Al5 Al1 62.470(13) 13_655 . ?
Al3 Al5 Al1 129.34(2) 9_655 . ?
Al3 Al5 Al1 38.50(2) 14 . ?
Al2 Al5 Al1 61.88(2) 4_654 . ?
Al2 Al5 Al1 92.39(2) 16_556 . ?
Al1 Al5 Al1 124.94(3) 13_655 . ?
Os1 Al5 Al3 149.694(11) 14 15_655 ?
Os1 Al5 Al3 31.163(11) 15_655 15_655 ?
Al2 Al5 Al3 106.09(3) 13_655 15_655 ?
Al2 Al5 Al3 70.34(3) . 15_655 ?
Al4 Al5 Al3 90.36(2) 9_655 15_655 ?
Al4 Al5 Al3 91.00(2) 14 15_655 ?
Al4 Al5 Al3 147.59(3) 7 15_655 ?
Al4 Al5 Al3 35.274(19) 15_655 15_655 ?
Al5 Al5 Al3 66.567(17) 2_655 15_655 ?
Al5 Al5 Al3 117.770(15) 3_665 15_655 ?
Y1 Al5 Al3 43.507(15) 13_655 15_655 ?
Y1 Al5 Al3 132.65(2) . 15_655 ?
Al4 Al5 Al3 107.01(3) 8_665 15_655 ?
Al4 Al5 Al3 76.85(3) 13_665 15_655 ?
Al5 Al5 Al3 87.747(17) 13_655 15_655 ?
Al3 Al5 Al3 62.422(17) 9_655 15_655 ?
Al3 Al5 Al3 116.764(16) 14 15_655 ?
Al2 Al5 Al3 82.43(2) 4_654 15_655 ?
Al2 Al5 Al3 95.46(2) 16_556 15_655 ?
Al1 Al5 Al3 35.746(16) 13_655 15_655 ?
Al1 Al5 Al3 140.83(2) . 15_655 ?
Os1 Al5 Al3 31.161(12) 14 7 ?
Os1 Al5 Al3 149.696(11) 15_655 7 ?
Al2 Al5 Al3 70.34(3) 13_655 7 ?
Al2 Al5 Al3 106.09(3) . 7 ?
Al4 Al5 Al3 91.00(2) 9_655 7 ?
Al4 Al5 Al3 90.36(2) 14 7 ?
Al4 Al5 Al3 35.273(19) 7 7 ?
Al4 Al5 Al3 147.59(3) 15_655 7 ?
Al5 Al5 Al3 117.765(15) 2_655 7 ?
Al5 Al5 Al3 66.561(17) 3_665 7 ?
Y1 Al5 Al3 132.64(2) 13_655 7 ?
Y1 Al5 Al3 43.505(14) . 7 ?
Al4 Al5 Al3 76.85(3) 8_665 7 ?
Al4 Al5 Al3 107.01(3) 13_665 7 ?
Al5 Al5 Al3 87.743(17) 13_655 7 ?
Al3 Al5 Al3 116.764(17) 9_655 7 ?
Al3 Al5 Al3 62.418(17) 14 7 ?
Al2 Al5 Al3 95.46(2) 4_654 7 ?
Al2 Al5 Al3 82.43(2) 16_556 7 ?
Al1 Al5 Al3 140.83(2) 13_655 7 ?
Al1 Al5 Al3 35.744(16) . 7 ?
Al3 Al5 Al3 175.49(3) 15_655 7 ?
Os1 Al5 Al5 90.0 14 16_556 ?
Os1 Al5 Al5 90.0 15_655 16_556 ?
Al2 Al5 Al5 110.33(2) 13_655 16_556 ?
Al2 Al5 Al5 69.67(2) . 16_556 ?
Al4 Al5 Al5 34.80(3) 9_655 16_556 ?
Al4 Al5 Al5 145.19(3) 14 16_556 ?
Al4 Al5 Al5 37.90(3) 7 16_556 ?
Al4 Al5 Al5 142.10(3) 15_655 16_556 ?
Al5 Al5 Al5 90.0 2_655 16_556 ?
Al5 Al5 Al5 90.0 3_665 16_556 ?
Y1 Al5 Al5 132.363(12) 13_655 16_556 ?
Y1 Al5 Al5 47.639(12) . 16_556 ?
Al4 Al5 Al5 55.789(13) 8_665 16_556 ?
Al4 Al5 Al5 124.211(13) 13_665 16_556 ?
Al5 Al5 Al5 90.0 13_655 16_556 ?
Al3 Al5 Al5 58.251(9) 9_655 16_556 ?
Al3 Al5 Al5 121.747(9) 14 16_556 ?
Al2 Al5 Al5 144.694(15) 4_654 16_556 ?
Al2 Al5 Al5 35.305(15) 16_556 16_556 ?
Al1 Al5 Al5 93.336(16) 13_655 16_556 ?
Al1 Al5 Al5 86.665(16) . 16_556 ?
Al3 Al5 Al5 120.174(10) 15_655 16_556 ?
Al3 Al5 Al5 59.828(10) 7 16_556 ?
Os1 Al5 Al5 90.0 14 16 ?
Os1 Al5 Al5 90.0 15_655 16 ?
Al2 Al5 Al5 69.67(2) 13_655 16 ?
Al2 Al5 Al5 110.33(2) . 16 ?
Al4 Al5 Al5 145.20(3) 9_655 16 ?
Al4 Al5 Al5 34.81(3) 14 16 ?
Al4 Al5 Al5 142.10(3) 7 16 ?
Al4 Al5 Al5 37.90(3) 15_655 16 ?
Al5 Al5 Al5 90.0 2_655 16 ?
Al5 Al5 Al5 90.0 3_665 16 ?
Y1 Al5 Al5 47.637(12) 13_655 16 ?
Y1 Al5 Al5 132.362(12) . 16 ?
Al4 Al5 Al5 124.211(13) 8_665 16 ?
Al4 Al5 Al5 55.789(13) 13_665 16 ?
Al5 Al5 Al5 90.0 13_655 16 ?
Al3 Al5 Al5 121.749(9) 9_655 16 ?
Al3 Al5 Al5 58.253(9) 14 16 ?
Al2 Al5 Al5 35.306(15) 4_654 16 ?
Al2 Al5 Al5 144.695(15) 16_556 16 ?
Al1 Al5 Al5 86.664(16) 13_655 16 ?
Al1 Al5 Al5 93.336(16) . 16 ?
Al3 Al5 Al5 59.826(10) 15_655 16 ?
Al3 Al5 Al5 120.172(10) 7 16 ?
Al5 Al5 Al5 180.00(3) 16_556 16 ?
Os1 Al5 Os1 84.43(2) 14 13_665 ?
Os1 Al5 Os1 84.43(2) 15_655 13_665 ?
Al2 Al5 Os1 138.94(2) 13_655 13_665 ?
Al2 Al5 Os1 138.94(2) . 13_665 ?
Al4 Al5 Os1 72.43(4) 9_655 13_665 ?
Al4 Al5 Os1 72.43(4) 14 13_665 ?
Al4 Al5 Os1 69.28(3) 7 13_665 ?
Al4 Al5 Os1 69.28(3) 15_655 13_665 ?
Al5 Al5 Os1 30.0 2_655 13_665 ?
Al5 Al5 Os1 30.0 3_665 13_665 ?
Y1 Al5 Os1 127.441(14) 13_655 13_665 ?
Y1 Al5 Os1 127.440(14) . 13_665 ?
Al4 Al5 Os1 34.253(13) 8_665 13_665 ?
Al4 Al5 Os1 34.253(13) 13_665 13_665 ?
Al5 Al5 Os1 180.0 13_655 13_665 ?
Al3 Al5 Os1 99.26(2) 9_655 13_665 ?
Al3 Al5 Os1 99.26(2) 14 13_665 ?
Al2 Al5 Os1 117.693(14) 4_654 13_665 ?
Al2 Al5 Os1 117.693(14) 16_556 13_665 ?
Al1 Al5 Os1 117.529(13) 13_655 13_665 ?
Al1 Al5 Os1 117.527(13) . 13_665 ?
Al3 Al5 Os1 92.256(17) 15_655 13_665 ?
Al3 Al5 Os1 92.255(17) 7 13_665 ?
Al5 Al5 Os1 90.0 16_556 13_665 ?
Al5 Al5 Os1 90.0 16 13_665 ?
Os1 Al5 Al2 143.04(3) 14 14_665 ?
Os1 Al5 Al2 26.666(16) 15_655 14_665 ?
Al2 Al5 Al2 140.54(3) 13_655 14_665 ?
Al2 Al5 Al2 87.85(3) . 14_665 ?
Al4 Al5 Al2 66.71(3) 9_655 14_665 ?
Al4 Al5 Al2 95.82(3) 14 14_665 ?
Al4 Al5 Al2 114.33(3) 7 14_665 ?
Al4 Al5 Al2 40.84(3) 15_655 14_665 ?
Al5 Al5 Al2 32.116(16) 2_655 14_665 ?
Al5 Al5 Al2 90.195(16) 3_665 14_665 ?
Y1 Al5 Al2 78.744(15) 13_655 14_665 ?
Y1 Al5 Al2 141.949(15) . 14_665 ?
Al4 Al5 Al2 71.77(3) 8_665 14_665 ?
Al4 Al5 Al2 60.51(3) 13_665 14_665 ?
Al5 Al5 Al2 119.151(16) 13_655 14_665 ?
Al3 Al5 Al2 58.207(19) 9_655 14_665 ?
Al3 Al5 Al2 133.13(2) 14 14_665 ?
Al2 Al5 Al2 110.854(13) 4_654 14_665 ?
Al2 Al5 Al2 95.55(2) 16_556 14_665 ?
Al1 Al5 Al2 57.390(15) 13_655 14_665 ?
Al1 Al5 Al2 171.55(2) . 14_665 ?
Al3 Al5 Al2 35.383(18) 15_655 14_665 ?
Al3 Al5 Al2 148.61(2) 7 14_665 ?
Al5 Al5 Al2 101.488(13) 16_556 14_665 ?
Al5 Al5 Al2 78.512(13) 16 14_665 ?
Os1 Al5 Al2 60.852(16) 13_665 14_665 ?
Os1 Al5 Al2 26.665(16) 14 3_665 ?
Os1 Al5 Al2 143.04(3) 15_655 3_665 ?
Al2 Al5 Al2 87.85(3) 13_655 3_665 ?
Al2 Al5 Al2 140.54(3) . 3_665 ?
Al4 Al5 Al2 95.81(3) 9_655 3_665 ?
Al4 Al5 Al2 66.70(3) 14 3_665 ?
Al4 Al5 Al2 40.84(3) 7 3_665 ?
Al4 Al5 Al2 114.32(3) 15_655 3_665 ?
Al5 Al5 Al2 90.190(16) 2_655 3_665 ?
Al5 Al5 Al2 32.112(16) 3_665 3_665 ?
Y1 Al5 Al2 141.945(15) 13_655 3_665 ?
Y1 Al5 Al2 78.740(15) . 3_665 ?
Al4 Al5 Al2 60.51(3) 8_665 3_665 ?
Al4 Al5 Al2 71.77(3) 13_665 3_665 ?
Al5 Al5 Al2 119.145(16) 13_655 3_665 ?
Al3 Al5 Al2 133.13(2) 9_655 3_665 ?
Al3 Al5 Al2 58.204(19) 14 3_665 ?
Al2 Al5 Al2 95.55(2) 4_654 3_665 ?
Al2 Al5 Al2 110.852(13) 16_556 3_665 ?
Al1 Al5 Al2 171.56(2) 13_655 3_665 ?
Al1 Al5 Al2 57.388(15) . 3_665 ?
Al3 Al5 Al2 148.61(2) 15_655 3_665 ?
Al3 Al5 Al2 35.381(18) 7 3_665 ?
Al5 Al5 Al2 78.512(13) 16_556 3_665 ?
Al5 Al5 Al2 101.488(13) 16 3_665 ?
Os1 Al5 Al2 60.852(16) 13_665 3_665 ?
Al2 Al5 Al2 121.70(3) 14_665 3_665 ?
Os1 Al5 Os1 126.10(3) 14 2_655 ?
Os1 Al5 Os1 65.049(15) 15_655 2_655 ?
Al2 Al5 Os1 68.51(2) 13_655 2_655 ?
Al2 Al5 Os1 21.15(2) . 2_655 ?
Al4 Al5 Os1 90.81(3) 9_655 2_655 ?
Al4 Al5 Os1 120.41(4) 14 2_655 ?
Al4 Al5 Os1 124.04(3) 7 2_655 ?
Al4 Al5 Os1 92.85(2) 15_655 2_655 ?
Al5 Al5 Os1 119.478(5) 2_655 2_655 ?
Al5 Al5 Os1 179.477(5) 3_665 2_655 ?
Y1 Al5 Os1 42.524(12) 13_655 2_655 ?
Y1 Al5 Os1 71.920(16) . 2_655 ?
Al4 Al5 Os1 134.325(18) 8_665 2_655 ?
Al4 Al5 Os1 136.49(2) 13_665 2_655 ?
Al5 Al5 Os1 30.528(5) 13_655 2_655 ?
Al3 Al5 Os1 55.755(18) 9_655 2_655 ?
Al3 Al5 Os1 106.59(2) 14 2_655 ?
Al2 Al5 Os1 76.949(15) 4_654 2_655 ?
Al2 Al5 Os1 54.913(15) 16_556 2_655 ?
Al1 Al5 Os1 32.051(9) 13_655 2_655 ?
Al1 Al5 Os1 92.942(17) . 2_655 ?
Al3 Al5 Os1 61.800(13) 15_655 2_655 ?
Al3 Al5 Os1 113.88(2) 7 2_655 ?
Al5 Al5 Os1 90.0 16_556 2_655 ?
Al5 Al5 Os1 90.0 16 2_655 ?
Os1 Al5 Os1 149.475(5) 13_665 2_655 ?
Al2 Al5 Os1 89.293(14) 14_665 2_655 ?
Al2 Al5 Os1 148.372(19) 3_665 2_655 ?
Os1 Al5 Os1 65.046(15) 14 3 ?
Os1 Al5 Os1 126.10(3) 15_655 3 ?
Al2 Al5 Os1 21.14(2) 13_655 3 ?
Al2 Al5 Os1 68.51(2) . 3 ?
Al4 Al5 Os1 120.41(4) 9_655 3 ?
Al4 Al5 Os1 90.80(3) 14 3 ?
Al4 Al5 Os1 92.84(2) 7 3 ?
Al4 Al5 Os1 124.04(3) 15_655 3 ?
Al5 Al5 Os1 179.469(5) 2_655 3 ?
Al5 Al5 Os1 119.469(5) 3_665 3 ?
Y1 Al5 Os1 71.920(16) 13_655 3 ?
Y1 Al5 Os1 42.523(12) . 3 ?
Al4 Al5 Os1 136.49(2) 8_665 3 ?
Al4 Al5 Os1 134.322(18) 13_665 3 ?
Al5 Al5 Os1 30.526(5) 13_655 3 ?
Al3 Al5 Os1 106.59(2) 9_655 3 ?
Al3 Al5 Os1 55.753(18) 14 3 ?
Al2 Al5 Os1 54.912(15) 4_654 3 ?
Al2 Al5 Os1 76.949(15) 16_556 3 ?
Al1 Al5 Os1 92.944(17) 13_655 3 ?
Al1 Al5 Os1 32.049(9) . 3 ?
Al3 Al5 Os1 113.88(2) 15_655 3 ?
Al3 Al5 Os1 61.798(13) 7 3 ?
Al5 Al5 Os1 90.0 16_556 3 ?
Al5 Al5 Os1 90.0 16 3 ?
Os1 Al5 Os1 149.472(5) 13_665 3 ?
Al2 Al5 Os1 148.375(19) 14_665 3 ?
Al2 Al5 Os1 89.289(14) 3_665 3 ?
Os1 Al5 Os1 61.054(11) 2_655 3 ?
Al7 Al6 Y2 180.0 . . ?
Al7 Al6 Y3 180.0 . . ?
Y2 Al6 Y3 0.0 . . ?
Al7 Al6 Al6 0.0 . 13 ?
Y2 Al6 Al6 180.000(1) . 13 ?
Y3 Al6 Al6 180.000(1) . 13 ?
Al7 Al6 Y2 180.0 . 16_556 ?
Y2 Al6 Y2 0.0 . 16_556 ?
Y3 Al6 Y2 0.0 . 16_556 ?
Al6 Al6 Y2 180.0 13 16_556 ?
Al7 Al6 Al1 77.8(3) . . ?
Y2 Al6 Al1 102.2(3) . . ?
Y3 Al6 Al1 102.2(3) . . ?
Al6 Al6 Al1 77.8(3) 13 . ?
Y2 Al6 Al1 102.2(3) 16_556 . ?
Al7 Al6 Al1 77.8(3) . 3 ?
Y2 Al6 Al1 102.2(3) . 3 ?
Y3 Al6 Al1 102.2(3) . 3 ?
Al6 Al6 Al1 77.8(3) 13 3 ?
Y2 Al6 Al1 102.2(3) 16_556 3 ?
Al1 Al6 Al1 115.6(2) . 3 ?
Al7 Al6 Al1 77.8(3) . 2 ?
Y2 Al6 Al1 102.2(3) . 2 ?
Y3 Al6 Al1 102.2(3) . 2 ?
Al6 Al6 Al1 77.8(3) 13 2 ?
Y2 Al6 Al1 102.2(3) 16_556 2 ?
Al1 Al6 Al1 115.6(2) . 2 ?
Al1 Al6 Al1 115.6(2) 3 2 ?
Al7 Al6 Y2 0.0 . 13 ?
Y2 Al6 Y2 180.0 . 13 ?
Y3 Al6 Y2 180.0 . 13 ?
Al6 Al6 Y2 0.0 13 13 ?
Y2 Al6 Y2 180.0 16_556 13 ?
Al1 Al6 Y2 77.8(3) . 13 ?
Al1 Al6 Y2 77.8(3) 3 13 ?
Al1 Al6 Y2 77.8(3) 2 13 ?
Al7 Al6 Al1 67.5(3) . 14 ?
Y2 Al6 Al1 112.5(3) . 14 ?
Y3 Al6 Al1 112.5(3) . 14 ?
Al6 Al6 Al1 67.5(3) 13 14 ?
Y2 Al6 Al1 112.5(3) 16_556 14 ?
Al1 Al6 Al1 57.82(10) . 14 ?
Al1 Al6 Al1 57.82(10) 3 14 ?
Al1 Al6 Al1 145.3(6) 2 14 ?
Y2 Al6 Al1 67.5(3) 13 14 ?
Al7 Al6 Al1 67.5(3) . 13 ?
Y2 Al6 Al1 112.5(3) . 13 ?
Y3 Al6 Al1 112.5(3) . 13 ?
Al6 Al6 Al1 67.5(3) 13 13 ?
Y2 Al6 Al1 112.5(3) 16_556 13 ?
Al1 Al6 Al1 145.3(6) . 13 ?
Al1 Al6 Al1 57.82(10) 3 13 ?
Al1 Al6 Al1 57.82(10) 2 13 ?
Y2 Al6 Al1 67.5(3) 13 13 ?
Al1 Al6 Al1 106.3(3) 14 13 ?
Al7 Al6 Al1 67.5(3) . 15 ?
Y2 Al6 Al1 112.5(3) . 15 ?
Y3 Al6 Al1 112.5(3) . 15 ?
Al6 Al6 Al1 67.5(3) 13 15 ?
Y2 Al6 Al1 112.5(3) 16_556 15 ?
Al1 Al6 Al1 57.82(10) . 15 ?
Al1 Al6 Al1 145.3(6) 3 15 ?
Al1 Al6 Al1 57.82(10) 2 15 ?
Y2 Al6 Al1 67.5(3) 13 15 ?
Al1 Al6 Al1 106.3(3) 14 15 ?
Al1 Al6 Al1 106.3(3) 13 15 ?
Al7 Al6 Al6 180.000(1) . 16_556 ?
Y2 Al6 Al6 0.000(1) . 16_556 ?
Y3 Al6 Al6 0.0 . 16_556 ?
Al6 Al6 Al6 180.000(1) 13 16_556 ?
Y2 Al6 Al6 0.0 16_556 16_556 ?
Al1 Al6 Al6 102.2(3) . 16_556 ?
Al1 Al6 Al6 102.2(3) 3 16_556 ?
Al1 Al6 Al6 102.2(3) 2 16_556 ?
Y2 Al6 Al6 180.0 13 16_556 ?
Al1 Al6 Al6 112.5(3) 14 16_556 ?
Al1 Al6 Al6 112.5(3) 13 16_556 ?
Al1 Al6 Al6 112.5(3) 15 16_556 ?
Al7 Al6 Y3 0.0 . 13 ?
Y2 Al6 Y3 180.0 . 13 ?
Y3 Al6 Y3 180.0 . 13 ?
Al6 Al6 Y3 0.0 13 13 ?
Y2 Al6 Y3 180.0 16_556 13 ?
Al1 Al6 Y3 77.8(3) . 13 ?
Al1 Al6 Y3 77.8(3) 3 13 ?
Al1 Al6 Y3 77.8(3) 2 13 ?
Y2 Al6 Y3 0.0 13 13 ?
Al1 Al6 Y3 67.5(3) 14 13 ?
Al1 Al6 Y3 67.5(3) 13 13 ?
Al1 Al6 Y3 67.5(3) 15 13 ?
Al6 Al6 Y3 180.000(1) 16_556 13 ?
Al7 Al6 Y2 0.0 . 4_554 ?
Y2 Al6 Y2 180.0 . 4_554 ?
Y3 Al6 Y2 180.0 . 4_554 ?
Al6 Al6 Y2 0.0 13 4_554 ?
Y2 Al6 Y2 180.0 16_556 4_554 ?
Al1 Al6 Y2 77.8(3) . 4_554 ?
Al1 Al6 Y2 77.8(3) 3 4_554 ?
Al1 Al6 Y2 77.8(3) 2 4_554 ?
Y2 Al6 Y2 0.0 13 4_554 ?
Al1 Al6 Y2 67.5(3) 14 4_554 ?
Al1 Al6 Y2 67.5(3) 13 4_554 ?
Al1 Al6 Y2 67.5(3) 15 4_554 ?
Al6 Al6 Y2 180.000(1) 16_556 4_554 ?
Y3 Al6 Y2 0.0 13 4_554 ?
Al7 Al6 Al3 114.0(2) . 8 ?
Y2 Al6 Al3 66.0(2) . 8 ?
Y3 Al6 Al3 66.0(2) . 8 ?
Al6 Al6 Al3 114.0(2) 13 8 ?
Y2 Al6 Al3 66.0(2) 16_556 8 ?
Al1 Al6 Al3 90.24(8) . 8 ?
Al1 Al6 Al3 50.03(8) 3 8 ?
Al1 Al6 Al3 153.8(2) 2 8 ?
Y2 Al6 Al3 114.0(2) 13 8 ?
Al1 Al6 Al3 52.33(6) 14 8 ?
Al1 Al6 Al3 103.49(3) 13 8 ?
Al1 Al6 Al3 147.63(4) 15 8 ?
Al6 Al6 Al3 66.0(2) 16_556 8 ?
Y3 Al6 Al3 114.0(2) 13 8 ?
Y2 Al6 Al3 114.0(2) 4_554 8 ?
Al7 Al6 Al3 114.0(2) . 2 ?
Y2 Al6 Al3 66.0(2) . 2 ?
Y3 Al6 Al3 66.0(2) . 2 ?
Al6 Al6 Al3 114.0(2) 13 2 ?
Y2 Al6 Al3 66.0(2) 16_556 2 ?
Al1 Al6 Al3 153.8(2) . 2 ?
Al1 Al6 Al3 50.03(8) 3 2 ?
Al1 Al6 Al3 90.24(8) 2 2 ?
Y2 Al6 Al3 114.0(2) 13 2 ?
Al1 Al6 Al3 103.49(3) 14 2 ?
Al1 Al6 Al3 52.33(6) 13 2 ?
Al1 Al6 Al3 147.63(4) 15 2 ?
Al6 Al6 Al3 66.0(2) 16_556 2 ?
Y3 Al6 Al3 114.0(2) 13 2 ?
Y2 Al6 Al3 114.0(2) 4_554 2 ?
Al3 Al6 Al3 63.68(12) 8 2 ?
Al7 Al6 Al3 114.0(2) . 7 ?
Y2 Al6 Al3 66.0(2) . 7 ?
Y3 Al6 Al3 66.0(2) . 7 ?
Al6 Al6 Al3 114.0(2) 13 7 ?
Y2 Al6 Al3 66.0(2) 16_556 7 ?
Al1 Al6 Al3 50.04(8) . 7 ?
Al1 Al6 Al3 153.8(2) 3 7 ?
Al1 Al6 Al3 90.23(8) 2 7 ?
Y2 Al6 Al3 114.0(2) 13 7 ?
Al1 Al6 Al3 103.49(3) 14 7 ?
Al1 Al6 Al3 147.63(4) 13 7 ?
Al1 Al6 Al3 52.33(6) 15 7 ?
Al6 Al6 Al3 66.0(2) 16_556 7 ?
Y3 Al6 Al3 114.0(2) 13 7 ?
Y2 Al6 Al3 114.0(2) 4_554 7 ?
Al3 Al6 Al3 104.6(2) 8 7 ?
Al3 Al6 Al3 130.9(4) 2 7 ?
Al7 Al6 Al3 114.0(2) . . ?
Y2 Al6 Al3 66.0(2) . . ?
Y3 Al6 Al3 66.0(2) . . ?
Al6 Al6 Al3 114.0(2) 13 . ?
Y2 Al6 Al3 66.0(2) 16_556 . ?
Al1 Al6 Al3 90.24(8) . . ?
Al1 Al6 Al3 153.8(2) 3 . ?
Al1 Al6 Al3 50.03(8) 2 . ?
Y2 Al6 Al3 114.0(2) 13 . ?
Al1 Al6 Al3 147.63(4) 14 . ?
Al1 Al6 Al3 103.49(3) 13 . ?
Al1 Al6 Al3 52.33(6) 15 . ?
Al6 Al6 Al3 66.0(2) 16_556 . ?
Y3 Al6 Al3 114.0(2) 13 . ?
Y2 Al6 Al3 114.0(2) 4_554 . ?
Al3 Al6 Al3 130.9(4) 8 . ?
Al3 Al6 Al3 104.6(2) 2 . ?
Al3 Al6 Al3 44.90(9) 7 . ?
Al7 Al6 Al3 114.0(2) . 9 ?
Y2 Al6 Al3 66.0(2) . 9 ?
Y3 Al6 Al3 66.0(2) . 9 ?
Al6 Al6 Al3 114.0(2) 13 9 ?
Y2 Al6 Al3 66.0(2) 16_556 9 ?
Al1 Al6 Al3 153.8(2) . 9 ?
Al1 Al6 Al3 90.24(8) 3 9 ?
Al1 Al6 Al3 50.03(8) 2 9 ?
Y2 Al6 Al3 114.0(2) 13 9 ?
Al1 Al6 Al3 147.63(4) 14 9 ?
Al1 Al6 Al3 52.33(6) 13 9 ?
Al1 Al6 Al3 103.49(3) 15 9 ?
Al6 Al6 Al3 66.0(2) 16_556 9 ?
Y3 Al6 Al3 114.0(2) 13 9 ?
Y2 Al6 Al3 114.0(2) 4_554 9 ?
Al3 Al6 Al3 104.6(2) 8 9 ?
Al3 Al6 Al3 44.90(9) 2 9 ?
Al3 Al6 Al3 104.6(2) 7 9 ?
Al3 Al6 Al3 63.69(12) . 9 ?
Al7 Al6 Al3 114.0(2) . 3 ?
Y2 Al6 Al3 66.0(2) . 3 ?
Y3 Al6 Al3 66.0(2) . 3 ?
Al6 Al6 Al3 114.0(2) 13 3 ?
Y2 Al6 Al3 66.0(2) 16_556 3 ?
Al1 Al6 Al3 50.03(8) . 3 ?
Al1 Al6 Al3 90.24(8) 3 3 ?
Al1 Al6 Al3 153.8(2) 2 3 ?
Y2 Al6 Al3 114.0(2) 13 3 ?
Al1 Al6 Al3 52.33(6) 14 3 ?
Al1 Al6 Al3 147.63(4) 13 3 ?
Al1 Al6 Al3 103.49(3) 15 3 ?
Al6 Al6 Al3 66.0(2) 16_556 3 ?
Y3 Al6 Al3 114.0(2) 13 3 ?
Y2 Al6 Al3 114.0(2) 4_554 3 ?
Al3 Al6 Al3 44.90(9) 8 3 ?
Al3 Al6 Al3 104.6(2) 2 3 ?
Al3 Al6 Al3 63.69(12) 7 3 ?
Al3 Al6 Al3 104.6(2) . 3 ?
Al3 Al6 Al3 130.9(4) 9 3 ?
Al7 Al6 Al7 180.0 . 4 ?
Y2 Al6 Al7 0.0 . 4 ?
Y3 Al6 Al7 0.0 . 4 ?
Al6 Al6 Al7 180.0 13 4 ?
Y2 Al6 Al7 0.0 16_556 4 ?
Al1 Al6 Al7 102.2(3) . 4 ?
Al1 Al6 Al7 102.2(3) 3 4 ?
Al1 Al6 Al7 102.2(3) 2 4 ?
Y2 Al6 Al7 180.0 13 4 ?
Al1 Al6 Al7 112.5(3) 14 4 ?
Al1 Al6 Al7 112.5(3) 13 4 ?
Al1 Al6 Al7 112.5(3) 15 4 ?
Al6 Al6 Al7 0.000(1) 16_556 4 ?
Y3 Al6 Al7 180.0 13 4 ?
Y2 Al6 Al7 180.0 4_554 4 ?
Al3 Al6 Al7 66.0(2) 8 4 ?
Al3 Al6 Al7 66.0(2) 2 4 ?
Al3 Al6 Al7 66.0(2) 7 4 ?
Al3 Al6 Al7 66.0(2) . 4 ?
Al3 Al6 Al7 66.0(2) 9 4 ?
Al3 Al6 Al7 66.0(2) 3 4 ?
Al7 Al6 Al1 142.80(12) . 17_556 ?
Y2 Al6 Al1 37.20(12) . 17_556 ?
Y3 Al6 Al1 37.20(12) . 17_556 ?
Al6 Al6 Al1 142.80(12) 13 17_556 ?
Y2 Al6 Al1 37.20(12) 16_556 17_556 ?
Al1 Al6 Al1 117.7(3) . 17_556 ?
Al1 Al6 Al1 117.7(3) 3 17_556 ?
Al1 Al6 Al1 65.04(19) 2 17_556 ?
Y2 Al6 Al1 142.80(12) 13 17_556 ?
Al1 Al6 Al1 149.7(4) 14 17_556 ?
Al1 Al6 Al1 91.44(16) 13 17_556 ?
Al1 Al6 Al1 91.44(16) 15 17_556 ?
Al6 Al6 Al1 37.20(12) 16_556 17_556 ?
Y3 Al6 Al1 142.80(12) 13 17_556 ?
Y2 Al6 Al1 142.80(12) 4_554 17_556 ?
Al3 Al6 Al1 100.2(3) 8 17_556 ?
Al3 Al6 Al1 67.97(18) 2 17_556 ?
Al3 Al6 Al1 67.97(18) 7 17_556 ?
Al3 Al6 Al1 39.19(11) . 17_556 ?
Al3 Al6 Al1 39.19(11) 9 17_556 ?
Al3 Al6 Al1 100.2(3) 3 17_556 ?
Al7 Al6 Al1 37.20(12) 4 17_556 ?
Al7 Al6 Al1 142.80(12) . 16_556 ?
Y2 Al6 Al1 37.20(12) . 16_556 ?
Y3 Al6 Al1 37.20(12) . 16_556 ?
Al6 Al6 Al1 142.80(12) 13 16_556 ?
Y2 Al6 Al1 37.20(12) 16_556 16_556 ?
Al1 Al6 Al1 65.04(19) . 16_556 ?
Al1 Al6 Al1 117.7(3) 3 16_556 ?
Al1 Al6 Al1 117.7(3) 2 16_556 ?
Y2 Al6 Al1 142.80(12) 13 16_556 ?
Al1 Al6 Al1 91.44(16) 14 16_556 ?
Al1 Al6 Al1 149.7(4) 13 16_556 ?
Al1 Al6 Al1 91.44(16) 15 16_556 ?
Al6 Al6 Al1 37.20(12) 16_556 16_556 ?
Y3 Al6 Al1 142.80(12) 13 16_556 ?
Y2 Al6 Al1 142.80(12) 4_554 16_556 ?
Al3 Al6 Al1 67.97(18) 8 16_556 ?
Al3 Al6 Al1 100.2(3) 2 16_556 ?
Al3 Al6 Al1 39.19(11) 7 16_556 ?
Al3 Al6 Al1 67.97(18) . 16_556 ?
Al3 Al6 Al1 100.2(3) 9 16_556 ?
Al3 Al6 Al1 39.19(11) 3 16_556 ?
Al7 Al6 Al1 37.20(12) 4 16_556 ?
Al1 Al6 Al1 63.14(19) 17_556 16_556 ?
Al7 Al6 Al1 142.80(12) . 18_556 ?
Y2 Al6 Al1 37.20(12) . 18_556 ?
Y3 Al6 Al1 37.20(12) . 18_556 ?
Al6 Al6 Al1 142.80(12) 13 18_556 ?
Y2 Al6 Al1 37.20(12) 16_556 18_556 ?
Al1 Al6 Al1 117.7(3) . 18_556 ?
Al1 Al6 Al1 65.04(19) 3 18_556 ?
Al1 Al6 Al1 117.7(3) 2 18_556 ?
Y2 Al6 Al1 142.80(12) 13 18_556 ?
Al1 Al6 Al1 91.44(16) 14 18_556 ?
Al1 Al6 Al1 91.44(16) 13 18_556 ?
Al1 Al6 Al1 149.7(4) 15 18_556 ?
Al6 Al6 Al1 37.20(11) 16_556 18_556 ?
Y3 Al6 Al1 142.80(12) 13 18_556 ?
Y2 Al6 Al1 142.80(12) 4_554 18_556 ?
Al3 Al6 Al1 39.19(11) 8 18_556 ?
Al3 Al6 Al1 39.19(11) 2 18_556 ?
Al3 Al6 Al1 100.2(3) 7 18_556 ?
Al3 Al6 Al1 100.2(3) . 18_556 ?
Al3 Al6 Al1 67.97(18) 9 18_556 ?
Al3 Al6 Al1 67.97(18) 3 18_556 ?
Al7 Al6 Al1 37.20(12) 4 18_556 ?
Al1 Al6 Al1 63.14(19) 17_556 18_556 ?
Al1 Al6 Al1 63.14(19) 16_556 18_556 ?
Al7 Al6 Al3 46.28(13) . 20 ?
Y2 Al6 Al3 133.72(13) . 20 ?
Y3 Al6 Al3 133.72(13) . 20 ?
Al6 Al6 Al3 46.28(13) 13 20 ?
Y2 Al6 Al3 133.72(13) 16_556 20 ?
Al1 Al6 Al3 85.3(2) . 20 ?
Al1 Al6 Al3 115.5(4) 3 20 ?
Al1 Al6 Al3 37.99(16) 2 20 ?
Y2 Al6 Al3 46.28(13) 13 20 ?
Al1 Al6 Al3 110.0(4) 14 20 ?
Al1 Al6 Al3 71.0(2) 13 20 ?
Al1 Al6 Al3 35.97(13) 15 20 ?
Al6 Al6 Al3 133.72(13) 16_556 20 ?
Y3 Al6 Al3 46.28(13) 13 20 ?
Y2 Al6 Al3 46.28(13) 4_554 20 ?
Al3 Al6 Al3 160.3(3) 8 20 ?
Al3 Al6 Al3 120.07(12) 2 20 ?
Al3 Al6 Al3 87.21(8) 7 20 ?
Al3 Al6 Al3 68.44(8) . 20 ?
Al3 Al6 Al3 87.21(8) 9 20 ?
Al3 Al6 Al3 135.29(16) 3 20 ?
Al7 Al6 Al3 133.72(13) 4 20 ?
Al1 Al6 Al3 98.84(3) 17_556 20 ?
Al1 Al6 Al3 126.21(4) 16_556 20 ?
Al1 Al6 Al3 155.12(9) 18_556 20 ?
Al7 Al6 Al3 46.28(13) . 14 ?
Y2 Al6 Al3 133.72(13) . 14 ?
Y3 Al6 Al3 133.72(13) . 14 ?
Al6 Al6 Al3 46.28(13) 13 14 ?
Y2 Al6 Al3 133.72(13) 16_556 14 ?
Al1 Al6 Al3 37.99(16) . 14 ?
Al1 Al6 Al3 115.5(4) 3 14 ?
Al1 Al6 Al3 85.3(2) 2 14 ?
Y2 Al6 Al3 46.28(13) 13 14 ?
Al1 Al6 Al3 71.0(2) 14 14 ?
Al1 Al6 Al3 110.0(4) 13 14 ?
Al1 Al6 Al3 35.97(13) 15 14 ?
Al6 Al6 Al3 133.72(13) 16_556 14 ?
Y3 Al6 Al3 46.28(13) 13 14 ?
Y2 Al6 Al3 46.28(13) 4_554 14 ?
Al3 Al6 Al3 120.07(12) 8 14 ?
Al3 Al6 Al3 160.3(3) 2 14 ?
Al3 Al6 Al3 68.44(8) 7 14 ?
Al3 Al6 Al3 87.21(8) . 14 ?
Al3 Al6 Al3 135.29(16) 9 14 ?
Al3 Al6 Al3 87.21(8) 3 14 ?
Al7 Al6 Al3 133.72(13) 4 14 ?
Al1 Al6 Al3 126.21(4) 17_556 14 ?
Al1 Al6 Al3 98.84(3) 16_556 14 ?
Al1 Al6 Al3 155.12(9) 18_556 14 ?
Al3 Al6 Al3 49.35(12) 20 14 ?
Al7 Al6 Al3 46.28(13) . 19 ?
Y2 Al6 Al3 133.72(13) . 19 ?
Y3 Al6 Al3 133.72(13) . 19 ?
Al6 Al6 Al3 46.28(13) 13 19 ?
Y2 Al6 Al3 133.72(13) 16_556 19 ?
Al1 Al6 Al3 115.5(4) . 19 ?
Al1 Al6 Al3 37.99(16) 3 19 ?
Al1 Al6 Al3 85.3(2) 2 19 ?
Y2 Al6 Al3 46.28(13) 13 19 ?
Al1 Al6 Al3 71.0(2) 14 19 ?
Al1 Al6 Al3 35.97(13) 13 19 ?
Al1 Al6 Al3 110.0(4) 15 19 ?
Al6 Al6 Al3 133.72(13) 16_556 19 ?
Y3 Al6 Al3 46.28(13) 13 19 ?
Y2 Al6 Al3 46.28(13) 4_554 19 ?
Al3 Al6 Al3 87.21(9) 8 19 ?
Al3 Al6 Al3 68.44(8) 2 19 ?
Al3 Al6 Al3 160.3(3) 7 19 ?
Al3 Al6 Al3 135.29(16) . 19 ?
Al3 Al6 Al3 87.21(8) 9 19 ?
Al3 Al6 Al3 120.07(12) 3 19 ?
Al7 Al6 Al3 133.72(13) 4 19 ?
Al1 Al6 Al3 126.21(4) 17_556 19 ?
Al1 Al6 Al3 155.12(9) 16_556 19 ?
Al1 Al6 Al3 98.84(3) 18_556 19 ?
Al3 Al6 Al3 77.5(2) 20 19 ?
Al3 Al6 Al3 92.0(3) 14 19 ?
Al7 Al6 Al3 46.28(13) . 13 ?
Y2 Al6 Al3 133.72(13) . 13 ?
Y3 Al6 Al3 133.72(13) . 13 ?
Al6 Al6 Al3 46.28(13) 13 13 ?
Y2 Al6 Al3 133.72(13) 16_556 13 ?
Al1 Al6 Al3 85.3(2) . 13 ?
Al1 Al6 Al3 37.99(16) 3 13 ?
Al1 Al6 Al3 115.5(4) 2 13 ?
Y2 Al6 Al3 46.28(13) 13 13 ?
Al1 Al6 Al3 35.97(13) 14 13 ?
Al1 Al6 Al3 71.0(2) 13 13 ?
Al1 Al6 Al3 110.0(4) 15 13 ?
Al6 Al6 Al3 133.72(13) 16_556 13 ?
Y3 Al6 Al3 46.28(13) 13 13 ?
Y2 Al6 Al3 46.28(13) 4_554 13 ?
Al3 Al6 Al3 68.44(8) 8 13 ?
Al3 Al6 Al3 87.21(9) 2 13 ?
Al3 Al6 Al3 135.29(16) 7 13 ?
Al3 Al6 Al3 160.3(3) . 13 ?
Al3 Al6 Al3 120.07(12) 9 13 ?
Al3 Al6 Al3 87.21(8) 3 13 ?
Al7 Al6 Al3 133.72(13) 4 13 ?
Al1 Al6 Al3 155.12(9) 17_556 13 ?
Al1 Al6 Al3 126.21(4) 16_556 13 ?
Al1 Al6 Al3 98.84(3) 18_556 13 ?
Al3 Al6 Al3 92.0(3) 20 13 ?
Al3 Al6 Al3 77.5(2) 14 13 ?
Al3 Al6 Al3 35.17(9) 19 13 ?
Al7 Al6 Al3 46.28(13) . 21 ?
Y2 Al6 Al3 133.72(13) . 21 ?
Y3 Al6 Al3 133.72(13) . 21 ?
Al6 Al6 Al3 46.28(13) 13 21 ?
Y2 Al6 Al3 133.72(13) 16_556 21 ?
Al1 Al6 Al3 37.99(16) . 21 ?
Al1 Al6 Al3 85.3(2) 3 21 ?
Al1 Al6 Al3 115.5(4) 2 21 ?
Y2 Al6 Al3 46.28(13) 13 21 ?
Al1 Al6 Al3 35.97(13) 14 21 ?
Al1 Al6 Al3 110.0(4) 13 21 ?
Al1 Al6 Al3 71.0(2) 15 21 ?
Al6 Al6 Al3 133.72(13) 16_556 21 ?
Y3 Al6 Al3 46.28(13) 13 21 ?
Y2 Al6 Al3 46.28(13) 4_554 21 ?
Al3 Al6 Al3 87.21(8) 8 21 ?
Al3 Al6 Al3 135.29(16) 2 21 ?
Al3 Al6 Al3 87.21(8) 7 21 ?
Al3 Al6 Al3 120.07(12) . 21 ?
Al3 Al6 Al3 160.3(3) 9 21 ?
Al3 Al6 Al3 68.44(8) 3 21 ?
Al7 Al6 Al3 133.72(13) 4 21 ?
Al1 Al6 Al3 155.12(9) 17_556 21 ?
Al1 Al6 Al3 98.84(3) 16_556 21 ?
Al1 Al6 Al3 126.21(4) 18_556 21 ?
Al3 Al6 Al3 77.5(2) 20 21 ?
Al3 Al6 Al3 35.18(9) 14 21 ?
Al3 Al6 Al3 77.5(2) 19 21 ?
Al3 Al6 Al3 49.35(12) 13 21 ?
Al6 Al7 Al6 180.0 13 . ?
Al6 Al7 Y2 0.000(1) 13 13 ?
Al6 Al7 Y2 180.0 . 13 ?
Al6 Al7 Y2 180.0 13 . ?
Al6 Al7 Y2 0.000(1) . . ?
Y2 Al7 Y2 180.0 13 . ?
Al6 Al7 Y3 0.000(1) 13 13 ?
Al6 Al7 Y3 180.0 . 13 ?
Y2 Al7 Y3 0.0 13 13 ?
Y2 Al7 Y3 180.0 . 13 ?
Al6 Al7 Y3 180.0 13 . ?
Al6 Al7 Y3 0.000(1) . . ?
Y2 Al7 Y3 180.0 13 . ?
Y2 Al7 Y3 0.0 . . ?
Y3 Al7 Y3 180.0 13 . ?
Al6 Al7 Y2 180.0 13 16_556 ?
Al6 Al7 Y2 0.000(1) . 16_556 ?
Y2 Al7 Y2 180.0 13 16_556 ?
Y2 Al7 Y2 0.0 . 16_556 ?
Y3 Al7 Y2 180.0 13 16_556 ?
Y3 Al7 Y2 0.0 . 16_556 ?
Al6 Al7 Y2 0.000(1) 13 4_554 ?
Al6 Al7 Y2 180.0 . 4_554 ?
Y2 Al7 Y2 0.0 13 4_554 ?
Y2 Al7 Y2 180.0 . 4_554 ?
Y3 Al7 Y2 0.0 13 4_554 ?
Y3 Al7 Y2 180.0 . 4_554 ?
Y2 Al7 Y2 180.0 16_556 4_554 ?
Al6 Al7 Al1 95.62(3) 13 . ?
Al6 Al7 Al1 84.38(3) . . ?
Y2 Al7 Al1 95.62(3) 13 . ?
Y2 Al7 Al1 84.38(3) . . ?
Y3 Al7 Al1 95.62(3) 13 . ?
Y3 Al7 Al1 84.38(3) . . ?
Y2 Al7 Al1 84.38(3) 16_556 . ?
Y2 Al7 Al1 95.62(3) 4_554 . ?
Al6 Al7 Al1 84.38(3) 13 15 ?
Al6 Al7 Al1 95.62(3) . 15 ?
Y2 Al7 Al1 84.38(3) 13 15 ?
Y2 Al7 Al1 95.62(3) . 15 ?
Y3 Al7 Al1 84.38(3) 13 15 ?
Y3 Al7 Al1 95.62(3) . 15 ?
Y2 Al7 Al1 95.62(3) 16_556 15 ?
Y2 Al7 Al1 84.38(3) 4_554 15 ?
Al1 Al7 Al1 60.946(9) . 15 ?
Al6 Al7 Al1 95.62(3) 13 3 ?
Al6 Al7 Al1 84.38(3) . 3 ?
Y2 Al7 Al1 95.62(3) 13 3 ?
Y2 Al7 Al1 84.38(3) . 3 ?
Y3 Al7 Al1 95.62(3) 13 3 ?
Y3 Al7 Al1 84.38(3) . 3 ?
Y2 Al7 Al1 84.38(3) 16_556 3 ?
Y2 Al7 Al1 95.62(3) 4_554 3 ?
Al1 Al7 Al1 119.054(9) . 3 ?
Al1 Al7 Al1 180.00(4) 15 3 ?
Al6 Al7 Al1 84.38(3) 13 14 ?
Al6 Al7 Al1 95.62(3) . 14 ?
Y2 Al7 Al1 84.38(3) 13 14 ?
Y2 Al7 Al1 95.62(3) . 14 ?
Y3 Al7 Al1 84.38(3) 13 14 ?
Y3 Al7 Al1 95.62(3) . 14 ?
Y2 Al7 Al1 95.62(3) 16_556 14 ?
Y2 Al7 Al1 84.38(3) 4_554 14 ?
Al1 Al7 Al1 60.946(9) . 14 ?
Al1 Al7 Al1 119.054(9) 15 14 ?
Al1 Al7 Al1 60.946(9) 3 14 ?
Al6 Al7 Al1 95.62(3) 13 2 ?
Al6 Al7 Al1 84.38(3) . 2 ?
Y2 Al7 Al1 95.62(3) 13 2 ?
Y2 Al7 Al1 84.38(3) . 2 ?
Y3 Al7 Al1 95.62(3) 13 2 ?
Y3 Al7 Al1 84.38(3) . 2 ?
Y2 Al7 Al1 84.38(3) 16_556 2 ?
Y2 Al7 Al1 95.62(3) 4_554 2 ?
Al1 Al7 Al1 119.054(9) . 2 ?
Al1 Al7 Al1 60.946(9) 15 2 ?
Al1 Al7 Al1 119.054(9) 3 2 ?
Al1 Al7 Al1 180.000(5) 14 2 ?
Al6 Al7 Al1 84.38(3) 13 13 ?
Al6 Al7 Al1 95.62(3) . 13 ?
Y2 Al7 Al1 84.38(3) 13 13 ?
Y2 Al7 Al1 95.62(3) . 13 ?
Y3 Al7 Al1 84.38(3) 13 13 ?
Y3 Al7 Al1 95.62(3) . 13 ?
Y2 Al7 Al1 95.62(3) 16_556 13 ?
Y2 Al7 Al1 84.38(3) 4_554 13 ?
Al1 Al7 Al1 180.0 . 13 ?
Al1 Al7 Al1 119.054(9) 15 13 ?
Al1 Al7 Al1 60.946(9) 3 13 ?
Al1 Al7 Al1 119.054(9) 14 13 ?
Al1 Al7 Al1 60.946(9) 2 13 ?
Al6 Al7 Al6 180.0 13 16_556 ?
Al6 Al7 Al6 0.000(1) . 16_556 ?
Y2 Al7 Al6 180.0 13 16_556 ?
Y2 Al7 Al6 0.0 . 16_556 ?
Y3 Al7 Al6 180.0 13 16_556 ?
Y3 Al7 Al6 0.0 . 16_556 ?
Y2 Al7 Al6 0.0 16_556 16_556 ?
Y2 Al7 Al6 180.0 4_554 16_556 ?
Al1 Al7 Al6 84.38(3) . 16_556 ?
Al1 Al7 Al6 95.62(3) 15 16_556 ?
Al1 Al7 Al6 84.38(3) 3 16_556 ?
Al1 Al7 Al6 95.62(3) 14 16_556 ?
Al1 Al7 Al6 84.38(3) 2 16_556 ?
Al1 Al7 Al6 95.62(3) 13 16_556 ?
Al6 Al7 Al6 0.000(1) 13 4_554 ?
Al6 Al7 Al6 180.0 . 4_554 ?
Y2 Al7 Al6 0.0 13 4_554 ?
Y2 Al7 Al6 180.0 . 4_554 ?
Y3 Al7 Al6 0.0 13 4_554 ?
Y3 Al7 Al6 180.0 . 4_554 ?
Y2 Al7 Al6 180.0 16_556 4_554 ?
Y2 Al7 Al6 0.0 4_554 4_554 ?
Al1 Al7 Al6 95.62(3) . 4_554 ?
Al1 Al7 Al6 84.38(3) 15 4_554 ?
Al1 Al7 Al6 95.62(3) 3 4_554 ?
Al1 Al7 Al6 84.38(3) 14 4_554 ?
Al1 Al7 Al6 95.62(3) 2 4_554 ?
Al1 Al7 Al6 84.38(3) 13 4_554 ?
Al6 Al7 Al6 180.0 16_556 4_554 ?
Al6 Al7 Al3 54.967(10) 13 20 ?
Al6 Al7 Al3 125.033(10) . 20 ?
Y2 Al7 Al3 54.967(10) 13 20 ?
Y2 Al7 Al3 125.033(10) . 20 ?
Y3 Al7 Al3 54.967(10) 13 20 ?
Y3 Al7 Al3 125.033(10) . 20 ?
Y2 Al7 Al3 125.033(10) 16_556 20 ?
Y2 Al7 Al3 54.967(10) 4_554 20 ?
Al1 Al7 Al3 97.54(2) . 20 ?
Al1 Al7 Al3 43.83(3) 15 20 ?
Al1 Al7 Al3 136.17(3) 3 20 ?
Al1 Al7 Al3 133.16(3) 14 20 ?
Al1 Al7 Al3 46.84(3) 2 20 ?
Al1 Al7 Al3 82.46(2) 13 20 ?
Al6 Al7 Al3 125.033(10) 16_556 20 ?
Al6 Al7 Al3 54.967(10) 4_554 20 ?
Al6 Al7 Al3 125.033(10) 13 8 ?
Al6 Al7 Al3 54.967(10) . 8 ?
Y2 Al7 Al3 125.033(10) 13 8 ?
Y2 Al7 Al3 54.967(10) . 8 ?
Y3 Al7 Al3 125.033(10) 13 8 ?
Y3 Al7 Al3 54.967(10) . 8 ?
Y2 Al7 Al3 54.967(10) 16_556 8 ?
Y2 Al7 Al3 125.033(10) 4_554 8 ?
Al1 Al7 Al3 82.46(2) . 8 ?
Al1 Al7 Al3 136.17(3) 15 8 ?
Al1 Al7 Al3 43.83(3) 3 8 ?
Al1 Al7 Al3 46.84(3) 14 8 ?
Al1 Al7 Al3 133.16(3) 2 8 ?
Al1 Al7 Al3 97.54(2) 13 8 ?
Al6 Al7 Al3 54.967(10) 16_556 8 ?
Al6 Al7 Al3 125.033(10) 4_554 8 ?
Al3 Al7 Al3 180.00(2) 20 8 ?
Al6 Al7 Al3 54.967(10) 13 14 ?
Al6 Al7 Al3 125.033(10) . 14 ?
Y2 Al7 Al3 54.967(10) 13 14 ?
Y2 Al7 Al3 125.033(10) . 14 ?
Y3 Al7 Al3 54.967(10) 13 14 ?
Y3 Al7 Al3 125.033(10) . 14 ?
Y2 Al7 Al3 125.033(10) 16_556 14 ?
Y2 Al7 Al3 54.967(10) 4_554 14 ?
Al1 Al7 Al3 46.84(3) . 14 ?
Al1 Al7 Al3 43.83(3) 15 14 ?
Al1 Al7 Al3 136.17(3) 3 14 ?
Al1 Al7 Al3 82.46(2) 14 14 ?
Al1 Al7 Al3 97.54(2) 2 14 ?
Al1 Al7 Al3 133.16(3) 13 14 ?
Al6 Al7 Al3 125.033(10) 16_556 14 ?
Al6 Al7 Al3 54.967(10) 4_554 14 ?
Al3 Al7 Al3 56.45(3) 20 14 ?
Al3 Al7 Al3 123.55(3) 8 14 ?
Al6 Al7 Al3 125.033(10) 13 2 ?
Al6 Al7 Al3 54.967(10) . 2 ?
Y2 Al7 Al3 125.033(10) 13 2 ?
Y2 Al7 Al3 54.967(10) . 2 ?
Y3 Al7 Al3 125.033(10) 13 2 ?
Y3 Al7 Al3 54.967(10) . 2 ?
Y2 Al7 Al3 54.967(10) 16_556 2 ?
Y2 Al7 Al3 125.033(10) 4_554 2 ?
Al1 Al7 Al3 133.16(3) . 2 ?
Al1 Al7 Al3 136.17(3) 15 2 ?
Al1 Al7 Al3 43.83(3) 3 2 ?
Al1 Al7 Al3 97.54(2) 14 2 ?
Al1 Al7 Al3 82.46(2) 2 2 ?
Al1 Al7 Al3 46.84(3) 13 2 ?
Al6 Al7 Al3 54.967(10) 16_556 2 ?
Al6 Al7 Al3 125.033(10) 4_554 2 ?
Al3 Al7 Al3 123.55(3) 20 2 ?
Al3 Al7 Al3 56.45(3) 8 2 ?
Al3 Al7 Al3 180.00(4) 14 2 ?
Al6 Al7 Al3 54.967(10) 13 19 ?
Al6 Al7 Al3 125.033(10) . 19 ?
Y2 Al7 Al3 54.967(10) 13 19 ?
Y2 Al7 Al3 125.033(10) . 19 ?
Y3 Al7 Al3 54.967(10) 13 19 ?
Y3 Al7 Al3 125.033(10) . 19 ?
Y2 Al7 Al3 125.033(10) 16_556 19 ?
Y2 Al7 Al3 54.967(10) 4_554 19 ?
Al1 Al7 Al3 136.17(3) . 19 ?
Al1 Al7 Al3 133.16(3) 15 19 ?
Al1 Al7 Al3 46.84(3) 3 19 ?
Al1 Al7 Al3 82.46(2) 14 19 ?
Al1 Al7 Al3 97.54(2) 2 19 ?
Al1 Al7 Al3 43.83(3) 13 19 ?
Al6 Al7 Al3 125.033(10) 16_556 19 ?
Al6 Al7 Al3 54.967(10) 4_554 19 ?
Al3 Al7 Al3 90.327(15) 20 19 ?
Al3 Al7 Al3 89.673(15) 8 19 ?
Al3 Al7 Al3 109.24(2) 14 19 ?
Al3 Al7 Al3 70.76(2) 2 19 ?
Al6 Al7 Al3 125.033(10) 13 7 ?
Al6 Al7 Al3 54.967(10) . 7 ?
Y2 Al7 Al3 125.033(10) 13 7 ?
Y2 Al7 Al3 54.967(10) . 7 ?
Y3 Al7 Al3 125.033(10) 13 7 ?
Y3 Al7 Al3 54.967(10) . 7 ?
Y2 Al7 Al3 54.967(10) 16_556 7 ?
Y2 Al7 Al3 125.033(10) 4_554 7 ?
Al1 Al7 Al3 43.83(3) . 7 ?
Al1 Al7 Al3 46.84(3) 15 7 ?
Al1 Al7 Al3 133.16(3) 3 7 ?
Al1 Al7 Al3 97.54(2) 14 7 ?
Al1 Al7 Al3 82.46(2) 2 7 ?
Al1 Al7 Al3 136.17(3) 13 7 ?
Al6 Al7 Al3 54.967(10) 16_556 7 ?
Al6 Al7 Al3 125.033(10) 4_554 7 ?
Al3 Al7 Al3 89.673(15) 20 7 ?
Al3 Al7 Al3 90.327(15) 8 7 ?
Al3 Al7 Al3 70.76(2) 14 7 ?
Al3 Al7 Al3 109.24(2) 2 7 ?
Al3 Al7 Al3 180.00(4) 19 7 ?
Al6 Al7 Al3 54.967(10) 13 13 ?
Al6 Al7 Al3 125.033(10) . 13 ?
Y2 Al7 Al3 54.967(10) 13 13 ?
Y2 Al7 Al3 125.033(10) . 13 ?
Y3 Al7 Al3 54.967(10) 13 13 ?
Y3 Al7 Al3 125.033(10) . 13 ?
Y2 Al7 Al3 125.033(10) 16_556 13 ?
Y2 Al7 Al3 54.967(10) 4_554 13 ?
Al1 Al7 Al3 97.54(2) . 13 ?
Al1 Al7 Al3 133.16(3) 15 13 ?
Al1 Al7 Al3 46.84(3) 3 13 ?
Al1 Al7 Al3 43.83(3) 14 13 ?
Al1 Al7 Al3 136.17(3) 2 13 ?
Al1 Al7 Al3 82.46(2) 13 13 ?
Al6 Al7 Al3 125.033(10) 16_556 13 ?
Al6 Al7 Al3 54.967(10) 4_554 13 ?
Al3 Al7 Al3 109.24(2) 20 13 ?
Al3 Al7 Al3 70.76(2) 8 13 ?
Al3 Al7 Al3 90.327(15) 14 13 ?
Al3 Al7 Al3 89.673(15) 2 13 ?
Al3 Al7 Al3 40.04(4) 19 13 ?
Al3 Al7 Al3 139.96(4) 7 13 ?
Al6 Al7 Al3 125.033(10) 13 . ?
Al6 Al7 Al3 54.967(10) . . ?
Y2 Al7 Al3 125.033(10) 13 . ?
Y2 Al7 Al3 54.967(10) . . ?
Y3 Al7 Al3 125.033(10) 13 . ?
Y3 Al7 Al3 54.967(10) . . ?
Y2 Al7 Al3 54.967(10) 16_556 . ?
Y2 Al7 Al3 125.033(10) 4_554 . ?
Al1 Al7 Al3 82.46(2) . . ?
Al1 Al7 Al3 46.84(3) 15 . ?
Al1 Al7 Al3 133.16(3) 3 . ?
Al1 Al7 Al3 136.17(3) 14 . ?
Al1 Al7 Al3 43.83(3) 2 . ?
Al1 Al7 Al3 97.54(2) 13 . ?
Al6 Al7 Al3 54.967(10) 16_556 . ?
Al6 Al7 Al3 125.033(10) 4_554 . ?
Al3 Al7 Al3 70.76(2) 20 . ?
Al3 Al7 Al3 109.24(2) 8 . ?
Al3 Al7 Al3 89.673(14) 14 . ?
Al3 Al7 Al3 90.327(14) 2 . ?
Al3 Al7 Al3 139.96(4) 19 . ?
Al3 Al7 Al3 40.04(4) 7 . ?
Al3 Al7 Al3 180.0 13 . ?
Al6 Al7 Al3 54.967(10) 13 21 ?
Al6 Al7 Al3 125.033(10) . 21 ?
Y2 Al7 Al3 54.967(10) 13 21 ?
Y2 Al7 Al3 125.033(10) . 21 ?
Y3 Al7 Al3 54.967(10) 13 21 ?
Y3 Al7 Al3 125.033(10) . 21 ?
Y2 Al7 Al3 125.033(10) 16_556 21 ?
Y2 Al7 Al3 54.967(10) 4_554 21 ?
Al1 Al7 Al3 46.84(3) . 21 ?
Al1 Al7 Al3 82.46(2) 15 21 ?
Al1 Al7 Al3 97.54(2) 3 21 ?
Al1 Al7 Al3 43.83(3) 14 21 ?
Al1 Al7 Al3 136.17(3) 2 21 ?
Al1 Al7 Al3 133.16(3) 13 21 ?
Al6 Al7 Al3 125.033(10) 16_556 21 ?
Al6 Al7 Al3 54.967(10) 4_554 21 ?
Al3 Al7 Al3 90.326(15) 20 21 ?
Al3 Al7 Al3 89.674(15) 8 21 ?
Al3 Al7 Al3 40.04(4) 14 21 ?
Al3 Al7 Al3 139.96(4) 2 21 ?
Al3 Al7 Al3 90.326(15) 19 21 ?
Al3 Al7 Al3 89.674(15) 7 21 ?
Al3 Al7 Al3 56.46(3) 13 21 ?
Al3 Al7 Al3 123.55(3) . 21 ?
Al6 Al7 Al3 125.033(10) 13 9 ?
Al6 Al7 Al3 54.967(10) . 9 ?
Y2 Al7 Al3 125.033(10) 13 9 ?
Y2 Al7 Al3 54.967(10) . 9 ?
Y3 Al7 Al3 125.033(10) 13 9 ?
Y3 Al7 Al3 54.967(10) . 9 ?
Y2 Al7 Al3 54.967(10) 16_556 9 ?
Y2 Al7 Al3 125.033(10) 4_554 9 ?
Al1 Al7 Al3 133.16(3) . 9 ?
Al1 Al7 Al3 97.54(2) 15 9 ?
Al1 Al7 Al3 82.46(2) 3 9 ?
Al1 Al7 Al3 136.17(3) 14 9 ?
Al1 Al7 Al3 43.83(3) 2 9 ?
Al1 Al7 Al3 46.84(3) 13 9 ?
Al6 Al7 Al3 54.967(10) 16_556 9 ?
Al6 Al7 Al3 125.033(10) 4_554 9 ?
Al3 Al7 Al3 89.674(15) 20 9 ?
Al3 Al7 Al3 90.326(15) 8 9 ?
Al3 Al7 Al3 139.96(4) 14 9 ?
Al3 Al7 Al3 40.04(4) 2 9 ?
Al3 Al7 Al3 89.674(15) 19 9 ?
Al3 Al7 Al3 90.326(15) 7 9 ?
Al3 Al7 Al3 123.54(3) 13 9 ?
Al3 Al7 Al3 56.45(3) . 9 ?
Al3 Al7 Al3 180.00(5) 21 9 ?
Al6 Al7 Al3 54.967(10) 13 15 ?
Al6 Al7 Al3 125.033(10) . 15 ?
Y2 Al7 Al3 54.967(10) 13 15 ?
Y2 Al7 Al3 125.033(10) . 15 ?
Y3 Al7 Al3 54.967(10) 13 15 ?
Y3 Al7 Al3 125.033(10) . 15 ?
Y2 Al7 Al3 125.033(10) 16_556 15 ?
Y2 Al7 Al3 54.967(10) 4_554 15 ?
Al1 Al7 Al3 136.17(3) . 15 ?
Al1 Al7 Al3 82.46(2) 15 15 ?
Al1 Al7 Al3 97.54(2) 3 15 ?
Al1 Al7 Al3 133.16(3) 14 15 ?
Al1 Al7 Al3 46.84(3) 2 15 ?
Al1 Al7 Al3 43.83(3) 13 15 ?
Al6 Al7 Al3 125.033(10) 16_556 15 ?
Al6 Al7 Al3 54.967(10) 4_554 15 ?
Al3 Al7 Al3 40.04(4) 20 15 ?
Al3 Al7 Al3 139.96(4) 8 15 ?
Al3 Al7 Al3 90.326(15) 14 15 ?
Al3 Al7 Al3 89.674(15) 2 15 ?
Al3 Al7 Al3 56.46(3) 19 15 ?
Al3 Al7 Al3 123.54(3) 7 15 ?
Al3 Al7 Al3 90.326(15) 13 15 ?
Al3 Al7 Al3 89.673(15) . 15 ?
Al3 Al7 Al3 109.24(2) 21 15 ?
Al3 Al7 Al3 70.76(2) 9 15 ?
Al6 Al7 Al3 125.033(10) 13 3 ?
Al6 Al7 Al3 54.967(10) . 3 ?
Y2 Al7 Al3 125.033(10) 13 3 ?
Y2 Al7 Al3 54.967(10) . 3 ?
Y3 Al7 Al3 125.033(10) 13 3 ?
Y3 Al7 Al3 54.967(10) . 3 ?
Y2 Al7 Al3 54.967(10) 16_556 3 ?
Y2 Al7 Al3 125.033(10) 4_554 3 ?
Al1 Al7 Al3 43.83(3) . 3 ?
Al1 Al7 Al3 97.54(2) 15 3 ?
Al1 Al7 Al3 82.46(2) 3 3 ?
Al1 Al7 Al3 46.84(3) 14 3 ?
Al1 Al7 Al3 133.16(3) 2 3 ?
Al1 Al7 Al3 136.17(3) 13 3 ?
Al6 Al7 Al3 54.967(10) 16_556 3 ?
Al6 Al7 Al3 125.033(10) 4_554 3 ?
Al3 Al7 Al3 139.96(4) 20 3 ?
Al3 Al7 Al3 40.04(4) 8 3 ?
Al3 Al7 Al3 89.674(15) 14 3 ?
Al3 Al7 Al3 90.326(15) 2 3 ?
Al3 Al7 Al3 123.54(3) 19 3 ?
Al3 Al7 Al3 56.46(3) 7 3 ?
Al3 Al7 Al3 89.674(15) 13 3 ?
Al3 Al7 Al3 90.327(15) . 3 ?
Al3 Al7 Al3 70.76(2) 21 3 ?
Al3 Al7 Al3 109.24(2) 9 3 ?
Al3 Al7 Al3 180.00(2) 15 3 ?
Al6 Al7 Al7 180.0 13 4 ?
Al6 Al7 Al7 0.000(1) . 4 ?
Y2 Al7 Al7 180.0 13 4 ?
Y2 Al7 Al7 0.0 . 4 ?
Y3 Al7 Al7 180.0 13 4 ?
Y3 Al7 Al7 0.0 . 4 ?
Y2 Al7 Al7 0.0 16_556 4 ?
Y2 Al7 Al7 180.0 4_554 4 ?
Al1 Al7 Al7 84.38(3) . 4 ?
Al1 Al7 Al7 95.62(3) 15 4 ?
Al1 Al7 Al7 84.38(3) 3 4 ?
Al1 Al7 Al7 95.62(3) 14 4 ?
Al1 Al7 Al7 84.38(3) 2 4 ?
Al1 Al7 Al7 95.62(3) 13 4 ?
Al6 Al7 Al7 0.000(1) 16_556 4 ?
Al6 Al7 Al7 180.0 4_554 4 ?
Al3 Al7 Al7 125.033(10) 20 4 ?
Al3 Al7 Al7 54.967(10) 8 4 ?
Al3 Al7 Al7 125.033(10) 14 4 ?
Al3 Al7 Al7 54.967(10) 2 4 ?
Al3 Al7 Al7 125.033(10) 19 4 ?
Al3 Al7 Al7 54.967(10) 7 4 ?
Al3 Al7 Al7 125.033(10) 13 4 ?
Al3 Al7 Al7 54.967(10) . 4 ?
Al3 Al7 Al7 125.033(10) 21 4 ?
Al3 Al7 Al7 54.967(10) 9 4 ?
Al3 Al7 Al7 125.033(10) 15 4 ?
Al3 Al7 Al7 54.967(10) 3 4 ?
Al6 Al7 Al7 0.000(1) 13 4_554 ?
Al6 Al7 Al7 180.0 . 4_554 ?
Y2 Al7 Al7 0.0 13 4_554 ?
Y2 Al7 Al7 180.0 . 4_554 ?
Y3 Al7 Al7 0.0 13 4_554 ?
Y3 Al7 Al7 180.0 . 4_554 ?
Y2 Al7 Al7 180.0 16_556 4_554 ?
Y2 Al7 Al7 0.0 4_554 4_554 ?
Al1 Al7 Al7 95.62(3) . 4_554 ?
Al1 Al7 Al7 84.38(3) 15 4_554 ?
Al1 Al7 Al7 95.62(3) 3 4_554 ?
Al1 Al7 Al7 84.38(3) 14 4_554 ?
Al1 Al7 Al7 95.62(3) 2 4_554 ?
Al1 Al7 Al7 84.38(3) 13 4_554 ?
Al6 Al7 Al7 180.0 16_556 4_554 ?
Al6 Al7 Al7 0.000(1) 4_554 4_554 ?
Al3 Al7 Al7 54.967(10) 20 4_554 ?
Al3 Al7 Al7 125.033(10) 8 4_554 ?
Al3 Al7 Al7 54.967(10) 14 4_554 ?
Al3 Al7 Al7 125.033(10) 2 4_554 ?
Al3 Al7 Al7 54.967(10) 19 4_554 ?
Al3 Al7 Al7 125.033(10) 7 4_554 ?
Al3 Al7 Al7 54.967(10) 13 4_554 ?
Al3 Al7 Al7 125.033(10) . 4_554 ?
Al3 Al7 Al7 54.967(10) 21 4_554 ?
Al3 Al7 Al7 125.033(10) 9 4_554 ?
Al3 Al7 Al7 54.967(10) 15 4_554 ?
Al3 Al7 Al7 125.033(10) 3 4_554 ?
Al7 Al7 Al7 180.0 4 4_554 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Y1 Al4 3.0490(15) 7 ?
Y1 Al4 3.0490(15) 3 ?
Y1 Al3 3.0934(14) 3 ?
Y1 Al3 3.0935(14) 7 ?
Y1 Al1 3.1963(13) 16_556 ?
Y1 Al1 3.1964(13) . ?
Y1 Al2 3.1974(13) 13_655 ?
Y1 Al2 3.1974(13) 4_655 ?
Y1 Al2 3.1976(12) 16_556 ?
Y1 Al2 3.1976(12) . ?
Y1 Al5 3.3504(7) . ?
Y1 Al5 3.3504(7) 16_556 ?
Y1 Al5 3.3503(7) 13_655 ?
Y1 Al5 3.3503(7) 4_655 ?
Y1 Os1 3.4093(5) 5 ?
Y1 Os1 3.4093(5) 14 ?
Y1 Os1 3.4093(5) 3 ?
Y1 Os1 3.4093(5) 18_556 ?
Y1 Al4 3.9650(17) 9_655 ?
Y1 Al4 3.9650(17) 2_655 ?
Y1 Al1 5.0827(9) 14 ?
Y1 Al1 5.0827(10) 6 ?
Y1 Al1 5.0827(9) 5 ?
Y1 Al1 5.0827(10) 15 ?
Y1 Os1 5.0960(8) 17_656 ?
Y1 Os1 5.0960(8) 2_655 ?
Y1 Os1 5.0960(8) 6_655 ?
Y1 Os1 5.0960(8) 15_655 ?
Y1 Y3 5.1004(9) . ?
Y1 Y2 5.1097(9) . ?
Y2 Y2 0.616(8) 16_556 ?
Y2 Al6 1.127(15) . ?
Y2 Al6 1.743(15) 16_556 ?
Y2 Al7 1.950(4) . ?
Y2 Al7 2.565(4) 4 ?
Y2 Al6 2.772(15) 13 ?
Y2 Al1 3.109(3) . ?
Y2 Al1 3.109(3) 3 ?
Y2 Al1 3.109(3) 2 ?
Y2 Al3 3.2347(11) 8 ?
Y2 Al3 3.2347(11) 2 ?
Y2 Al3 3.2348(11) 7 ?
Y2 Al3 3.2348(11) . ?
Y2 Al3 3.2348(11) 9 ?
Y2 Al3 3.2348(11) 3 ?
Y2 Al6 3.388(15) 4 ?
Y2 Al1 3.416(3) 14 ?
Y2 Al1 3.416(3) 13 ?
Y2 Al1 3.416(3) 15 ?
Y2 Al1 3.483(3) 17_556 ?
Y2 Al1 3.483(3) 16_556 ?
Y2 Al1 3.483(3) 18_556 ?
Y2 Al1 3.842(3) 6 ?
Y2 Al1 3.842(3) 5 ?
Y2 Al1 3.842(3) 4 ?
Y2 Y2 3.899(8) 13 ?
Y2 Y3 4.207(4) 13 ?
Y2 Y2 4.5150(10) 4 ?
Y2 Y2 4.5150(10) 4_554 ?
Y2 Y3 4.823(4) 13_556 ?
Y3 Y2 0.308(4) 16_556 ?
Y3 Al6 1.435(14) . ?
Y3 Al6 1.435(14) 16_556 ?
Y3 Al7 2.2575(5) 4 ?
Y3 Al7 2.2575(5) . ?
Y3 Al6 3.080(14) 4 ?
Y3 Al6 3.080(14) 13 ?
Y3 Al3 3.2201(10) 8 ?
Y3 Al3 3.2201(10) 2 ?
Y3 Al3 3.2201(10) 7 ?
Y3 Al3 3.2201(10) . ?
Y3 Al3 3.2201(10) 9 ?
Y3 Al3 3.2201(10) 3 ?
Y3 Al1 3.2872(12) . ?
Y3 Al1 3.2872(12) 3 ?
Y3 Al1 3.2872(12) 17_556 ?
Y3 Al1 3.2872(12) 16_556 ?
Y3 Al1 3.2872(12) 18_556 ?
Y3 Al1 3.2872(12) 2 ?
Y3 Al1 3.6223(13) 6 ?
Y3 Al1 3.6223(13) 14 ?
Y3 Al1 3.6223(13) 13 ?
Y3 Al1 3.6223(13) 15 ?
Y3 Al1 3.6223(13) 5 ?
Y3 Al1 3.6223(13) 4 ?
Y3 Y2 4.207(4) 4 ?
Y3 Y2 4.207(4) 13 ?
Y3 Y3 4.5150(10) 13_556 ?
Y3 Y3 4.5150(10) 13 ?
Y3 Y2 4.823(4) 4_554 ?
Os1 Al5 2.5610(4) 15 ?
Os1 Al5 2.5608(4) 14_565 ?
Os1 Al4 2.6297(6) . ?
Os1 Al4 2.6297(6) 20 ?
Os1 Al3 2.6546(7) . ?
Os1 Al3 2.6546(7) 20 ?
Os1 Al1 2.6672(7) 15 ?
Os1 Al1 2.6672(7) 2 ?
Os1 Al2 2.6819(7) 3_665 ?
Os1 Al2 2.6819(7) 14_565 ?
Os1 Y1 3.4093(5) 15 ?
Os1 Y1 3.4093(5) 2 ?
Os1 Al2 4.3708(11) 18_666 ?
Os1 Al2 4.3708(11) 5_564 ?
Os1 Al3 4.3995(12) 7 ?
Os1 Al3 4.3995(12) 15 ?
Os1 Os1 4.5150(10) 16_556 ?
Os1 Os1 4.5150(10) 16 ?
Os1 Al4 4.5269(11) 19_665 ?
Os1 Al4 4.5269(11) 3_565 ?
Os1 Os1 4.5711(7) 15 ?
Os1 Al7 4.5711(7) . ?
Os1 Os1 4.5712(7) 14 ?
Os1 Al4 4.6437(15) 2_665 ?
Os1 Al4 4.6437(15) 21_565 ?
Os1 Al6 4.644(3) 13 ?
Os1 Al6 4.644(3) . ?
Os1 Al5 4.6634(12) 13_665 ?
Os1 Al2 4.7479(12) 15 ?
Os1 Al2 4.7479(12) 2 ?
Al1 Al7 2.6205(12) . ?
Al1 Os1 2.6672(7) 3 ?
Al1 Os1 2.6673(7) 14 ?
Al1 Al2 2.6755(16) 13_655 ?
Al1 Al1 2.6579(13) 14 ?
Al1 Al1 2.6579(13) 15 ?
Al1 Al6 2.669(3) . ?
Al1 Al3 2.7321(11) 7 ?
Al1 Al3 2.7321(11) 3 ?
Al1 Al6 2.822(6) 13 ?
Al1 Al3 2.8694(13) 14 ?
Al1 Al3 2.8694(13) 21 ?
Al1 Y2 3.416(3) 13 ?
Al1 Y2 3.483(3) 16_556 ?
Al1 Y3 3.6223(13) 13 ?
Al1 Y2 3.842(3) 4_554 ?
Al1 Al1 4.002(3) 16_556 ?
Al1 Al6 4.314(11) 16_556 ?
Al1 Al2 4.3864(11) 3_665 ?
Al1 Al2 4.3864(11) 2_545 ?
Al1 Al5 4.4070(13) . ?
Al1 Al5 4.4068(13) 13_655 ?
Al1 Al4 4.4005(13) 7 ?
Al1 Al4 4.4005(13) 3 ?
Al1 Al3 4.4303(15) . ?
Al1 Al3 4.4303(15) 8 ?
Al1 Al2 4.5192(18) 4_654 ?
Al2 Al2 2.638(2) 16_556 ?
Al2 Al1 2.6754(16) 13_655 ?
Al2 Os1 2.6818(7) 2_655 ?
Al2 Os1 2.6818(7) 15_655 ?
Al2 Al5 2.7011(10) . ?
Al2 Al5 2.7012(10) 13_655 ?
Al2 Al3 2.8045(13) 9_655 ?
Al2 Al3 2.8046(13) 2_655 ?
Al2 Al4 3.1606(16) 9_655 ?
Al2 Al4 3.1606(16) 2_655 ?
Al2 Y1 3.1974(13) 13_655 ?
Al2 Al2 3.548(2) 13_655 ?
Al2 Os1 4.3708(11) 17_656 ?
Al2 Os1 4.3708(11) 6_655 ?
Al2 Al5 4.3827(12) 16_556 ?
Al2 Al5 4.3827(12) 4_655 ?
Al2 Al1 4.3863(12) 2_655 ?
Al2 Al1 4.3863(11) 3_655 ?
Al2 Al3 4.3938(14) 15_655 ?
Al2 Al3 4.3938(14) 19_655 ?
Al2 Al4 4.4174(14) 19_655 ?
Al2 Al4 4.4174(14) 15_655 ?
Al2 Al4 4.4378(19) 3 ?
Al2 Al4 4.4378(19) 7 ?
Al2 Al1 4.5191(18) 4_655 ?
Al2 Al5 4.7116(9) 15_545 ?
Al2 Al5 4.7117(8) 2_655 ?
Al2 Os1 4.7479(12) 14 ?
Al2 Os1 4.7480(12) 3 ?
Al3 Os1 2.6546(7) 16_556 ?
Al3 Al3 2.693(3) 7 ?
Al3 Al4 2.7161(15) . ?
Al3 Al1 2.7321(11) 2 ?
Al3 Al1 2.7321(11) 17_556 ?
Al3 Al2 2.8046(13) 18_666 ?
Al3 Al2 2.8046(13) 3_665 ?
Al3 Al1 2.8693(13) 15 ?
Al3 Al1 2.8693(13) 6 ?
Al3 Y1 3.0935(14) 2 ?
Al3 Y2 3.2348(11) 16_556 ?
Al3 Al6 3.525(6) . ?
Al3 Al6 3.526(6) 16_556 ?
Al3 Al3 3.7200(19) 9 ?
Al3 Al7 3.9326(9) . ?
Al3 Al7 3.9326(9) 4 ?
Al3 Al5 4.2904(9) 6 ?
Al3 Al5 4.2904(9) 15 ?
Al3 Al2 4.3938(14) 14_565 ?
Al3 Al2 4.3938(14) 5_565 ?
Al3 Os1 4.3996(12) 5 ?
Al3 Os1 4.3996(12) 14 ?
Al3 Al6 4.456(10) 13 ?
Al3 Al6 4.456(10) 4 ?
Al3 Al1 4.4304(15) 16_556 ?
Al3 Al5 4.4914(12) 5_565 ?
Al4 Os1 2.6297(6) 16_556 ?
Al4 Al5 2.7494(10) 6 ?
Al4 Al5 2.7494(10) 15 ?
Al4 Al4 2.7746(18) 2_665 ?
Al4 Al4 2.7746(18) 3_565 ?
Al4 Al5 2.8609(12) 14_565 ?
Al4 Al5 2.8609(12) 5_565 ?
Al4 Y1 3.0489(15) 2 ?
Al4 Al2 3.1606(16) 3_665 ?
Al4 Al2 3.1606(16) 18_666 ?
Al4 Y1 3.9649(17) 3_665 ?
Al4 Al5 4.0152(12) 4_665 ?
Al4 Al5 4.0152(12) 13_665 ?
Al4 Al1 4.4005(13) 2 ?
Al4 Al1 4.4005(13) 17_556 ?
Al4 Al2 4.4174(14) 14_565 ?
Al4 Al2 4.4174(14) 5_565 ?
Al4 Al2 4.4378(19) 2 ?
Al4 Al2 4.4378(19) 17_556 ?
Al4 Al4 4.5199(10) 20 ?
Al4 Al4 4.5199(10) 20_556 ?
Al4 Os1 4.5269(11) 17_666 ?
Al4 Os1 4.5269(11) 2_665 ?
Al4 Al1 4.5970(15) 15 ?
Al4 Al1 4.5970(15) 6 ?
Al4 Os1 4.6438(15) 18_566 ?
Al4 Os1 4.6438(15) 3_565 ?
Al4 Al3 4.777(2) 7 ?
Al5 Os1 2.5609(4) 14 ?
Al5 Os1 2.5608(4) 15_655 ?
Al5 Al2 2.7012(11) 13_655 ?
Al5 Al4 2.7494(10) 9_655 ?
Al5 Al4 2.7494(10) 14 ?
Al5 Al4 2.8610(12) 7 ?
Al5 Al4 2.8609(12) 15_655 ?
Al5 Al5 2.9797(16) 2_655 ?
Al5 Al5 2.9797(16) 3_665 ?
Al5 Y1 3.3503(7) 13_655 ?
Al5 Al4 4.0152(12) 8_665 ?
Al5 Al4 4.0152(12) 13_665 ?
Al5 Al5 4.0736(19) 13_655 ?
Al5 Al3 4.2902(9) 9_655 ?
Al5 Al3 4.2904(9) 14 ?
Al5 Al2 4.3827(12) 4_654 ?
Al5 Al2 4.3826(12) 16_556 ?
Al5 Al1 4.4068(13) 13_655 ?
Al5 Al3 4.4914(12) 15_655 ?
Al5 Al3 4.4916(12) 7 ?
Al5 Al5 4.5150(10) 16_556 ?
Al5 Al5 4.5150(10) 16 ?
Al5 Os1 4.6634(12) 13_665 ?
Al5 Al2 4.7116(9) 14_665 ?
Al5 Al2 4.7118(8) 3_665 ?
Al5 Os1 5.0178(11) 2_655 ?
Al5 Os1 5.0179(11) 3 ?
Al6 Al7 0.822(14) . ?
Al6 Al6 1.64(3) 13 ?
Al6 Y2 1.743(15) 16_556 ?
Al6 Al1 2.669(3) 3 ?
Al6 Al1 2.669(3) 2 ?
Al6 Y2 2.772(15) 13 ?
Al6 Al1 2.822(6) 14 ?
Al6 Al1 2.822(6) 13 ?
Al6 Al1 2.822(6) 15 ?
Al6 Al6 2.87(3) 16_556 ?
Al6 Y3 3.080(14) 13 ?
Al6 Y2 3.388(15) 4_554 ?
Al6 Al3 3.525(6) 8 ?
Al6 Al3 3.525(6) 2 ?
Al6 Al3 3.525(6) 7 ?
Al6 Al3 3.526(6) 9 ?
Al6 Al3 3.526(6) 3 ?
Al6 Al7 3.693(14) 4 ?
Al6 Al1 4.314(11) 17_556 ?
Al6 Al1 4.314(11) 16_556 ?
Al6 Al1 4.314(11) 18_556 ?
Al6 Al3 4.456(10) 20 ?
Al6 Al3 4.456(10) 14 ?
Al6 Al3 4.456(10) 19 ?
Al6 Al3 4.456(10) 13 ?
Al6 Al3 4.456(10) 21 ?
Al7 Al6 0.822(14) 13 ?
Al7 Y2 1.949(4) 13 ?
Al7 Y3 2.2575(5) 13 ?
Al7 Y2 2.566(4) 16_556 ?
Al7 Y2 2.566(4) 4_554 ?
Al7 Al1 2.6205(12) 15 ?
Al7 Al1 2.6205(12) 3 ?
Al7 Al1 2.6205(12) 14 ?
Al7 Al1 2.6205(12) 2 ?
Al7 Al1 2.6205(12) 13 ?
Al7 Al6 3.693(14) 16_556 ?
Al7 Al6 3.693(14) 4_554 ?
Al7 Al3 3.9326(9) 20 ?
Al7 Al3 3.9326(9) 8 ?
Al7 Al3 3.9326(9) 14 ?
Al7 Al3 3.9326(9) 2 ?
Al7 Al3 3.9326(9) 19 ?
Al7 Al3 3.9326(9) 7 ?
Al7 Al3 3.9326(9) 13 ?
Al7 Al3 3.9326(9) 21 ?
Al7 Al3 3.9326(9) 9 ?
Al7 Al3 3.9326(9) 15 ?
Al7 Al3 3.9326(9) 3 ?
Al7 Al7 4.5150(10) 4 ?
Al7 Al7 4.5150(10) 4_554 ?
